*637*
*176*
*15MB*

*English*
*Pages [330]*
*Year 2021*

- Author / Uploaded
- Lisa Hall
- Valeriy Ginzburg

*Table of contents : PrefaceContentsContributors1 Polymer Reference Interaction Site Model (PRISM) Theory and Molecular Simulation Studies of Polymer Nanocomposites 1.1 Introduction 1.2 Relevant Past Experimental and Computational Studies on PNCs 1.3 PRISM Theory 1.3.1 Basics 1.3.2 Linking to Molecular Simulation 1.3.3 Open-Source Package pyPRISM 1.4 Past, Present, and Future of PRISM Theory-Based PNC Studies 1.5 Limitations of PRISM Theory 1.6 Conclusions References2 Density Functional Theory-Based Modeling of Polymer Nanocomposites 2.1 Introduction 2.2 DFT Overview 2.3 Applications of DFT to PNCs 2.3.1 Polymers and Nanospheres 2.3.2 Polymers and Nanorods 2.3.3 Polymers and Nanoplatelets 2.4 The SCF-DFT Approach 2.4.1 Nanoparticles in Block Copolymers—Bulk and Films 2.4.2 “Giant Surfactants”—Single-Ligand Nanoparticles 2.4.3 “Hairy Nanoparticles”—Single-Component Assemblies and Mixtures with Polymers 2.5 Summary and Outlook References3 Coarse-Grained Modeling of Polymer Nanocomposites: Field-Theoretic Simulations 3.1 Introduction 3.2 Standard Field Theory—Compressible Diblock with Homopolymer 3.3 Hybrid Particle-Field Theory— Explicit Nanospheres 3.4 Field-Based Nanospheres and Finite-Segment Polymers 3.4.1 Recent Results 3.5 Field-Based Nanorods 3.5.1 Recent Results 3.6 Homopolymer Grafted Nanoparticles 3.7 Complex Grafted Nanoparticles 3.7.1 Recent Applications 3.8 General Interparticle Potentials 3.8.1 Adsorbing Diblock Copolymer 3.9 Theoretically-Informed Langevin Dynamics (TILD) 3.9.1 Recent Applications 3.10 Comparison of the Different Methods 3.11 Challenges and Area for Development References4 Polymer Dynamics in Polymer- Nanoparticle Interface 4.1 Introduction 4.2 Polymer Dynamics Around Spherical or Anisotropic Nanoparticles 4.2.1 Experiments 4.2.2 Simulations 4.3 Polymer Dynamics Around a Flat Surface 4.3.1 Experiments 4.3.2 Simulations 4.4 Conclusions References5 The Interfacial Layers Around Nanoparticle and Its Impact on Structural Relaxation and Glass Transition in Model Polymer Nanocomposites 5.1 Introduction 5.2 Modeling and Simulations 5.3 Interfacial Zone Around Nanoparticles in Nanocomposites and Near Substrate in Thin Polymer Films 5.3.1 Qualitative Description of the Influence of Interfacial Interactions on Mobility Near Interfaces 5.3.2 Mobility Gradient Near Interfaces 5.3.3 Density Gradient Near Interfaces and Its Scale ξρ 5.3.4 Comparison Between Interfacial Mobility and Density Scales 5.4 Effects of Bound Interfacial Layer Around NP and Near Substrate on Polymer Relaxation and Overall Tg 5.4.1 Influence of Interface Interaction on Polymer Relaxation 5.4.2 Effect of Interfacial Interaction Strength on Tg Estimates from Thermodynamic and Dynamic Methods 5.5 Conclusions References6 Multiscale Modeling Examples: New Polyelectrolyte Nanocomposite Membranes for Perspective Fuel Cells and Flow Batteries 6.1 Introduction 6.2 Multiscale Modeling of Polyelectrolyte Membranes and Their Transport Properties 6.3 Confined Film Model of a Nanocomposite Membrane 6.4 Atomistic Simulations of Nafion/Graphene Oxide Membranes 6.5 Modeling of Doped Non-humidified Membranes 6.6 Mesoscopic Simulations and Simulated Example: SPEEK Membrane 6.7 Summary References7 Explorations into the Mechanics of Hairy Nanoparticle Assemblies with Molecular Dynamics 7.1 Introduction 7.2 Energy Renormalization (ER) Approach to Coarse-Graining 7.2.1 ER Methodology 7.2.2 Validation of ER Approach 7.3 Modeling of Hairy Nanoparticle Assemblies 7.3.1 System Setup 7.3.2 Simulation Protocols 7.3.3 Mechanical Property Characterization 7.3.4 Evaluating Polymer Conformational Behavior 7.4 Mesoscale Modeling of aHNPs 7.4.1 PMF-Based Approach 7.4.2 Functional Form of Effective Interactions 7.5 Conclusion References8 Predicting Mechanical Properties Using Continuum Mechanics-Based Approach: Micro-mechanics and Finite Element Analysis 8.1 Introduction 8.2 Discrete-Medium Modeling Tools 8.3 Continuous-Medium Modeling Tools 8.3.1 Analytical Modeling: Micro-mechanics 8.3.2 Comparison of the Different Analytical Micro-mechanical Models 8.3.3 Laminate Plate Theory 8.4 Computational Modeling: Finite Element Analysis (FEA) 8.4.1 Computational Micro-mechanics 8.5 Multiscale Modeling Concepts 8.5.1 Bottom-Up Approach: Equivalent Continuum 8.5.2 Top-Down Approach 8.5.3 Concurrent Modeling 8.6 Summary References9 Modeling the Thermal Conductivity of Polymer-Inorganic Nanocomposites 9.1 Introduction 9.2 Thermal Conductivities of Typical Polymers and Fillers 9.2.1 Polymers 9.2.2 Fillers 9.3 Analytical Theories and Micromechanical Models 9.3.1 The Parallel and Series Models as the Upper and Lower Limit Estimates 9.3.2 EMA for Spherical Fillers 9.3.3 Non-spherical Fillers 9.3.4 Bruggeman Model 9.3.5 Combined Approaches 9.4 Computer Simulations 9.4.1 Finite Element Modeling 9.4.2 Interfacial Thermal Resistance Modeling 9.4.3 Multiscale Modeling 9.5 Summary and Outlook References10 Predicting the Optical and Electrical Properties of Polymer Nanocomposites 10.1 Introduction 10.2 Calculation of Optical Properties 10.2.1 Mie Theory Applied to Polymer Nanocomposites 10.2.2 The Discrete Dipole Approximation (DDA) 10.2.3 Finite-Difference Time-Domain (FDTD) Method 10.3 Calculation of Electrical Properties 10.3.1 Resistor Network Models 10.3.2 The Poisson-Nernst-Planck (PNP) Formalism 10.4 Summary and Outlook References11 Data-Driven Multiscale Science for Tire Compounding: Methods and Future Directions 11.1 Introduction 11.1.1 Early Laboratory Compound Design Concepts 11.1.2 Chapter Scope 11.2 Methods Framework 11.2.1 Simple Representations of Filled Soft Composites 11.2.2 Filler Microstructure Statistical Characterization and Stochastic Reconstruction 11.2.3 Nanocomposite Properties and Statistical Study of the Representative Volume Element 11.2.4 Summary 11.3 Future Directions 11.3.1 Material Informatics and Cheminformatics 11.3.2 Machine Learning 11.3.3 Summary ReferencesIndex*

Springer Series in Materials Science 310

Valeriy V. Ginzburg Lisa M. Hall Editors

Theory and Modeling of Polymer Nanocomposites

Springer Series in Materials Science Volume 310

Series Editors Robert Hull, Center for Materials, Devices, and Integrated Systems, Rensselaer Polytechnic Institute, Troy, NY, USA Chennupati Jagadish, Research School of Physical, Australian National University, Canberra, ACT, Australia Yoshiyuki Kawazoe, Center for Computational Materials, Tohoku University, Sendai, Japan Jamie Kruzic, School of Mechanical & Manufacturing Engineering, UNSW Sydney, Sydney, NSW, Australia Richard M. Osgood, Department of Electrical Engineering, Columbia University, New York, USA Jürgen Parisi, Universität Oldenburg, Oldenburg, Germany Udo W. Pohl, Institute of Solid State Physics, Technical University of Berlin, Berlin, Germany Tae-Yeon Seong, Department of Materials Science & Engineering, Korea University, Seoul, Korea (Republic of) Shin-ichi Uchida, Electronics and Manufacturing, National Institute of Advanced Industrial Science and Technology, Tsukuba, Ibaraki, Japan Zhiming M. Wang, Institute of Fundamental and Frontier Sciences - Electronic, University of Electronic Science and Technology of China, Chengdu, China

The Springer Series in Materials Science covers the complete spectrum of materials research and technology, including fundamental principles, physical properties, materials theory and design. Recognizing the increasing importance of materials science in future device technologies, the book titles in this series reflect the state-of-the-art in understanding and controlling the structure and properties of all important classes of materials.

More information about this series at http://www.springer.com/series/856

Valeriy V. Ginzburg Lisa M. Hall •

Editors

Theory and Modeling of Polymer Nanocomposites

123

Editors Valeriy V. Ginzburg Dow Chemical Company (United States) Midland, MI, USA

Lisa M. Hall The Ohio State University Columbus, OH, USA

ISSN 0933-033X ISSN 2196-2812 (electronic) Springer Series in Materials Science ISBN 978-3-030-60442-4 ISBN 978-3-030-60443-1 (eBook) https://doi.org/10.1007/978-3-030-60443-1 © Springer Nature Switzerland AG 2021 This work is subject to copyright. All rights are reserved by the Publisher, whether the whole or part of the material is concerned, speciﬁcally the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microﬁlms or in any other physical way, and transmission or information storage and retrieval, electronic adaptation, computer software, or by similar or dissimilar methodology now known or hereafter developed. The use of general descriptive names, registered names, trademarks, service marks, etc. in this publication does not imply, even in the absence of a speciﬁc statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. The publisher, the authors and the editors are safe to assume that the advice and information in this book are believed to be true and accurate at the date of publication. Neither the publisher nor the authors or the editors give a warranty, expressed or implied, with respect to the material contained herein or for any errors or omissions that may have been made. The publisher remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations. This Springer imprint is published by the registered company Springer Nature Switzerland AG The registered company address is: Gewerbestrasse 11, 6330 Cham, Switzerland

Preface

Polymer nanocomposites (PNCs) are multiphase, multicomponent materials in which one or more components come in the form of particulates with the size less than 100 nm in at least one spatial dimension. The particulates (dispersed phase or ﬁllers) can be metal, ceramic, carbon, or even polymer nanocrystals; they could have spherical, cylindrical, platelet, or other shapes; they can possess various chemical, mechanical, optical, or electrical properties. The polymer matrix, in turn, can be thermoplastic or thermoset; the polymer can be partially crystalline, rubbery, or glassy. One example of a PNC is cross-linked styrene-butadiene rubber with nanoscopic silica or carbon black ﬁller particles, along with other additives, included in varying amounts to create car tires with good traction and acceptable rolling resistance and wear properties. Another example is a typical paint, where sub-100-nm pigments can be added to a liquid formulation, which then undergoes the processes of drying and ﬁlm formation to create a nanocomposite coating seen on the walls of our houses and on the bodies of our vehicles. In these and other cases where PNCs have already found signiﬁcant use, including in consumer products such as shoe soles, packaging, and membranes, even minor adjustments to the formulation to improve the material properties can have signiﬁcant practical implications. It is thus important to develop the Formulation!Structure!Property!Performance roadmap, in which both experimental and theoretical/modeling studies are utilized. Nanocomposite modeling has made signiﬁcant progress in recent decades, and many excellent reviews highlighting various speciﬁc topics have been published in recent years. Yet, with some notable exceptions (such as “Modeling and Prediction of Polymer Nanocomposite Properties,” edited by Vikas Mittal, Wiley, 2012), there have been very few books surveying multiple theoretical methods and analyzing multiple topics under the same cover. Indeed, in order to successfully develop, say, a nanocomposite gas separation membrane, one needs to consider the question of the nanoparticle design (length and density of grafted ligands), their dispersion in the polymer matrix, the processability of the material, and lastly, the gas permeability and selectivity. This design requires multiscale, multiphysics, interdisciplinary modeling that does not come naturally even to the best researchers.

v

vi

Preface

In putting this book together, we hope to stimulate such efforts and highlight some successful examples. The structure of the book can be described as follows. The ﬁrst three chapters describe molecular or mesoscale approaches to predict the structure, dispersion, and nanoscale morphologies of nanocomposite materials, given the nanoparticle shape and loading and, in some cases, the length and density of grafted ligands. The next two chapters discuss the dynamics of nanocomposites, concentrating speciﬁcally on the behavior of polymer chains at and near the particle surfaces. The remaining six chapters deal with the prediction of mechanical, transport, electrical, and optical properties of nanocomposites, and the implications for product design. We now proceed to describe each chapter more speciﬁcally. In Chap. 1, Arthi Jayaraman discusses the use of the polymer reference interaction site model (PRISM) theory, which is generally applied at the coarse-grained level and includes monomer-scale packing effects along with overall chain and nanoparticle statistical behavior. PRISM requires information about the polymer conformations as an input, and this can be either assumed or calculated selfconsistently from molecular simulations as is briefly discussed. A recently developed open-source code pyPRISM is described that allows for easy use of these methods. In Chap. 2, Valeriy V. Ginzburg describes the application of density functional theory (DFT) to PNCs, which is also generally applied at the coarse-grained level. This approach, based on classical statistical mechanical functionals that calculate the free energy from the density proﬁle, has been particularly useful for describing monomer and nanoparticle packing in conﬁnement or near surfaces. The chapter ﬁrst details several examples of standard DFT methods, including calculations of the polymer-mediated interactions between polymer-grafted spherical, rod, and plate-shaped particles. The combination of DFT with self-consistent ﬁeld theory (SCFT) is then discussed. As is made clear by several examples, this is especially attractive to describe nanoparticle behavior in systems with long-range microphase separation such as in block copolymers (where SCFT has found widespread application for systems without nanoparticles). In Chap. 3, Robert A. Riggleman and co-workers review their newly developed coarse-grained method of simulating nanocomposite morphologies, polymer nanocomposite ﬁeld theory (PNC-FT). Based on the state-of-the-art polymer ﬁeld theory, PNC-FT incorporates the nanoparticles via the excluded volume interactions (“cavity functions”) and enables the evaluation of the free energy of various nanoscale structures. The authors discuss the application of their modeling approach to predict the distribution of “hairy” nanospheres in drying polymer ﬁlms; calculate the effective interactions between nanoparticles with multicomponent ligands; and evaluate the interaction between nanorods in a cylinder-forming block copolymer ﬁlm. Similar to SCFT-DFT, PNC-FT is now widely used to predict nanocomposite equilibrium structures and morphologies. In Chap. 4, Argyrios V. Karatrantos and Nigel Clarke describe the dynamics of polymers near the nanoﬁller surfaces, and speciﬁcally the impact of the nanoparticle size and the particle–polymer interaction on the relaxation time, the self-diffusion

Preface

vii

coefﬁcient, and the glass transition temperature. They utilize coarse-grained molecular dynamics (CG-MD) to show that the mobility of the polymer chains near a strongly attracting particle surface is severely depressed compared to the bulk polymer; near a weakly attracting or repulsive surface, on the other hand, the mobility seems to be slightly enhanced. Overall, CG-MD provides a very useful insight into the interfacial dynamics of PNCs. In Chap. 5, Jack F. Douglas, Francis W. Starr, and co-workers attack a very similar problem using a combination of CG-MD and analytical scaling theories. They speciﬁcally investigate the relationship between the glass transition temperature shift in nanocomposite materials and the density changes induced by the addition of nanoparticles. The authors discuss the relationship between the mobility gradient scale and the density gradient scale, and also comment on the similarities and differences between nanocomposites and thin ﬁlms in terms of their glass transition and glassy dynamics. In Chap. 6, Alexey V. Lyulin and co-workers describe the use of multiscale modeling to predict the transport properties of polyelectrolyte membranes (PEMs). Such membranes are used in fuel cells and batteries. The authors discuss how the addition of nanoparticles (such as graphene oxide or silicon dioxide) can influence the proton conductivity through the membrane by impacting the phase separation between the water-rich and polymer-rich domains, as well as the diffusion coefﬁcient and mobility of water near the particle surfaces. Several relevant simulation techniques, from ab initio simulations of electronic structure to classical atomistic molecular dynamics to coarse-grained dynamic density functional theory (DDFT), are employed in this multiscale modeling study. In Chap. 7, Nitin K. Hansoge and Sinan Keten describe the use of multiscale modeling to predict mechanical properties of matrix-free (or “one-component nanocomposites”) assemblies of “hairy nanoparticles.” They start by discussing the “energy renormalization” procedure to go from atomistic to coarse-grained molecular dynamics. Using CG-MD, they calculate the morphology of the nanocomposite (i.e., the crystalline structure of the rigid nanoparticle cores separated by the soft ligands). They then used CG-MD to calculate mechanical properties (Young’s modulus and toughness) and generate Ashby plots and Pareto fronts to come up with the optimal designs to balance the two properties. Finally, an approach is described whereby the conformational degrees of freedom for the ligands can be integrated out, allowing for computationally inexpensive mesoscale models involving only the particle cores interacting via effective pairwise potential of mean force (PMF). In Chap. 8, Pavan K. Valavala and Gregory M. Odegard review various approaches to predict mechanical properties of composites and nanocomposites. They start by differentiating between discrete-medium (like MD) and continuous-medium models, and provide an extensive overview of the latter. Within the continuous-medium framework, the authors distinguish between analytical micromechanical theories and computational ﬁnite element analysis (FEA), both of which are based on linear elasticity and enable the prediction of linear elastic moduli (Young’s modulus and shear modulus for the case of isotropic

viii

Preface

materials). Multiscale modeling is also discussed for those cases where a number of disparate length scales is involved. In Chap. 9, Valeriy V. Ginzburg and Jian Yang describe theoretical and modeling approaches to the prediction of thermal conductivity (critically important in many applications, including electronics and transportation). Similar to the previous chapter, the authors discuss the use of analytical micromechanical models and FEA. The role of interfacial thermal resistance—often leading to thermal conductivity being signiﬁcantly lower than expected—is also reviewed. In Chap. 10, Michael J. A. Hore discusses ways to predict optical and electrical properties of PNCs. Calculating those properties requires solving Maxwell’s equations in complex media, at either very high frequencies (optical) or low frequencies (electrical). Optical properties of interest include scattering and absorption cross section, UV–Vis spectra, and plasmonic resonances. As the author shows, the calculation techniques here range from analytical theories (Rayleigh and Mie scattering) to more computationally expensive ﬁnite difference, time domain (FDTD) simulations. For the case of electrical properties (static electrical conductivity), the author emphasizes the importance of percolation (inﬁnite clusters of conducting bonds) and simple methods to predict it (resistor network models). The dependence of electrical conductivity on the conducting ﬁller loading, shape, and alignment is also discussed. Finally, in Chap. 11, Craig Burkhart, L. Catherine Brinson, and co-workers describe the application of both ﬁrst-principles and data-driven approaches to the design of nanocomposite materials for automotive tires. The material considered is carbon-black (CB)-ﬁlled styrene-butadiene rubber (SBR). The authors discuss the importance of experimental characterization (microscopy) to precisely determine the morphology of the CB network in the SBR matrix; once this morphology is determined, it can serve as input into FEA simulations analyzing the viscoelastic behavior of the material. The predicted linear viscoelastic (LVE) response can be then compared to the “optimal” response known to the industry. Given the complexity of the process, one also looks to simplify the search for best compositions by employing machine learning (ML) tools, and the authors highlight their roadmap in this quest. In summary, PNC material designers seeking to take advantage of many potential options for polymer and nanoparticles, including their chemical types and amounts, length/size, and architecture (e.g., whether and to what extent chains are cross-linked or grafted to the nanoparticle surface), can turn to modeling approaches to understand how PNC component properties lead to desirable overall material behavior. While the chapters of this book, in order, are meant to present a coherent picture of the range of current PNC modeling techniques from small to large scales and from structure to dynamics to speciﬁc material properties, each chapter is written to be independent and readable by itself. We hope the reader will take away an understanding of which modeling methods can be effective and how

Preface

ix

they can be used, depending on the system and properties of interest, to closely connect synthetically controllable polymer and particle variables to the resulting overall PNC structure and/or dynamics, and allow for rational design of future materials. Midland, USA Columbus, USA

Valeriy V. Ginzburg Lisa M. Hall

Acknowledgments We thank the staff at Springer Nature, and specifically Sara Kate Heukerott, Zachary Evenson, Viradasarani Natarajan, Priyadharshini Subramani, and Adelheid Duhm for their help and encouragement in making this book possible. We would like to thank our families for their patience and support.

Contents

1

2

Polymer Reference Interaction Site Model (PRISM) Theory and Molecular Simulation Studies of Polymer Nanocomposites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Arthi Jayaraman 1.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Relevant Past Experimental and Computational Studies on PNCs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 PRISM Theory . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.1 Basics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3.2 Linking to Molecular Simulation . . . . . . . . . . . 1.3.3 Open-Source Package pyPRISM . . . . . . . . . . . 1.4 Past, Present, and Future of PRISM Theory-Based PNC Studies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 Limitations of PRISM Theory . . . . . . . . . . . . . . . . . . . 1.6 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

......

1

......

1

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

. . . . .

2 5 5 9 12

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

13 17 18 18

....

23

. . . . . . .

. . . . . . .

23 25 26 26 28 29 33

.... ....

35 36

Density Functional Theory-Based Modeling of Polymer Nanocomposites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Valeriy V. Ginzburg 2.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 DFT Overview . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Applications of DFT to PNCs . . . . . . . . . . . . . . . . . . . . . 2.3.1 Polymers and Nanospheres . . . . . . . . . . . . . . . . . 2.3.2 Polymers and Nanorods . . . . . . . . . . . . . . . . . . . 2.3.3 Polymers and Nanoplatelets . . . . . . . . . . . . . . . . 2.4 The SCF-DFT Approach . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.1 Nanoparticles in Block Copolymers—Bulk and Films . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.2 “Giant Surfactants”—Single-Ligand Nanoparticles

. . . . . . .

. . . . . . .

xi

xii

Contents

“Hairy Nanoparticles”—Single-Component Assemblies and Mixtures with Polymers . . . . . . . . . . . 2.5 Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.3

3

4

Coarse-Grained Modeling of Polymer Nanocomposites: Field-Theoretic Simulations . . . . . . . . . . . . . . . . . . . . . . . . . Jason P. Koski, Huikuan Chao, Christian Tabedzki, and Robert A. Riggleman 3.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Standard Field Theory—Compressible Diblock with Homopolymer . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Hybrid Particle-Field Theory— Explicit Nanospheres . . 3.4 Field-Based Nanospheres and Finite-Segment Polymers 3.4.1 Recent Results . . . . . . . . . . . . . . . . . . . . . . . . 3.5 Field-Based Nanorods . . . . . . . . . . . . . . . . . . . . . . . . . 3.5.1 Recent Results . . . . . . . . . . . . . . . . . . . . . . . . 3.6 Homopolymer Grafted Nanoparticles . . . . . . . . . . . . . . 3.7 Complex Grafted Nanoparticles . . . . . . . . . . . . . . . . . . 3.7.1 Recent Applications . . . . . . . . . . . . . . . . . . . . 3.8 General Interparticle Potentials . . . . . . . . . . . . . . . . . . 3.8.1 Adsorbing Diblock Copolymer . . . . . . . . . . . . 3.9 Theoretically-Informed Langevin Dynamics (TILD) . . . 3.9.1 Recent Applications . . . . . . . . . . . . . . . . . . . . 3.10 Comparison of the Different Methods . . . . . . . . . . . . . 3.11 Challenges and Area for Development . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Polymer Dynamics in Polymer-Nanoparticle Interface . . Argyrios V. Karatrantos and Nigel Clarke 4.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Polymer Dynamics Around Spherical or Anisotropic Nanoparticles . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . 4.2.2 Simulations . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Polymer Dynamics Around a Flat Surface . . . . . . . . 4.3.1 Experiments . . . . . . . . . . . . . . . . . . . . . . . . 4.3.2 Simulations . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

38 39 40

......

45

......

45

. . . . . . . . . . . . . . . .

. . . . . . . . . . . . . . . .

47 51 53 56 56 58 58 61 63 64 66 69 71 73 75 77

........

81

........

81

. . . . . . . .

82 82 86 89 89 90 94 94

. . . . . . . .

. . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . .

. . . . . . . . . . . . . . . .

. . . . . . . .

. . . . . . . .

Contents

5

6

xiii

The Interfacial Layers Around Nanoparticle and Its Impact on Structural Relaxation and Glass Transition in Model Polymer Nanocomposites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Wengang Zhang, Hamed Emamy, Fernando Vargas-Lara, Beatriz A. Pazmiño Betancourt, Dong Meng, Francis W. Starr, and Jack F. Douglas 5.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Modeling and Simulations . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3 Interfacial Zone Around Nanoparticles in Nanocomposites and Near Substrate in Thin Polymer Films . . . . . . . . . . . . . . 5.3.1 Qualitative Description of the Inﬂuence of Interfacial Interactions on Mobility Near Interfaces . . . . . . . . . 5.3.2 Mobility Gradient Near Interfaces . . . . . . . . . . . . . . 5.3.3 Density Gradient Near Interfaces and Its Scale nq . . 5.3.4 Comparison Between Interfacial Mobility and Density Scales . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Effects of Bound Interfacial Layer Around NP and Near Substrate on Polymer Relaxation and Overall Tg . . . . . . . . . . 5.4.1 Inﬂuence of Interface Interaction on Polymer Relaxation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Effect of Interfacial Interaction Strength on Tg Estimates from Thermodynamic and Dynamic Methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Conclusions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Multiscale Modeling Examples: New Polyelectrolyte Nanocomposite Membranes for Perspective Fuel Cells and Flow Batteries . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Soumyadipta Sengupta, Alexey V. Lyulin, Georgios Kritikos, Konstantinos Karatasos, Arun Venkatnathan, Rakesh Pant, and Pavel V. Komarov 6.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Multiscale Modeling of Polyelectrolyte Membranes and Their Transport Properties . . . . . . . . . . . . . . . . . . . . . 6.3 Conﬁned Film Model of a Nanocomposite Membrane . . . 6.4 Atomistic Simulations of Naﬁon/Graphene Oxide Membranes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Modeling of Doped Non-humidiﬁed Membranes . . . . . . . 6.6 Mesoscopic Simulations and Simulated Example: SPEEK Membrane . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.7 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . 101

. . 102 . . 104 . . 106 . . 106 . . 108 . . 114 . . 117 . . 118 . . 119

. . 122 . . 125 . . 127

. . . . 133

. . . . 134 . . . . 140 . . . . 142 . . . . 149 . . . . 156 . . . . 160 . . . . 168 . . . . 169

xiv

7

8

9

Contents

Explorations into the Mechanics of Hairy Nanoparticle Assemblies with Molecular Dynamics . . . . . . . . . . . . . . . . . . . . Nitin K. Hansoge and Sinan Keten 7.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Energy Renormalization (ER) Approach to Coarse-Graining 7.2.1 ER Methodology . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.2 Validation of ER Approach . . . . . . . . . . . . . . . . . . 7.3 Modeling of Hairy Nanoparticle Assemblies . . . . . . . . . . . . 7.3.1 System Setup . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.2 Simulation Protocols . . . . . . . . . . . . . . . . . . . . . . . 7.3.3 Mechanical Property Characterization . . . . . . . . . . 7.3.4 Evaluating Polymer Conformational Behavior . . . . 7.4 Mesoscale Modeling of aHNPs . . . . . . . . . . . . . . . . . . . . . 7.4.1 PMF-Based Approach . . . . . . . . . . . . . . . . . . . . . . 7.4.2 Functional Form of Effective Interactions . . . . . . . . 7.5 Conclusion . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Predicting Mechanical Properties Using Continuum Mechanics-Based Approach: Micro-mechanics and Finite Element Analysis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Pavan K. Valavala and Gregory M. Odegard 8.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Discrete-Medium Modeling Tools . . . . . . . . . . . . . . . . . 8.3 Continuous-Medium Modeling Tools . . . . . . . . . . . . . . . 8.3.1 Analytical Modeling: Micro-mechanics . . . . . . . 8.3.2 Comparison of the Different Analytical Micro-mechanical Models . . . . . . . . . . . . . . . . . 8.3.3 Laminate Plate Theory . . . . . . . . . . . . . . . . . . . 8.4 Computational Modeling: Finite Element Analysis (FEA) 8.4.1 Computational Micro-mechanics . . . . . . . . . . . . 8.5 Multiscale Modeling Concepts . . . . . . . . . . . . . . . . . . . . 8.5.1 Bottom-Up Approach: Equivalent Continuum . . 8.5.2 Top-Down Approach . . . . . . . . . . . . . . . . . . . . 8.5.3 Concurrent Modeling . . . . . . . . . . . . . . . . . . . . 8.6 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . 179 . . . . . . . . . . . . . .

. . . . . . . . . . . . . .

. . . . . . . . . . . . . .

180 181 181 184 185 186 187 188 191 193 194 195 197 198

. . . . . 203 . . . .

. . . .

. . . .

. . . .

. . . .

203 204 205 206

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

211 212 215 217 219 220 228 229 230 230

Modeling the Thermal Conductivity of Polymer-Inorganic Nanocomposites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235 Valeriy V. Ginzburg and Jian Yang 9.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 235

Contents

9.2

Thermal Conductivities of Typical Polymers and Fillers 9.2.1 Polymers . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2.2 Fillers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 Analytical Theories and Micromechanical Models . . . . 9.3.1 The Parallel and Series Models as the Upper and Lower Limit Estimates . . . . . . . . . . . . . . . 9.3.2 EMA for Spherical Fillers . . . . . . . . . . . . . . . . 9.3.3 Non-spherical Fillers . . . . . . . . . . . . . . . . . . . . 9.3.4 Bruggeman Model . . . . . . . . . . . . . . . . . . . . . 9.3.5 Combined Approaches . . . . . . . . . . . . . . . . . . 9.4 Computer Simulations . . . . . . . . . . . . . . . . . . . . . . . . . 9.4.1 Finite Element Modeling . . . . . . . . . . . . . . . . 9.4.2 Interfacial Thermal Resistance Modeling . . . . . 9.4.3 Multiscale Modeling . . . . . . . . . . . . . . . . . . . . 9.5 Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

xv

. . . .

. . . .

. . . .

. . . .

. . . .

. . . .

237 237 239 240

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

. . . . . . . . . . .

240 241 243 244 245 245 246 251 252 254 255

10 Predicting the Optical and Electrical Properties of Polymer Nanocomposites . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Michael J. A. Hore 10.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.2 Calculation of Optical Properties . . . . . . . . . . . . . . . . . . . 10.2.1 Mie Theory Applied to Polymer Nanocomposites . 10.2.2 The Discrete Dipole Approximation (DDA) . . . . . 10.2.3 Finite-Difference Time-Domain (FDTD) Method . 10.3 Calculation of Electrical Properties . . . . . . . . . . . . . . . . . 10.3.1 Resistor Network Models . . . . . . . . . . . . . . . . . . 10.3.2 The Poisson-Nernst-Planck (PNP) Formalism . . . . 10.4 Summary and Outlook . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . 259 . . . . . . . . . .

. . . . . . . . . .

11 Data-Driven Multiscale Science for Tire Compounding: Methods and Future Directions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Hongyi Xu, Richard J. Sheridan, L. Catherine Brinson, Wei Chen, Bing Jiang, George Papakonstantopoulos, Patrycja Polinska, and Craig Burkhart 11.1 Introduction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.1.1 Early Laboratory Compound Design Concepts . . . . . 11.1.2 Chapter Scope . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 Methods Framework . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2.1 Simple Representations of Filled Soft Composites . . 11.2.2 Filler Microstructure Statistical Characterization and Stochastic Reconstruction . . . . . . . . . . . . . . . . .

. . . . . . . . . .

. . . . . . . . . .

259 260 261 263 269 273 273 276 278 279

. . 281

. . . . .

. . . . .

282 283 285 285 287

. . 289

xvi

Contents

11.2.3 Nanocomposite Properties and Statistical Study of the Representative Volume Element . . . . . . 11.2.4 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3 Future Directions . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.3.1 Material Informatics and Cheminformatics . . . . 11.3.2 Machine Learning . . . . . . . . . . . . . . . . . . . . . 11.3.3 Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . References . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

. . . . . . .

300 304 306 306 308 309 309

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313

Contributors

Beatriz A. Pazmiño Betancourt Materials Science and Engineering Division, National Institute of Standards and Technology, Maryland, USA; Department of Physics, Wesleyan University, Connecticut, USA Craig Burkhart Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, Akron, OH, USA L. Catherine Brinson Department of Materials Science and Engineering, Duke University, Durham, NC, USA Huikuan Chao Core Research and Development, The Dow Chemical Company, Midland, USA Wei Chen Department of Mechanical Engineering, Northwestern University, Evanston, IL, USA Nigel Clarke Department of Physics and Astronomy, University of Shefﬁeld, Shefﬁeld, UK Jack F. Douglas Materials Science and Engineering Division, National Institute of Standards and Technology, Maryland, USA Hamed Emamy Department of Physics, Wesleyan University, Connecticut, USA; Department of Chemical Engineering, Columbia University, New York, NY, USA Valeriy V. Ginzburg Core Research and Development, The Dow Chemical Company, Midland, MI, USA Nitin K. Hansoge Department of Mechanical Engineering, Center for Hierarchical Materials Design, Northwestern University, Evanston, IL, USA Michael J. A. Hore Department of Macromolecular Science and Engineering, Case Western Reserve University, Cleveland, OH, USA

xvii

xviii

Contributors

Arthi Jayaraman Department of Chemical and Biomolecular Engineering, Colburn Laboratory, Department of Materials Science and Engineering, University of Delaware, Newark, DE, USA Bing Jiang Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, Akron, OH, USA Konstantinos Karatasos Department of Chemical Engineering, Aristotle University of Thessaloniki, Thessaloniki, Greece Argyrios V. Karatrantos Materials Research and Technology, Luxembourg Institute of Science and Technology, Esch-sur-Alzette, Luxembourg Sinan Keten Department of Mechanical Engineering, Center for Hierarchical Materials Design, Department of Civil & Environmental Engineering, Northwestern University, Evanston, IL, USA Pavel V. Komarov A.N. Nesmeyanov Institute of Organoelement Compounds of Russian Academy of Sciences, Moscow, Russia; Tver State University, Tver, Russia Jason P. Koski Sandia National Laboratories, Albuquerque, NM, USA Georgios Kritikos Department of Chemical Engineering, Aristotle University of Thessaloniki, Thessaloniki, Greece Alexey V. Lyulin Group Theory of Polymers and Soft Matter and Center for Computational Energy Research, Department of Applied Physics, Technische Universiteit Eindhoven, Eindhoven, The Netherlands Dong Meng Department of Chemical Engineering, Columbia University, New York, NY, USA Gregory M. Odegard Mechanical Engineering—Engineering Michigan Technological University, Houghton, India

Mechanics,

Rakesh Pant Department of Chemistry and Center for Energy Science, Indian Institute of Science Education and Research, Pashan, Pune, Maharashtra, India George Papakonstantopoulos Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, Akron, OH, USA Patrycja Polinska Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, Colmar-Berg, Luxembourg Robert A. Riggleman Chemical and Biomolecular Engineering, University of Pennsylvania, Philadelphia, USA

Contributors

xix

Soumyadipta Sengupta Group Theory of Polymers and Soft Matter and Center for Computational Energy Research, Department of Applied Physics, Technische Universiteit Eindhoven, Eindhoven, The Netherlands Richard J. Sheridan Department of Materials Science and Engineering, Duke University, Durham, NC, USA Francis W. Starr Department of Physics, Wesleyan University, Connecticut, USA Christian Tabedzki Chemical and Biomolecular Engineering, University of Pennsylvania, Philadelphia, USA Pavan K. Valavala Research and Development, Packaging and Specialty Plastics, Dow Inc., Midland, USA Fernando Vargas-Lara Materials Science and Engineering Division, National Institute of Standards and Technology, Maryland, USA; Department of Physics, Wesleyan University, Connecticut, USA Arun Venkatnathan Department of Chemistry and Center for Energy Science, Indian Institute of Science Education and Research, Pashan, Pune, Maharashtra, India Hongyi Xu Department of Mechanical Engineering, The University of Connecticut, Storrs, CT, USA Jian Yang PE Product Research, The Dow Chemical Company, Lake Jackson, TX, USA Wengang Zhang Materials Science and Engineering Division, National Institute of Standards and Technology, Maryland, USA; Department of Physics, Wesleyan University, Connecticut, USA

Chapter 1

Polymer Reference Interaction Site Model (PRISM) Theory and Molecular Simulation Studies of Polymer Nanocomposites Arthi Jayaraman Abstract This chapter is focused on Polymer Reference Interaction Site Model (PRISM) theory and its use along with molecular simulation techniques for studying polymer nanocomposites (PNCs). In the first section of this chapter, we summarize key experimental and computational studies on PNCs from the literature to show the reader the types of fundamental questions that these studies have tackled. These are the types of questions that one could also use PRISM theory to answer. Then, we describe the basics of PRISM theory with relevant equations and show how PRISM theory is linked to molecular simulations to obtain meaningful results pertaining to PNC structure and thermodynamics. We also bring to the readers’ attention the open-source package, pyPRISM, developed for both expert and novice computational researchers to easily incorporate PRISM theory into their PNC studies. We then discuss briefly past, present, and potential new directions of PNC studies using PRISM theory and conclude the chapter highlighting some of the limitations of PRISM theory.

1.1 Introduction Polymer nanocomposites (PNCs) are a specific class of macromolecular soft materials that have garnered significant attention in the past two to three decades from researchers around the world. This is evident from the many review articles and perspectives on this topic [1–17]. As the name suggests, a polymer nanocomposite is a mixture of the polymer (matrix) as the majority component and nanoscale additives (fillers) as the minority component. The chemical and physical nature of the fillers and matrix and their relative composition in the PNC is selected based on the eventual A. Jayaraman (B) Department of Chemical and Biomolecular Engineering, Colburn Laboratory, University of Delaware, 150 Academy Street, Newark, DE 19716, USA e-mail: [email protected] Department of Materials Science and Engineering, University of Delaware, Newark, DE 19716, USA © Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1_1

1

2

A. Jayaraman

application of the PNC. There is a broad range of applications where PNCs have been used, such as in automobile parts (e.g., car bumpers, tires) [18], aerospace industry (e.g., components of thermal resistance aircraft body parts) [19], in separations (e.g., membranes for gas transport and absorption) [20], in electronics (e.g., organic/hybrid solar cells) [21], and in biomaterials (e.g., tissue mimics, drug delivery vehicles) [22]. To achieve the desired function or macroscopic property of the PNC needed for these applications, one has to select the components of the PNCs based on their individual properties (e.g., biocompatible matrix and filler when used in biomedical applications, electron donating/accepting matrix and filler in organic/hybrid electronics) as well as on how they interact and spatially organize within the PNC (i.e., structure/morphology). Additionally, the ease during processing (e.g., response to shear, temperature) of the PNC, a critical feature for large-scale manufacturing, is another variable to consider during the material selection process. The non-trivial relationship between the structure/morphology, dynamics, and thermodynamics for a selected filler and matrix at a specific composition within PNCs has motivated exciting research aimed at unraveling the complex interplay between PNC design and its macroscopic behavior. In particular, computational tools (e.g., coarse-grained models, theory, and simulation) have become valuable tools in this quest to both predict PNC behavior for a variety of PNC design parameters as well as to explain less understood experimental observations in PNCs. This chapter specifically focuses on how Polymer Reference Interaction Site Model (PRISM) theory and molecular simulation methods have been used to tackle questions about PNC structure and thermodynamics. To help the reader appreciate the value of these tools, we first review in Sect. 1.2 relevant past experimental, computational, and theoretical work on PNC structure and thermodynamics to describe the types of fundamental questions that researchers working with PNCs tackle and that PRISM theory can be used for. Then, in Sect. 1.3, the details of PRISM theory, the open-source package for readers wishing to use this method, and complementary molecular simulation methods used along with PRISM theory are discussed. In Sects. 1.4 and 1.5, the past, present, and potential new directions for PRISM theory-based studies of PNCs are described along with the key limitations of PRISM theory.

1.2 Relevant Past Experimental and Computational Studies on PNCs Past studies focused on PNCs (see references in review articles [1–13, 15, 17]) have shown that any experimental or computational tool that is used to study PNC structure and morphology should be able to tackle/probe all relevant length scales including the size of the monomer, the polymer chain, the nanoscale (bare or unmodified) particle or filler, and if phase separated, size of the domains of fillers and matrix chains. As the nanoscale dimension of the fillers decreases (e.g., curvature of spherical nanoparticle

1 Polymer Reference Interaction Site Model …

3

increases), the total interfacial area between filler and matrix in the PNC increases, which in turn affects the polymer chain conformation (e.g., radius of gyration) as compared to its (zero-filler or neat polymer) melt-state ideal chain conformation. The chain conformation also alters the effective filler-matrix interaction. If one sets aside the polymer and filler chemistry and the resulting enthalpic driving forces from consideration for a moment, they will realize that the effective filler-matrix interaction is purely a function of the entropic driving forces determined by the filler shape and size, the matrix polymer molecular weight and architecture, and their relative volume fractions in the PNC. The effective filler-matrix or filler-filler interactions dictate whether the filler and the polymer matrix remain mixed (i.e., dispersed filler morphology) or demixed (i.e., aggregated filler morphology) within the PNC. If one also takes into consideration the actual chemistries of the (unmodified) filler and matrix polymer(s), the enthalpic driving forces arising from the filler-filler, matrixmatrix, and filler-matrix (direct) interactions will cooperate/compete with entropic driving forces to alter/retain the chain conformations and the effective filler-matrix interactions that lead to dispersed/aggregated filler morphologies. To go beyond the (limited) design space of PNCs with unmodified or bare additives and incorporate additional tuning parameters that can alter the energetic and entropic driving forces for the PNC morphology and dynamics, one can functionalize the filler surfaces. The many advances in synthetic schemes in the past two decades have paved the way for controllably engineering functionalized/grafted/tethered nanoparticles at the molecular level with a variety of ligand—surfactants, polymers, proteins, and nucleic acids—at a desired grafting density, dispersity, and with desired chemistries. PNCs comprised of polymer-grafted nanoparticles (PGNs) have garnered much interest within the PNC community, both from computational and experimental researchers. References in review articles [10–13, 15–17] have established the link between the molecular design of PGNs and the macroscale structure of PGNs within a polymer matrix for linear (architecture) graft and matrix polymers. At high grafting density or the brush-limit, if the chemistry of the graft and matrix polymer is the same or similar, the system is driven purely by entropic driving forces. Much focus has been placed on tailoring the PGNs such that the resulting entropic driving forces favor mixing of PGNs and matrix chains. The extent to which the matrix chains mix with and penetrate the grafted layer is termed extent of ‘wetting.’ As wetting increases, the matrix chains and PGNs mix, and the extent of filler dispersion within the PNC increases. The key design rules for tuning entropic driving forces to favor wetting are: (a) use matrix polymers of a smaller molecular weight than that of the graft polymer, with the curvature of the filler particle and the value of grafting density dictating how much smaller the matrix chains need to be compared to the graft chain to achieve wetting; (b) include a high dispersity in molecular masses of the graft polymers so as to include few long graft polymers and many short polymers within the grafted layer; and (c) if grafting density and particle size are fixed, choose graft and matrix polymer chemistries that are less flexible and have higher persistence lengths. If the matrix and graft polymer chemistries are dissimilar, then the Flory-Huggins χ parameter between the matrix and graft polymer chemistry together with the other factors that govern the entropic driving forces dictateS whether the PGNs and the

4

A. Jayaraman

matrix will demix or mix at a given temperature. Using a negative χ graft–matrix pair, one can improve grafted layer wetting and push the limits of PGN volume fraction that exhibit PNC dispersion. Recent studies [23–25] have shown that the first-order dispersion to aggregation transition is not synonymous with the wetting to dewetting transition; the latter occurs continuously as the PNC transitions from dispersed to aggregated states. For linear graft and matrix polymers, at low grafting density, the filler surface may not be completely shielded by the grafted chains from the matrix chains and then the energetic driving forces based on the direct filler-graft, fillerfiller, and filler-matrix interactions along with the entropic driving forces decide the extent of mixing/demixing of the PGNs and the matrix. Moving away from a traditional definition of PNCs that has a matrix and a filler component mixed together, one could also consider a melt of PGNs in the absence of a matrix making an effectively one-component PNC. These systems are termed ‘matrix-free PGNs’ and have been receiving attention in the past few years (see for example studies in references [20, 26–29]). One advantage of using these matrixfree PGNs is the ease of processing without dealing with the hassles of creating a homogeneously mixed PNC. Second advantage is the regularity of particle spacing in a polymer melt accomplished through the grafted polymer segments extending from the nanoparticle core. This regularity in interparticle spacing can be exploited in applications like optics, photonics, separation of small molecules, etc. In the absence of free matrix chains, at high grafting density, the grafted chains create a dense region around the core extended outward. Depending on the molecular weight of the grafted chains and the grafting density, one could observe interpenetration between grafted chains on adjacent particles or isolated ‘soft’-grafted particles arranged in an array. Instead of melts, if one created a dense solution of matrix-free PGNs, one can create porous polymer material that can be used for separations [20, 29, 30]. In a recent study conducted on a dried matrix-free PGN solution, upon exposure to a solvent, a combination of small angle x-ray and neutron scattering results showed that the small molecule solvent uniformly distributes around the nanoparticle surface [29]. Going beyond homopolymers as grafts, one could also use block copolymer grafts in such matrix-free PGN melts/dense solutions to achieve matrix-free PNCs with nanoparticles at precise periodicities within microphase-separated block copolymer domains. For example, in a recent experimental study done on poly(styrene-block-(nbutyl acrylate))-grafted silica nanoparticles, the authors found that at higher grafting density, there was better microphase separation of the block copolymers and more uniform filler (core) dispersion in the covalently linked matrix polymer than at lower grafting density with similar polymer chain length and composition [31]. In thin films of PGNs with and without matrix, additional factors including the competing PGN interaction with the free surface, substrate and matrix will affect structure and dynamics. Kim and Green [32], for instance, showed the three regimes of structural organization—PGNs phase separating from the matrix and residing at the free surface and bottom substrate (unstable film is regime I and stable film is regime II) or PGNs being miscible within the film (regime III). They also find that the phase separation in regime I is analogous to thin film of polymer blends (specifically micelles in homopolymers) while the phase separation in regime II is like that seen

1 Polymer Reference Interaction Site Model …

5

in hard spheres in an athermal homopolymer melt. Going beyond homogeneous surfaces, recent experiments on topographically patterned substrate [33] show that the segregation of PGNs can be achieved by varying the relative confinement entropy of grafted versus matrix chains. In studies of matrix-free PGNs adsorbed on a surface, it has been found that increasing the monomer–surface adsorption strength leads to extended polymer chain conformations and adsorption on the surface and adoption of a ‘canopy’ shape. The grafted chains from neighboring ‘canopies’ can interpenetrate at low-moderate graft density and low surface attraction strength. In contrast, at high graft density and/or high surface attraction strengths, the spacing between particles increases and interparticle entanglements reduce. Self-assembly within monolayers of PGNs on surfaces as a function of core–core and core–polymer interactions has also been shown using simulations [34]. These simulations show the relative values of these interactions where one can observe dispersed PGNs, single PGN wide strings of PGNs, stripes of PGNs with width equal to two or three PGNs and clusters of PGNs. PRISM theory has played an important role in some of the above studies. Before describing these studies in Sect. 1.4, it is useful to first go into the basics of PRISM theory, how it links to simulations and ways one could conduct PRISM theory calculations, in the next section.

1.3 PRISM Theory 1.3.1 Basics PRISM theory was developed by Schweizer and Curro [35, 36] from the Reference Interaction Site Model (RISM) theory [37–40] to study chain molecules (i.e., polymers). Its formalism is similar to the Ornstein–Zernike integral equation [40, 41] with the total site–site intermolecular pair correlation function, hij (r), being related to the intermolecular direct correlation function, cij (r), and intramolecular pair correlation function, ωij (r). In Fourier space, PRISM theory takes on the form: H (k) = (k)C (k) (k) + H (k)

(1.1)

where each term is a matrix of size N × N for a system that can be modeled with N types of interaction sites. For example, in a PNC comprised of homopolymer matrix chains of chemistry A with bare nanoscale fillers of chemistry B, if all repeat units along each matrix chain can be treated as equivalent sites of type A and each nanofiller treated as a single site or collection of sites of type B, N would be equal to 2. If the PNC has PGNs, then the graft polymer site (A), matrix polymer site (B) and particle site (C) make it a 3-site system (see Fig. 1.1), and thus, the matrices would be 3 × 3. In that 3-site system, the components of the matrices in (1.1) will be:

6

A. Jayaraman

Fig. 1.1 Schematic of a polymer-grafted nanoparticle (PGN) and a matrix polymer chain, and the definition of the three possible types of sites A, B, and C. The reader should note that in this figure, for the grafted chains, the tethered end segment, the intermediate segments and the free end segment are treated equally with the same type of site (type A). Similarly, for the matrix chain, the free ends and intermediate segments are treating equally (with type B site). In principle, this could be relaxed by using different types of sites representing various parts of the chains. As the number of sites used to represent/model, the system increases so does the size of the matrices in (1.2a−c) and the corresponding numerical complexity for solving the PRISM equations

⎡

⎤ pair pair pair ρ A A hˆ A A (k) ρ AB hˆ AB (k) ρ AC hˆ AC (k) ⎢ ⎥ pair ˆ pair ˆ ˆ H (k) = ⎣ ρ Bpair A h B A (k) ρ B B h B B (k) ρ BC h BC (k) ⎦ pair pair pair ρC A hˆ C A (k) ρC B hˆ C B (k) ρCC hˆ CC (k)

(1.2a)

pair

in which ραβ = ρα ρβ and ρα and ρβ correspond to the site number densities of site types α and β, ⎡

⎤ site site ρ site A A ω A A (k) ρ AB ω AB (k) ρ AC ω AC (k) site site ⎦ (k) = ⎣ ρ Bsite A ω B A (k) ρ B B ω B B (k) ρ BC ω BC (k) site site site ρC A ωC A (k) ρC B ωC B (k) ρCC ωCC (k)

(1.2b)

site site = (ρα + ρβ ) if α = β otherwise ραβ = ρα , and where ραβ

⎡

⎤ cˆ A A (k) cˆ AB (k) cˆ AC (k) C (k) = ⎣ cˆ B A (k) cˆ B B (k) cˆ BC (k) ⎦ cˆC A (k) cˆC B (k) cˆCC (k)

(1.2c)

1 Polymer Reference Interaction Site Model …

7

where cαβ = cβα . The design parameters of the PNC, for example, the filler composition (or volume fraction of filler), grafting density, and graft and/or matrix molecular masses (i.e., chain lengths of the polymer) dictate the ρ i of the sites of type i. The matrix elements of (k) are the intramolecular pair correlation functions in inverse space (or wave vector k) between sites i and j within a certain molecule; these are known and given as an input to the (1.1). For some systems, these functions can be derived analytically (e.g., ideal chain conformations in a polymer melt). The analytical expression for a Gaussian chain conformation is

ωαβ (k) =

1− f2 −

2f n

+

(1 − f )2

2 f n+1 n

(1.3)

where f is defined as f = exp −k 2 σ 2 /6 , n is the number of monomers in the Gaussian chain, and σ is the characteristic distance unit [42]. Similarly, (1.3) can be used to model a freely jointed chain (FJC) with f = sin(kl)/kl, where l is the bond length between sites along the chain [42]. For PGNs, analytic expressions for the particle–graft and graft–graft ωαβ (k) have been derived when the number of grafted chains on the surface is small [43–46]. The scattering community has also derived many analytical forms of ωαβ (k) as ‘form factors’ for fitting the scattering data of commonly studied polymer systems. However, in many cases, analytical expressions for ωαβ (k) for the PNC of interest does not exist. Rather than deriving a new analytical expression, one can simulate the PNC and sample configurations of the molecule of interest to calculate the ωαβ (k) (see description in Sect. 1.3.2.1). The matrix elements of H (k) and C(k) are usually unknown and are to be solved for. Given two unknown matrices and one PRISM equation (1.1), we need one more independent equation to solve for the two unknowns. This additional equation is called the closure relation. Closure relations connect the real-space direct pair correlation functions cij (r), total intermolecular pair correlation function hij (r), and pair-wise interaction potentials, U ij (r). Since the closures include pair-wise interaction potentials, U ij (r), it is through these closures that the chemical details of the PNC are specified. Examples of closures include Percus–Yevick (PY), Hypernetted Chain (HNC), Mean-Spherical Approximation (MSA), Martynov–Sarkisov (MS), and Laria–Wu–Chandler (LWC) [47, 48]. The choice of the type of closure used to solve (1.1) is critical as this choice dictates how realistic or correct the PRISM theory predictions are. We discuss this again in the limitations of this method (Sect. 1.5). Therefore, the right closure must be found or developed for the system being studied. For PNCs, based on agreement between PRISM theory and molecular simulations, for mixtures of nanoparticles and homopolymers, many studies [43–46, 49–54] have used the PY closure for polymer–polymer pair and polymer–particle pair, and the HNC closure for particle–particle pair. If σ ij is the distance of closest approach between sites i and j, (e.g., σ ij = d for monomer–monomer pairs and σ ij = (D + d)/2 for particle–monomer pairs, where d is the size of the monomer site and D is the size of the particle) the impenetrability condition applies inside the hard core.

8

A. Jayaraman

gi j (r ) = 0 r < σi j

(1.4a)

Outside the hard core, the PY approximation for ij pair of sites is written as ci j (r ) = 1 − eβUi j (r ) gi j (r ) r > σi j

(1.4b)

and the HNC closure, often used for the particle–particle pair (hence the subscript CC based on type of sites as shown in Fig. 1.1), is described as cCC (r ) = h CC (r ) − ln gCC (r ) − βUCC (r )

r>D

(1.4c)

Past studies by Schweizer and Yethiraj have suggested that molecular closures [47, 55, 56] could prove more accurate for systems with strongly segregating polymers or monomer species (e.g., strongly segregating copolymer matrix polymer or copolymers grafts, or strongly segregating graft and matrix homopolymers). For this statement to be confirmed for the PNC system at hand, one needs to conduct systematic comparisons of results from PRISM theory using atomic and molecular closures against results from experiments and/or molecules simulation results. After the closures have been selected, one can solve the above system of coupled nonlinear integral (PRISM theory) equation and closure(s). Analytical solutions only exist for atomic systems while numerical solutions are found for complex polymer systems. In principle, one could select any method from existing numerical methods used commonly to solve integral equations [57, 58]. Recent studies have employed the KINSOL algorithm [59] with the line search optimization strategy which minimizes the objective function along an optimum descent direction. KINSOL exhibits convergence for complex nonlinear integral equations easier and faster as compared to the Picard technique, which has also been used in some PRISM theory studies [7, 58]. Irrespective of the numerical algorithm one chooses to use, upon solving the PRISM equation and closure(s), one will obtain the total intermolecular pair correlation functions, hij (r), which can be related to the gij (r) (=hij (r) + 1) and the partial collective structure factors, S ij (k). The partial structure factors are the elements of the S (k) matrix which are related to the direct pair correlation functions and total pair correlation functions as

S (k) = C(k) + H (k)

(1.5a)

These pair-wise structure factors can be compared to the corresponding pair correlation functions from simulations or scattering results from experiments. By obtaining the gij (r), one can calculate other properties of interest as well. For example, the potential of mean force (PMF) between particles, W CC (r), can be calculated, from the particle–particle pair correlation function as follows. WCC (r ) = −kT ln gCC (r )

(1.5b)

1 Polymer Reference Interaction Site Model …

9

Similarly, the second virial coefficient can be calculated from gcc (r) for PNCs at infinitely dilute concentrations. The pair-wise structure factors and the intermolecular direct correlation function together also provide an estimate of the induced solvation potential that one component (e.g., PGN) feels because of the other component (e.g., matrix chains); this is described in Sect. 1.3.2.2. For some PNC design parameters, (e.g., stronger attractive interaction strengths, large site size ratios, D/d, etc.), the numerical method selected may not yield any solutions. This could be an issue with numerical convergence due to a poor initial guess [57] or due to deviations from liquid-like behavior due to (micro/macro) phase separation within the system. This is discussed further in the limitations described in Sect. 1.5.

1.3.2 Linking to Molecular Simulation PRISM theory calculations can be complemented by molecular simulations in multiple ways and this section describes some of these synergies.

1.3.2.1

Providing Realistic Intramolecular Pair Correlation Function (i.e., Shapes of Molecules)

In many past PRISM theory studies of PNCs (e.g., bare fillers in homopolymer matrix or lightly grafted PGNs in homopolymer matrix) [43–46, 49–54] the intramolecular pair correlation, ij , was calculated by assuming ideal conformations of the matrix chains. But, assuming ideal chain conformations for the polymer could be far from reality in some systems. For example, the chains on a densely grafted PGN or a copolymer-grafted particle have been shown to adopt non-ideal conformations, and therefore, using ideal conformations for the grafted chains is not valid. Similarly, the grafted chains in chemically dissimilar graft–matrix systems could adopt extended (collapsed) configurations to initiate (deter) formation of energetically favorable (unfavorable) contacts with matrix chains. For such cases where an off-the-shelf analytical expression of the intramolecular pair correlation, ij , is not available or existing analytical intramolecular pair correlation functions are not valid, molecular simulations serve as a valuable tool for providing realistic intramolecular pair correlation, ij . For example, one can use molecular dynamics simulations or Monte Carlo (MC) simulation techniques (e.g., see review articles on simulations of polymers and PNCs [60–64]) to sample a single homopolymer-grafted nanoparticle in a polymer matrix. These simulations provide the ensemble average graft monomer–graft monomer, graft monomer–particle, matrix monomer–matrix monomer intramolecular pair correlation functions. These correlation functions are calculated using the Debye scattering relation [65, 66]

10

A. Jayaraman

ωαβ (k) =

1 N total

Nβ Nα sin(k·ri j ) i

j

k·ri j

(1.6)

in which α and β represent site types, Nα is the total number of sites of type α in each molecule, Nβ is the total number of sites of type β in each molecule, N total = (Nα + Nβ ) if α = β otherwise N total = Nα , ri j is the distance between sites i and j, and the angle brackets represent ensemble averaging over uncorrelated snapshots in a simulation trajectory. In some cases, to reduce the computational intensity of having to simulate the PGN(s) in a melt-like matrix, one could simulate separately a single matrix polymer chain in vacuum and a single PGN in vacuum to obtain the pair-wise intramolecular correlations. However, these vacuum simulations do not capture the effects of the matrix chains on the grafted polymer configurations or vice versa, and thus, are approximate intramolecular pair correlations.

1.3.2.2

Self-consistent PRISM Theory-Simulation Loop

PRISM theory and molecular simulations can also be linked together in a selfconsistent loop where the intramolecular pair correlation functions (e.g., chain conformations) that are input to PRISM theory are provided by simulations of a single PGN in an external medium-induced solvation potential that is obtained from PRISM theory. The interdependence of the chain conformations and the mediuminduced solvation potential gives rise to the self-consistent loop (Fig. 1.2). The steps involved in this self-consistent loop are described next. First, the pair-wise decomposed medium-induced solvation potential, ψ ij (r), is obtained from the PRISM theory output. This pair-wise function describes the interaction between any two sites i and j as mediated by all the other sites in the system. The form of the solvation potential depends on the approximation used in its derivation [67–72]. The PY and HNC forms of the solvation potential are as follows: ΔψiPY j (r ) = −k B T ln 1 + cik (r ) ∗ skk (r ) ∗ ck j (r )

(1.7a)

ΔψiHj N C (r ) = −k B T cik (r ) ∗ skk (r ) ∗ ck j (r )

(1.7b)

where ‘*’ in (1.7a) and (1.7b) denote a convolution integral in spatial coordinates and k B is the Boltzmann constant and T is the temperature. The terms on the right-hand side of (1.7a) and (1.7b) are the real-space pair-wise direct pair correlation function and real-space analog of the structure factors. The solvation potential, ψ ij (r), is then input to a molecular simulation of a single PGN and/or a single matrix chain. In the simulation, the total interaction potential between sites i and j separated by a distance r, Uitot j (r ) is defined as the sum of U ij (r) and the solvation potential, ψ ij (r), obtained from the preceding PRISM step. To ensure the sites in the PRISM theory

1 Polymer Reference Interaction Site Model …

11

Fig. 1.2 Flowchart of self-consistent PRISM—molecular simulation approach. ‘pyPRISM’ is the open-source package which the reader could use to conduct this calculation. This package is described in Sect. 1.3.3. This figure is reprinted with permission from [58] (2018) American Chemical Society

and molecular simulations represent the same thing, it is best to keep the model chosen to represent the PGN and the matrix polymer to be the same in both PRISM theory and molecular simulations. Next, the PRISM theory calculation and molecular simulation steps are repeated one after the other. In PNCs with PGNs, one could either alternately simulate a single PGN or a single matrix chain with the newest set of pair-wise solvation potentials from PRISM calculations or simultaneously simulate the single PGN and a single matrix chain (in parallel) with the same set of solvation potentials calculated from the previous PRISM step. Irrespective of the simulation method, the intramolecular structure factors between site pairs are sampled from uncorrelated configurations and the ensemble average of the intramolecular structure factors is calculated to serve as the new input for the following iteration of PRISM theory calculations. The self-consistent PRISM theory—molecular simulation loop iterations are continued until convergence is achieved. One convergence criterion is the sum of squared errors (SSE) of ψ ij (r) between iterations n and n + 1:

12

A. Jayaraman

SS E n→n+1 =

Nr 2 n ψin+1 j (r m ) − ψi j (r m )

(1.7a)

i, j m=1

where N r is the number of points over which real space has been discretized. The subscripts i and j denote those pairs of sites whose interactions are relevant to the simulation. The convergence counter, n, is set to 0 for the first iteration. The SSE for the transition n → n+1 (n ≥ 1) is expressed relative to that from 0 → 1. Convergence is attained when the following criterion is fulfilled in say three or five consecutive iterations: SS E n→n+1 ≤ 0.01 SS E 0→1

(n ≥ 1)

(1.7b)

This approach was specifically used in work by Nair and Jayaraman [73] to tackle non-ideal conformations along the grafted copolymers and matrix polymers that were neglected in the studies of homopolymer-grafted nanoparticles [43–46] preceding Nair and Jayaraman’s work. Furthermore, in contrast to older self-consistent PRISMMC studies on homopolymer melts alone [68, 70, 71, 74–76] or work on bare particles in a homopolymer melt [77, 78] where the self-consistent loop involved MC simulations of only one matrix polymer chain, in the study by Nair and Jayaraman [73], alternate self-consistent loops for a single copolymer-grafted particle and a single matrix chain were used. This approach accounts for non-idealities in both the grafted and matrix chain conformations. A similar self-consistent PRISM-MC approach was previously applied to a blend of two polymers where the self-consistent loops involved MC simulations of each polymer [79, 80].

1.3.3 Open-Source Package pyPRISM Having discussed the above basics features of PRISM theory and how to link it to molecular simulations, we now present briefly some details of an open-source package that one could use to conduct PRISM theory calculations on PNCs. Recently, we developed pyPRISM, a Python-based open-source package, to ease the implementation and use of PRISM theory by expert and novice researchers who study PNCs and other soft materials. pyPRISM provides a user-friendly interface for setting up PRISM theory calculations for the problem at hand, along with underlying data structures that simplify the mathematics involved in setting up and solving PRISM theory. The documentation and knowledge base materials are hosted on the repository website [81–83] and maintained by Dr. Tyler Martin and coworkers at National Institute of Standards and Technology (NIST). This online resource helps users to produce correct results with PRISM theory and easily contribute, create, and modify closures, numerical solution algorithms, and analyses for other users. Along with the details of this package, we published a detailed pedagogical review [58] describing

1 Polymer Reference Interaction Site Model …

13

Fig. 1.3 a Particle–particle site–site pair correlations, g P P (r ), versus reduced separation distance, r/d, in a PNC at a total packing fraction, η = 0.4, with a freely jointed chain matrix of length, N = 100, with attractive polymer–particle interactions at an attraction strength, ε = 1.0, and with varying interaction range, α, as described in Fig. 1.3 of [49]. b Particle–particle potential of mean force, w P P (r ), versus reduced separation distance, r/d, between polymer grafted particles in a linear polymer matrix at a total packing fraction of η = 0.35 for varying graft architecture and matrix length, N M , as discussed in Fig. 9 of [84]. The lines are the predictions from pyPRISM and the symbols are data extracted from the corresponding referenced literature. In both subplots, d = 1.0 is the characteristic length scale of the system equal to the monomer site diameter. The details of how these data are generated using pyPRISM can be found in the companion pyPRISM tutorial [83]. Caption and figure were reprinted with permission from [58] (2018) American Chemical Society

how PRISM theory has been applied to a large range of soft matter studies along with results for a few case studies, including PNCs. The results of the PNC case studies calculated using pyPRISM were compared to the original studies (see Fig. 1.3), some of which we describe next.

1.4 Past, Present, and Future of PRISM Theory-Based PNC Studies PRISM theory has been a valuable tool for predicting of how PNC design parameters impact the PNC morphology and phase behavior. Early studies by Hooper

14

A. Jayaraman

and Schweizer as well as Hall and Schweizer have established how the structure of PNCs with bare particles in free polymer matrix is affected by particle–particle attraction, polymer–particle attraction, particle size to polymer matrix chain length ratio, PNC filler fraction, etc. [49–54]. Some of these results have also been corroborated with direct structural comparisons with experiments, in particular scattering results [52]. Jayaraman and Schweizer have extended PRISM theory to study lightly grafted particles (i.e., PGNs with homopolymers tethered on the particles at a low grafting density) in dense solutions without matrix as well as in chemically identical homopolymer matrix chains [43–46]. These studies have shown how increasing the number of grafts and varying their placement on the particle surface impact effective interparticle interactions, PNC structure, and the microphase spinodal curves. Martin and Jayaraman used PRISM theory to predict that increasing dispersity in the chain lengths of the homopolymer grafts on PGNs improves dispersions of the PGNs in a chemically identical homopolymer matrix (Fig. 1.4a) [85–87]. Moving beyond chemically identical graft and matrix polymers, in PNCs with PGNs placed a)

Monodisperse

Polydisperse

b)

Fig. 1.4 a PGNs with disperse polymer grafts increase the particle–particle repulsion in a polymer nanocomposite. b PNCs with chemically distinct graft and matrix polymers exhibit gradual change in wetting with temperature in contrast to a first-order particle dispersion to aggregation transition. Figures in part a are reproduced from [85] with permission from Royal Society of Chemistry. Figure in part b has been reprinted with permission from [25] (2016) American Chemical Society

1 Polymer Reference Interaction Site Model …

15

in a chemically dissimilar polymer matrix (Fig. 1.4b), PRISM theory along with molecular simulations has shown that the grafted layer wetting–dewetting transition is a second-order transition and distinct from the PGN dispersion–aggregation (firstorder) transition [23–25]. Calculation of the effective χ parameter and second virial coefficient underlying these wetting–dewetting and dispersion–aggregation transitions provided additional insight into the dispersion–aggregation transition occurring when the extent of grafted layer wetting matched that of the analogous athermal PNC. The above PRISM theory-based studies have focused on linear polymers, both in graft and matrix chains, and polymer chemistries that can be modeled using isotropic intersite interaction potentials. One can expect to observe unique phase behavior, not seen previously, by moving toward nonlinear polymer architectures (e.g., bottlebrushes, comb/graft polymers, cyclic/ring polymers) and/or polymer chemistries with directional and specific interactions (e.g., hydrogen bonding, pi-pi stacking). Given the many advances in polymer synthesis and techniques for grafting polymers to or from particle surfaces, there is a strong motivation to understand potential impacts of nonlinear polymer architecture in graft and/or matrix chains on PNC structure and dynamics. For example, bottlebrush polymer is one specific class of nonlinear architectures that has received significant attention in many recent synthetic, computational, and theoretical studies [88–94]. Bottlebrush polymers are comprised of a linear backbone with side chains emanating from the backbone. These polymers can be synthesized in a controlled manner with varying side chain chemistry, molecular weight, and grafting density along the backbone. In the context of PNCs, the complexity brought about by grafting such bottlebrush polymers onto particle surface is worth exploring. The increased crowding between the sidechains on the bottlebrush and between the bottlebrushes on the nanoparticle surface should significantly increase the conformational entropy loss of the (linear or nonlinear) matrix polymer chain penetrating the grafted layer. By dialing down the grafting density on the particle surface, one may approach the same wetting–dewetting and/or dispersion–aggregation physics as the densely grafted linear polymer containing PGNs. Two PRISM theory-based studies have tackled some of the above questions. One study by Modica et al. using PRISM theory and Langevin dynamics compared and contrasted comb polymers (i.e., bottlebrush with low grafting density along the polymer backbone) grafts versus linear grafts in PNCs with linear matrix chains [84]. They found that compared to linear polymers, the comb polymers exhibit a stronger effective attraction between the grafted particles in both small molecule solvent and polymer matrix due to the increased crowding in the grafted layer from the comb polymer side chains. They also found that the effective interactions (i.e., PMF) between the grafted particles are more sensitive to the comb polymer design (i.e., side chain length and spacing) in a small molecule solvent than in a polymer matrix. Using nonlinear polymer architecture in the matrix can also alter the tendency for particle dispersion/aggregation as compared linear polymer matrix. In another PRISM theory study [95], the use of comb polymer architecture in the matrix leads to reduced (bare) nanoparticle aggregation for moderate nanoparticle–monomer attraction strength and increased bridging of nanoparticles at relatively large nanoparticle–monomer attraction. These effects brought about by using comb polymer architecture versus linear

16

A. Jayaraman

polymer architecture in the matrix can be subdued/enhanced through the choice of comb polymer grafting density, side chain to backbone length ratio, etc. Gradients in sidechain length and crowding along bottlebrushes could be exploited, say with increasing crowding from the tethering point outward to create polymer grafted particles with uniform monomer density radially. Alternately, gradient brushes could be designed to engineer layers of varying monomer densities in the grafted layer. These are potential new topics for PRISM theory-based studies. The subject of how associating polymer chemistries (e.g., hydrogen bonding or π-π stacking between graft and matrix polymers) alter the grafted chain conformation, matrix-graft interpenetration, grafted layer structure, effective interactions, PNC morphology has received far less attention than other simpler polymer chemistries modeled using isotropic interactions. These directional interactions have been studied in detail in polymer blends (i.e., mixture of homopolymers or copolymers with hydrogen bonding chemistries) where hydrogen bonding has been shown to alter the structure (e.g., conformations associated with intrachain vs. interchain hydrogen bonding) and chain dynamics. Past experimental studies [96–99] have shown that polymer blends with intermolecular hydrogen bonds are characterized by a single glass transition temperature indicating miscibility between blend components. Hydrogen bonded polymer blends show coupling of segmental relaxations (leading to a single alpha relaxation) in blend components and also suppressed concentration fluctuations [100]. The inter- and intra-associations between hydrogen bonding moieties have also been shown to affect the dynamic moduli (G’ and G”) in the terminal regime [101]. The potential of similar striking effects in PNCs motivates investigations in this avenue. Motivated by these experiments, Kulshreshtha et al. developed new coarse-grained models to study PNCs with a single polymer grafted nanoparticle with (linear) graft polymers placed in a linear polymer matrix with graft and matrix polymers having directional and specific interactions [102]. Interestingly, even if one observed equivalent grafted layer wetting in PNCs with isotropic interactions and PNCs with directional graft–matrix interactions, there were some major differences in the way graft and matrix chains interacted. Each graft polymer in the PNC with directional graft–matrix interactions interacts with fewer matrix chains and has much lower free volume than in the PNCs with isotropic graft–matrix interactions. This difference could have major implications on the particle–particle effective interactions, glass transition temperature of the PNC, as well as the mechanical and rheological properties for these PNCs. Incorporation of this new coarse-grained model [102] within the PRISM theory framework and studies of PNCs with directional and specific interactions between the grafts and matrix polymers at finite filler fractions is another new direction for a PRISM theory-based study.

1 Polymer Reference Interaction Site Model …

17

1.5 Limitations of PRISM Theory Despite the many successful applications of PRISM theory for PNC studies, it is important to highlight some limitations associated with the use of PRISM theory especially for studying PNCs. The first limitation is the strong dependence of PRISM theory’s results on the closures chosen. For example, past work has shown that by using atomic closures to describe the phase behavior of polymer blends results leads to an incorrect scaling dependence of the spinodal temperature on the polymer chain length [103]. To produce the correct scaling, one could use thermodynamic perturbation theory [104] or molecular closures [47, 105]. These issues are also relevant for PNCs with a mixed polymer blend as matrix or with chemically dissimilar graft and matrix polymers. As stated above in Sect. 1.3.3, the pyPRISM package allows users to assess the effect of the closure itself on the results by making an easier user-interface to switch between closures and/or implement new closures. PRISM theory’s foundation as a liquid-state theory implies that it is only applicable for systems with liquid-like structural correlations [106]. One could interpret this as an inability of PRISM theory to directly predict correlations for the glassy or crystalline states of polymer matrix or grafted layer in the PNC. Also, PRISM theory cannot directly predict the structure of an ordered, macrophase-separated, or microphase-separated phases in PNCs. However, modern thermodynamic density functional theories that can be used to study spatially inhomogeneous systems need liquid-state correlations as input, and PRISM theory could be useful for this task [107–110]. Furthermore, PRISM theory study of thin films of PNCs or PNCs near surfaces/interfaces is not as straightforward as studies of bulk PNCs (i.e., away from surface effects) and needs a fairly complex treatment (see, for example, [111]). Another major challenge is simply (numerically) solving the PRISM theory equations. In particular, the choice of the algorithm, (e.g., Picard, Inexact Newton), the chosen initial guess of the solution, and the convergence criteria for the iterations within the numerical solution method are among the many considerations that impact convergence of the PRISM theory equations to a solution. These choices are not trivial and require multiple tests before a lack of solution for the given system, can be attributed to the system being structurally inhomogeneous rather than a numerical issue. Lastly, unlike stochastic and deterministic molecular simulation methods like molecular dynamics or MC, PRISM theory does not produce a trajectory of coordinates of the ‘sites’ in the system. The output from PRISM theory is purely in the form of pair correlations in real/inverse space, and inferences about the structure and phase behavior come from these pair correlations. For computational or experimental users of PRISM theory, the lack of a visual interpretation of their results (e.g., in the form of simulation snapshots) is often disappointing. Interestingly, self-consistent PRISM-simulation methods partially mitigate this problem by providing trajectories of single molecules in a mean-field, medium-induced solvation potential. Lastly,

18

A. Jayaraman

unlike molecular dynamics, PRISM theory cannot provide any information about the dynamics within the PNCs.

1.6 Conclusions This chapter presented the basics of PRISM theory and the key considerations that one needs to make in order to obtain meaningful results from PRISM theory studies of PNC structure and phase behavior. We presented a review of past studies on PNCs using experiments, theory, and simulations to describe the main fundamental questions that have been posed and tackled in this field. PRISM theory’s successes were also highlighted to demonstrate the many valuable research contributions to the PNC literature made possible by use of PRISM theory. We also briefly mentioned pyPRISM, an open-source package developed by Martin, Jayaraman, and coworkers and hosted by NIST to encourage readers to use PRISM theory without concerning themselves with the tedious computational implementation. We concluded the chapter with a few key limitations of PRISM theory to caution the readers of the potential challenges they could encounter when using PRISM theory for studying PNCs.

References 1. R.A. Vaia, E.P. Giannelis, Polymer nanocomposites: status and opportunities. MRS Bull. 26(5), 394–401 (2001) 2. J. Jordan et al., Experimental trends in polymer nanocomposites—a review. Mater. Sci. Eng. A 393(1–2), 1–11 (2005) 3. A.J. Crosby, J.Y. Lee, Polymer nanocomposites: the “nano” effect on mechanical properties. Polym. Rev. 47(2), 217–229 (2007) 4. R. Krishnamoorti, R.A. Vaia, Polymer nanocomposites. J. Polym. Sci. Part B: Polym. Phys. 45(24), 3252–3256 (2007) 5. K.I. Winey, R.A. Vaia, Polymer nanocomposites. MRS Bull. 32(4), 314–322 (2007) 6. V. Ganesan, C.J. Ellison, V. Pryamitsyn, Mean-field models of structure and dispersion of polymer-nanoparticle mixtures. Soft Matter 6(17), 4010–4025 (2010) 7. L.M. Hall, A. Jayaraman, K.S. Schweizer, Molecular theories of polymer nanocomposites. Curr. Opinion Solid State Mater. Sci. 14(2), 38–48 (2010) 8. J. Jancar et al., Current issues in research on structure–property relationships in polymer nanocomposites. Polymer 51(15), 3321–3343 (2010) 9. S.K. Kumar, R. Krishnamoorti, Nanocomposites: structure, phase behavior, and properties. Ann. Rev. Chem. Biomol. Eng. 1, 37–58 (2010) 10. P.F. Green, The structure of chain end-grafted nanoparticle/homopolymer nanocomposites. Soft Matter 7(18), 7914–7926 (2011) 11. A. Jayaraman, Polymer grafted nanoparticles: effect of chemical and physical heterogeneity in polymer grafts on particle assembly and dispersion. J. Polym. Sci. Part B—Polym. Phys. 51(7), 524–534 (2013) 12. S.K. Kumar et al., Nanocomposites with polymer grafted nanoparticles. Macromolecules 46(9), 3199–3214 (2013)

1 Polymer Reference Interaction Site Model …

19

13. V. Ganesan, A. Jayaraman, Theory and simulation studies of effective interactions, phase behavior and morphology in polymer nanocomposites. Soft Matter 10(1), 13–38 (2014) 14. S. Srivastava et al., 25th anniversary article: polymer–particle composites: phase stability and applications in electrochemical energy storage. Adv. Mater. 26(2), 201–234 (2014) 15. V.V. Ginzburg, In: Problems of Nonlinear Mechanics and Physics of Materials Springer, (2019) 16. M.J. Hore, Polymers on nanoparticles: structure & dynamics. Soft Matter 15(6), 1120–1134 (2019) 17. S.K. Kumar et al., 50th anniversary perspective: are polymer nanocomposites practical for applications? Macromolecules 50(3), 714–731 (2017) 18. J.M. Garcés et al., Polymeric nanocomposites for automotive applications. Adv. Mater. 12(23), 1835–1839 (2000) 19. V.T. Rathod, J.S. Kumar, A. Jain, Polymer and ceramic nanocomposites for aerospace applications. Appl. Nanosci. 7(8), 519–548 (2017) 20. J.W. Barnett, S.K. Kumar, Modeling gas transport in polymer-grafted nanoparticle membranes. Soft Matter 15(3), 424–432 (2019) 21. S.R. Silva, et al., Hybrid and Nanocomposite Materials for Flexible Organic Electronics Applications (2015), pp. 57–84 22. I. Armentano et al., Biodegradable polymer matrix nanocomposites for tissue engineering: a review. Polym. Degrad. Stab. 95(11), 2126–2146 (2010) 23. T.B. Martin, A. Jayaraman, Tuning the wetting–dewetting and dispersion–aggregation transitions in polymer nanocomposites using composition of graft and matrix polymers. Mater. Res. Express 3(3), 034001 (2016) 24. T.B. Martin, A. Jayaraman, Using theory and simulations to calculate effective interactions in polymer nanocomposites with polymer-grafted nanoparticles. Macromolecules 49(24), 9684–9692 (2016) 25. T.B. Martin et al., Wetting-dewetting and dispersion aggregation transitions are distinct for polymer grafted nanoparticles in chemically dissimilar polymer matrix. J. Am. Chem. Soc. 137(33), 10624–10631 (2015) 26. N.J. Fernandes et al., Hairy nanoparticle assemblies as one-component functional polymer nanocomposites: opportunities and challenges. MRS Commun. 3(1), 13–29 (2013) 27. G. Hou et al., Designing superlattice structure via self-assembly of one-component polymergrafted nanoparticles. J. Phys. Chem. B 123(9), 2157–2168 (2019) 28. C.R. Bilchak et al., High-frequency mechanical behavior of pure polymer-grafted nanoparticle constructs. ACS Macro Lett. 8(3), 294–298 (2019) 29. E. Buenning et al., Location of imbibed solvent in polymer-grafted nanoparticle membranes. ACS Macro Lett. 7(9), 1051–1055 (2018) 30. C.R. Bilchak et al., Polymer-grafted nanoparticle membranes with controllable free volume. Macromolecules 50(18), 7111–7120 (2017) 31. Y. Huang et al., Matrix-free polymer nanocomposite thermoplastic elastomers. Macromolecules 50(12), 4742–4753 (2017) 32. J. Kim, P.F. Green, Phase behavior of thin film brush-coated nanoparticles/homopolymer mixtures. Macromolecules 43(3), 1524–1529 (2010) 33. R. Zhang et al., Entropy-driven segregation of polymer-grafted nanoparticles under confinement. Proc. Natl. Acad. Sci. 114(10), 2462 (2017) 34. T. Lafitte, S.K. Kumar, A.Z. Panagiotopoulos, Self-assembly of polymer-grafted nanoparticles in thin films. Soft Matter 10(5), 786–794 (2014) 35. K.S. Schweizer, J.G. Curro, Integral-equation theory of the structure of polymer melts. Phys. Rev. Lett. 58(3), 246–249 (1987) 36. J.G. Curro, K.S. Schweizer, Theory of polymer melts—an integral-equation approach. Macromolecules 20(8), 1928–1934 (1987) 37. C.S. Hsu, D. Chandler, RISM calculation of the structure of liquid chloroform. Mol. Phys. 37(1), 299–301 (1979)

20

A. Jayaraman

38. C.S. Hsu, D. Chandler, RISM calculation of structure of liquid acetonitrile. Mol. Phys. 36(1), 215–224 (1978) 39. C.S. Hsu, D. Chandler, L.J. Lowden, Applications of RISM equation to diatomic fluids— liquids nitrogen, oxygen and bromine. Chem. Phys. 14(2), 213–228 (1976) 40. L.J. Lowden, D. Chandler, Solution of a new integral-equation for pair correlation-functions in molecular liquids. J. Chem. Phys. 59(12), 6587–6595 (1973) 41. L.S. Ornstein, F. Zernike, Acculental deviations of density and opalescence at the critical point of a simple substance. Proc. Koninklijke Akademie Van Wetenschappen Te Amsterdam 17, 793–806 (1914) 42. K.S. Schweizer, J.G. Curro, Integral-equation theory of polymer melts—intramolecular structure, local order, and the correlation hole. Macromolecules 21(10), 3070–3081 (1988) 43. A. Jayaraman, K.S. Schweizer, Effective interactions and self-assembly of hybrid polymer grafted nanoparticles in a homopolymer matrix. Macromolecules 42(21), 8423–8434 (2009) 44. A. Jayaraman, K.S. Schweizer, Effective interactions, structure, and phase behavior of lightly tethered nanoparticles in polymer melts. Macromolecules 41(23), 9430–9438 (2008) 45. A. Jayaraman, K.S. Schweizer, Effect of the number and placement of polymer tethers on the structure of concentrated solutions and melts of hybrid nanoparticles. Langmuir 24(19), 11119–11130 (2008) 46. A. Jayaraman, K.S. Schweizer, Structure and assembly of dense solutions and melts of single tethered nanoparticles. J. Chem. Phys. 128(16) (2008) 47. K.S. Schweizer, A. Yethiraj, Polymer reference interaction site model theory: new molecular closures for phase separating fluids and alloys. J. Chem. Phys. 98, 9053–9079 (1993) 48. A. Yethiraj, K.S. Schweizer, Self-consistent polymer integral-equation theory—comparisons with monte-carlo simulations and alternative closure approximations. J. Chem. Phys. 97(2), 1455–1464 (1992) 49. J.B. Hooper, K.S. Schweizer, Contact aggregation, bridging, and steric stabilization in dense polymer-particle mixtures. Macromolecules 38, 8858–8869 (2005) 50. J.B. Hooper, K.S. Schweizer, Theory of phase separation in polymer nanocomposites. Macromolecules 39, 5133–5142 (2006) 51. J.B. Hooper et al., Structure, surface excess and effective interactions in polymer nanocomposite melts and concentrated solutions. J. Chem. Phys. 121(14), 6986–6997 (2004) 52. L.M. Hall et al., Concentration fluctuations, local order, and the collective structure of polymer nanocomposites. Macromolecules 42(21), 8435–8442 (2009) 53. L.M. Hall, K.S. Schweizer, Many body effects on the phase separation and structure of dense polymer-particle melts. J. Chem. Phys. 128, 234901 (2008) 54. L.M. Hall, K.S. Schweizer, Structure, scattering patterns and phase behavior of polymer nanocomposites with nonspherical fillers. Soft Matter 6(5), 1015–1025 (2010) 55. K.S. Schweizer, Analytic RISM theory of polymer alloys—molecular closure predictions for structurally symmetrical blends. Macromolecules 26(22), 6033–6049 (1993) 56. A. Yethiraj, K.S. Schweizer, Integral equation theory of polymer blends: numerical investigation of molecular closure approximations. J. Chem. Phys. 98, 9080–9093 (1993) 57. I. Collins, W. George, Fundamental Numerical Methods and Data Analysis (Harvard University Press, 2003) 58. T.B. Martin et al., pyPRISM: a computational tool for liquid-state theory calculations of macromolecular materials. Macromolecules 51(8), 2906–2922 (2018) 59. A.C. Hindmarsh et al., SUNDIALS: suite of nonlinear and differential/algebraic equation solvers. ACM Trans. Math. Softw. 31(3), 363–396 (2005) 60. M. Kotelyanskii, D.N. Theodorou, Simulation Methods for Polymers (Marcel Dekker, New York, 2004) 61. A. Karatrantos, N. Clarke, M. Kroger, Modeling of polymer structure and conformations in polymer nanocomposites from atomistic to mesoscale: a review. Polym. Rev. 56(3), 385–428 (2016) 62. A. Gooneie, S. Schuschnigg, C. Holzer, A review of multiscale computational methods in polymeric materials. Polymers 9(1), 16 (2017)

1 Polymer Reference Interaction Site Model …

21

63. G.G. Vogiatzis, D.N. Theodorou, Multiscale molecular simulations of polymer-matrix nanocomposites: or what molecular simulations have taught us about the fascinating nanoworld. Arch. Comput. Methods Eng.: State Art Rev. 25(3), 591–645 (2018) 64. T.E. Gartner, A. Jayaraman, Modeling and simulations of polymers: a roadmap. Macromolecules 52(3), 755–786 (2019) 65. J.D. McCoy et al., Single-chain structure in model polyethylene melts. Macromolecules 25(19), 4905–4910 (1992) 66. P.J. Flory, Statistical Mechanics of Chain Molecules (John Wiley & Sons, Inc, 1969) 67. K.S. Schweizer, J.G. Curro, Integral equation theory of polymer melts: intramolecular structurem local order, and the correlation hole. Macromolecules 21, 3070–3081 (1988) 68. J. Melenkevitz, K.S. Schweizer, J.G. Curro, Self consistent integral equation theory for the equilibrium properties of polymer solutions. Macromolecules 26, 6190–6196 (1993) 69. C.J. Grayce, K.S. Schweizer, Solvation potentials for macromolecules. J. Chem. Phys. 100, 6846–6856 (1994) 70. C.J. Grayce, A. Yethiraj, K.S. Schweizer, Liquid state theory of the density dependent conformation of nonpolar linear polymers. J. Chem. Phys. 100, 6857–6872 (1994) 71. P.G. Khalatur, A.R. Khokhlov, Hybrid MC/RISM technique for simulation of polymer solutions: MC + RISM integral eqns. Mol. Phys. 93, 555–572 (1998) 72. K.S. Schweizer, J.G. Curro, PRISM theory of the structure, thermodynamics, and phasetransitions of polymer liquids and alloys. Adv. Polym. Sci. 116, 319–377 (1994) 73. N. Nair, A. Jayaraman, Self-consistent PRISM theory—Monte Carlo simulation studies of copolymer grafted nanoparticles in a homopolymer matrix. Macromolecules 43(19), 8251– 8263 (2010) 74. S. Mendez et al., An integral equation theory for polymer solutions: explicit inclusion of the solvent molecules. J. Chem. Phys. 115, 5669–5678 (2001) 75. M. Putz, J.G. Curro, G.S. Grest, Self-consistent integral equation theory for polyolefins: comparison to molecular dynamics simulations and x-ray scattering. J. Chem. Phys. 114, 2847–2860 (2001) 76. A. Yethiraj, C.K. Hall, Monte Carlo simulations and integral equation theory for microscopic correlations in polymeric fluids. J. Chem. Phys. 96, 797–807 (1991) 77. A.L. Frischknecht, E.S. McGarrity, M.E. Mackay, Expanded chain dimensions in polymer melts with nanoparticle fillers. J. Chem. Phys. 132, 204901 (2010) 78. P.G. Khalatur, L.V. Zherenkova, A.R. Khokhlov, Entropy-driven polymer collapse: application of the hybrid MC/RISM method to the study of conformational transitions in macromolecules interacting with hard colloidal particles. Eur. Phys. J. B 5(4), 881–897 (1998) 79. D.R. Heine, G.S. Grest, J.G. Curro, Structure of polymer melts and blends: comparison of integral equation theory and computer simulations. Adv. Comput. Simul. Approaches Soft Matter Sci. I(173), 209–249 (2005) 80. D. Heine et al., Role of intramolecular energy on polyolefin miscibility: Isotactic polypropylene/polyethylene blends. J. Chem. Phys. 118(2), 914–924 (2003) 81. T.B. Martin, typyPRISM Tutorial Package. Available from: http://github.com/usnistgov/typ yPRISM_tutorial 82. T.B. Martin, typyPRISM Package. Available from: http://github.com/usnistgov/typyPRISM 83. T.B. Martin, T.E. Gartner III, pyPRISM Tutorial. Available from: http://pyprism.readthedocs. io/en/latest/tutorial/tutorial.html 84. K.J. Modica, T.B. Martin, A. Jayaraman, Effect of polymer architecture on the structure and interactions of polymer grafted particles: theory and simulations. Macromolecules 50(12), 4854–4866 (2017) 85. T.B. Martin, A. Jayaraman, Polydisperse homopolymer grafts stabilize dispersions of nanoparticles in a chemically identical homopolymer matrix: an integrated theory and simulation study. Soft Matter 9(29), 6876–6889 (2013) 86. T.B. Martin, A. Jayaraman, Identifying the ideal characteristics of the grafted polymer chain length distribution for maximizing dispersion of polymer grafted nanoparticles in a polymer matrix. Macromolecules 46(22), 9144–9150 (2013)

22

A. Jayaraman

87. T.B. Martin, P.M. Dodd, A. Jayaraman, Polydispersity for tuning the potential of mean force between polymer grafted nanoparticles in a polymer matrix. Phys. Rev. Lett. 110(1), 018301 (2013) 88. J.N. Albert, T.H. Epps III, Self-assembly of block copolymer thin films. Mater. Today 13(6), 24–33 (2010) 89. P.M. Claesson et al., Bottle-brush polymers: adsorption at surfaces and interactions with surfactants. Adv. Coll. Interface. Sci. 155(1–2), 50–57 (2010) 90. S. Peleshanko, V.V. Tsukruk, The architectures and surface behavior of highly branched molecules. Prog. Polym. Sci. 33(5), 523–580 (2008) 91. R. Verduzco et al., Structure, function, self-assembly, and applications of bottlebrush copolymers. Chem. Soc. Rev. 44, 2405–2420 (2015) 92. G. Xie et al., Molecular bottlebrushes as novel materials. Biomacromol 20(1), 27–54 (2018) 93. G.E. Stein, T.S. Laws, R. Verduzco, Tailoring the attraction of polymers toward surfaces. Macromolecules 52(13), 4787–4802 (2019) 94. D.J. Walsh, D. Guironnet, Macromolecules with programmable shape, size, and chemistry. Proc. Natl. Acad. Sci. 116(5), 1538–1542 (2019) 95. Q. Xu et al., Structure and effective interactions of comb polymer nanocomposite melts. J. Chem. Phys. 141(20), 204901 (2014) 96. E.J. Moskala et al., On the role of intermolecular hydrogen bonding in miscible polymer blends. Macromolecules 17(9), 1671–1678 (1984) 97. S. Viswanathan, M.D. Dadmun, Guidelines to creating a true molecular composite: inducing miscibility in blends by optimizing intermolecular hydrogen bonding. Macromolecules 35(13), 5049–5060 (2002) 98. S.-W. Kuo, C.-L. Lin, F.-C. Chang, The study of hydrogen bonding and miscibility in poly (vinylpyridines) with phenolic resin. Polymer 43(14), 3943–3949 (2002) 99. Y. He, B. Zhu, Y. Inoue, Hydrogen bonds in polymer blends. Prog. Polym. Sci. 29(10), 1021–1051 (2004) 100. S. Zhang, P.C. Painter, J. Runt, Coupling of component segmental relaxations in a polymer blend containing intermolecular hydrogen bonds. Macromolecules 35(25), 9403–9413 (2002) 101. Z. Yang, C.D. Han, Rheology of miscible polymer blends with hydrogen bonding. Macromolecules 41(6), 2104–2118 (2008) 102. A. Kulshreshtha, K.J. Modica, A. Jayaraman, Impact of hydrogen bonding interactions on graft-matrix wetting and structure in polymer nanocomposites. Macromolecules 52(7), 2725– 2735 (2019) 103. H.P. Deutsch, K. Binder, Evidence against the integral-equation theory of polymer blends. Europhys. Lett. 17(8BIS), 697–702 (1992) 104. J.J. Rajasekaran, J.G. Curro, J.D. Honeycutt, Theory for the phase-behavior of polyolefin blends—application to the polyethylene/isotactic polypropylene blend. Macromolecules 28(20), 6843–6853 (1995) 105. A. Yethiraj, K.S. Schweizer, Integral-equation theory of polymer blends—numerical investigation of molecular closure approximations. J. Chem. Phys. 98(11), 9080–9093 (1993) 106. J.-P. Hansen, I.R. McDonald, Chapter 4—distribution function theories, Theory of Simple Liquids, 4th edn. (Academic Press, Oxford, 2013), pp. 105–147 107. C.N. Patra, A. Yethiraj, Density functional theory for nonuniform polymers: accurate treatment of the effect of attractive interactions. J. Chem. Phys. 118(10), 4702–4706 (2003) 108. A.L. Frischknecht, et al., Density functional theory for inhomogeneous polymer systems. I. Numerical methods. J. Chem. Phys. 117(22), 10385–10397 (2002) 109. A.L. Frischknecht, J.G. Curro, L.J.D. Frink, Density functional theory for inhomogeneous polymer systems. II. Application to block copolymer thin films. J. Chem. Phys. 117(22), 10398–10411 (2002) 110. J.P. Donley et al., Microscopic approach to inhomogeneous polymeric liquids. J. Chem. Phys. 103(12), 5061–5069 (1995) 111. J.G. Curro et al., The structure of amorphous polymers near surfaces: athermal systems. Comput. Theor. Polym. Sci. 8(1), 159–168 (1998)

Chapter 2

Density Functional Theory-Based Modeling of Polymer Nanocomposites Valeriy V. Ginzburg

Abstract Density functional theory (DFT) is a powerful approach utilized successfully in both quantum and classical theoretical and computational physics. Since the 1970s, DFT has been applied to predict the phase behavior of simple fluids, including the liquid-to-crystal transition in hard-sphere and Lennard–Jones fluids. Beginning in the 1990s, it was recognized that DFT can be adapted to describe the equilibrium morphologies of polymer-based nanocomposites (PNC). Here, we review various examples where DFT is applied to PNCs, from polymer–clay and polymer-nanotube mixtures to one-component hairy nanoparticle assemblies. We also discuss hybrid approaches where DFT is combined with other coarse-grained field theories, in particular, the Self-Consistent Field/Density Functional Theory (SCF-DFT) method and its applications.

2.1 Introduction The performance of polymer nanocomposites depends crucially on the “morphology” or “nanostructure”. The nanofillers can be organized into crystal-like patterns or dispersed randomly within a polymer matrix or aggregated into large clusters. The polymers can also form a homogeneous phase or, alternatively, undergo a microor macro- phase separation. The overall nanocomposite morphology can also be impacted by confinement (e.g., thin films vs. bulk). Understanding and predicting the morphology as a function of the nanocomposite formulation, filler type and geometry, and processing conditions is the biggest challenge in expanding the use of nanocomposite materials to new application areas. Multiple approaches are utilized to address this challenge [1–22]. In this chapter, we mainly concentrate on one approach to predicting the equilibrium nanocomposite morphology—the coarsegrained Density Functional Theory (DFT) based modeling. While DFT—like other equilibrium models—does not describe the dynamics of ordering, phase separation, V. V. Ginzburg (B) Core R&D, The Dow Chemical Company, Midland, MI 48674, USA e-mail: [email protected] © Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1_2

23

24

V. V. Ginzburg

Fig. 2.1 Two classes of polymer nanocomposites

or alignment, it can predict the morphologies that are the most advantageous in a sense that they correspond to the free energy minima, either global or local. Before discussing DFT in-depth, we would like to introduce a “miniclassification”, dividing all nanocomposites into two classes (Fig. 2.1). In the first class, “Nanoparticle limit”, the polymer chains and the nanofillers have comparable dimensions; in the second class, “Colloidal limit”, the nanofillers are significantly larger than the polymers (at least in one dimension). The implication of this distinction, in our view, is as follows. For the first class of nanocomposites, the equilibration occurs simultaneously for both polymers and nanofillers. Thus, one needs to construct the free energy as a functional of the singleparticle distribution functions (“densities”) of both polymers and fillers, and then minimize it appropriately to obtain the equilibrium morphologies. For the second class, however, the equilibration of the nanofillers is much slower than the equilibration of the polymers. Thus, it is necessary to construct the free energy for the polymers and minimize it subject to the “frozen” positions of the fillers; usually, only two filler particles are used for this initial minimization. The positions of the two particles are then updated, and the polymer-free energy is calculated for each inter-particle separation. The result of this process is the so-called potential of mean force (PMF) for the particles due to their interactions with the polymers. Once the PMF is known, the particles are equilibrated next. Thus, the approach used to model the morphology and phase behavior of nanocomposites depends crucially on the nanoparticle size. It is clear that spherical nanoparticles with RP < 2 nm belongs to the first class, while most nanorods, nanoplatelets, and nanospheres with RP > 10 nm belong to the second class. However, for nanospheres with 2 nm < RP < 10 nm, the classification might be more ambiguous, especially if the fillers and polymers are polydisperse.

2 Density Functional Theory-Based Modeling …

25

The rest of the chapter is structured as follows. In Sect. 2.2, we review the history of the density functional theory and its applications to polymers, liquid crystals, and colloids. In Sect. 2.3, the applications of the DFT to polymer nanocomposites are discussed. In Sect. 2.4, we describe a special “hybrid” approach to nanocomposite modeling, combining the “standard” DFT for spherical particles with the polymer self-consistent field theory (SCFT). Lastly, Sect. 2.5 contains the summary and outlook for future theory developments.

2.2 DFT Overview Density functional theory originated in the 1960s with the pioneering work of Hohenberg and Kohn [23] and Kohn and Sham [24], outlining a radically new method of calculating electronic structures of complex atoms. This work was subsequently recognized by 1998 Nobel Prize in Chemistry awarded to Walter Kohn [25]. The main idea of the DFT approach is that the energy and other characteristics of a multiparticle system can be fully described by a functional of a single-particle density, provided that one correctly captures correlations and “exchange” interactions. The triumph of DFT in quantum chemistry also helped promote its applications in classical condensed matter. Ramakrishnan and Yussouff [26] first formulated a classical DFT-like model to describe the first-order liquid–solid transition (“freezing”) in simple liquids. To parameterize the non-ideal portion of the free energy functional, several approaches (local density approximation [LDA] [27, 28], weighted density approximation [WDA] [29–33], and fundamental measure theory [FMT] [34–39]) have been developed and refined over the course of the last thirty years (see reviews [40, 41] for a more detailed discussion). The original analysis centered on the hard-sphere and Lennard–Jones sphere freezing; subsequently, the method was also extended to describe phase transitions in anisotropic, liquid-crystalline particles [42–50]. Equally momentous, in the 1980s and 1990s DFT was extended to describe flexible polymer chains [51–62]; for more details on those polymer DFTs, see reviews [63, 64]. Example applications of polymer DFT include bulk crystallization [65–67] and ordering near hard surfaces [59, 68–71]. The general idea of DFT in the context of classical fluids is as follows. Let us consider, as an example, a multicomponent polymer melt. For each monomer type, labeled α, one can define the single-particle density, ρα (r), and write down the free energy of the overall system in the following form (here, we use the grand-canonical ensemble, with the chemical potential of the α-polymer denoted μα ), [ρα (r)] ≡ F[ρα (r)] +

drρα (r)[Vα (r) − μα ]

α

= Fid [ρα (r)] + Fex [ρα (r)] + Fch [ρα (r)] + Fint [ρα (r)] + drρα (r)[Vα (r) − μα ] α

(2.1)

26

V. V. Ginzburg

Here, the first term in the right-hand side, F id , is the ideal-gas contribution, given by, Fid [ρα (r)] = k B T

α

drρα (r) ln 3α ρα (r) − 1

(2.2)

The second term, F ex , describes the hard-sphere excess free energy contribution. As discussed above, there are multiple ways to capture those terms in an approximate fashion, from weighted density approximation [WDA] to fundamental measure theory [FMT]. The third term, F ch , evaluates the effects of connecting hard-spheres into polymeric chains; it is generally based on the Wertheim perturbation scheme [72, 73]. The fourth term, F int , estimates enthalpic contributions to the free energy, e.g., from van-der-Waals forces. Finally, the last term considers the role of external interactions (such as hard walls) via an imposed potential V α (r). To calculate the morphology of the overall system, one needs to minimize the free energy (2.1) with respect to all the densities ρα (r), δ F[ρα (r)] = μα − Vα (r) δρα (r)

(2.3)

The resulting self-consistency equations generally are quite complex and need to be solved numerically in an iterative fashion. In particular, F ex generally is a complex nonlinear and nonlocal functional of the single-particle densities. Thus, the minimization (2.3) leads to fairly complicated integral equations, requiring a fairly fine spatial discretization and leading to slow convergence of the iterative process. For more details on the numerical algorithms used, we refer the readers to papers by Frischknecht and co-workers [61, 62]. We now proceed to the discussion of DFT application to nanocomposites.

2.3 Applications of DFT to PNCs 2.3.1 Polymers and Nanospheres As a first example of the application of DFT to nanocomposites, one can look at the problem of the interaction between hard spheres of radius RP and homopolymers (melt or solution). A simple treatment of this problem for the solution case was proposed in the early 2000s by Schmidt and co-workers [74–77] who used the Asakura-Oosawa (AO) [78, 79] approximation. Within the AO analysis, the polymer chains are treated as impermeable spheres of radius Rg , where Rg is the polymer radius of gyration and depends on the polymer molecular weight and the solvent quality (good or poor) [80]. The AO analysis and subsequent theoretical work [81, 82] famously demonstrated that the colloidal particles experience so-called “depletion

2 Density Functional Theory-Based Modeling …

27

attraction”, as the polymer chains resist confinement in the narrow spaces between the colloidal particles. In the cases where q = Rg /RP < 0.15 (the “colloidal limit” we discussed earlier), the polymeric degrees of freedom can be integrated out to yield an effective pair potential between the colloids. Schmidt and co-workers built on that earlier body of work and developed a new DFT-based approach to calculate phase diagrams of AO mixtures as a function of the size ratio q, the polymer volume fraction, and the colloid volume fraction. The phase diagrams included colloidpoor phase (“Gas”), colloid-rich liquid phase (“Liquid”), and colloidal crystal phase (“Crystal”). Depending on the size ratio q, the demixing can occur either via “Gas– Liquid” or via “Gas–Solid” coexistence. Furthermore, DFT was applied to describe the particle and polymer density profiles at the “Gas–Liquid” interfaces or near a hard wall. The above analysis, while straightforward and accurate in the limit of large nanospheres, is expected to run into difficulties for the cases where q = Rg /RP ~ 1, and representing polymers as simple spheres is no longer tenable. In the 2000s, new approaches have been developed based on polymer DFTs. Some examples are shown in Figs. 2.2 and 2.3. In Fig. 2.2, the density profiles of polymers and nanospheres near a hard wall are plotted as a function of the distance from the wall, as computed by McGarrity, Frischknecht, and Mackay [83, 84]. They considered an athermal mixture (no vander-Waals interactions), used an FMT approach for the excess sphere free energy, and the Tripathy-Chapman association term [85, 86]. The calculations are done for RP = 2 σ, where σ is the monomer Kuhn length; the chain length N = 100. At low particle densities, the polymer expels the particles from the wall (Fig. 2.2a), while at high particle densities, the particles segregate to the surface layer (Fig. 2.2b). Additional complexity can be introduced by adding van-der-Waals interactions and considering block copolymers instead of homopolymers. Cao and Wu [87] modeled a solution of AB diblock copolymers and nanoparticles near a hard wall; the total film thickness was set to 20 σ. The A-block is attractive to the particles, while the B-block is either neutral (Fig. 2.3a, b) or slightly repulsive (Fig. 2.3c, d) to the particles. The calculations show that as the interaction between the particles and the B-block become less favorable, the system undergoes a transition from a “multilayer film” to a “monolayer”. The “multilayer” morphology is likely due to the three-dimensional ordering of the particles into soft colloidal crystals (even though the simulations are one-dimensional); the “monolayer” morphology represents the block copolymer templating, with the particles segregating into the favorable domain. One last example in this section describes the melt of “hairy nanoparticles” or “nanoparticle-organic hybrid materials” (NOHM) [11, 88–94]. Here, DFT was used to compute the transition between the liquid and the face-centered cubic (FCC) solid (Fig. 2.4). We will return to this same system below when discussing the hybrid SCF-DFT technique.

28

V. V. Ginzburg

Fig. 2.2 Polymer/nanoparticle mixture near a hard wall. As the particle density is increased, the layer near the wall changes from polymer-rich to particle-rich. a Particle (black) and polymer (blue) density profiles for the polymer-rich structure; b Same for the particle-rich structure. Reproduced with permission from [83]. Copyright (2009) American Institute of Physics

2.3.2 Polymers and Nanorods Our next example includes rodlike nanoparticles in a polymer melt, as shown in Fig. 2.5, left panel. The nanorods are assumed to have a high aspect ratio and wellaligned. The surfaces of the rods are covered with grafted oligomers of chain length N, and they are immersed in a homopolymer melt with chains of length P. The grafting density σ gr is obviously one important parameter governing the dispersion of the rods; another parameter is the ratio of the free chain length to the grafted chain length, α= P/N. The DFT calculations by Frischknecht, Hore, Composto, and co-workers [95–97] determined the effective interaction potential between the nanorods and evaluated whether it was attractive (leading to the nanorod aggregation) or repulsive (leading to their dispersion). The results are shown in Fig. 2.5, right panel. For the moderate grafting densities, the phase behavior was found to be sensitive to

2 Density Functional Theory-Based Modeling …

29

Fig. 2.3 Self-organization of nanoparticles (with diameter σ P = 4σ ) by short-chain block copolymers consisting of A/B segments (chain length M = 8). a and c give the reduced density profiles of the polymeric segments and of the nanoparticles confined within a thin film of thickness H = 20 s. b and d Visualize the corresponding structures. In (a) and (b), B segments are neutral to the nanoparticles, while in (c) and (d), B segments repel the particles. In both cases, the packing fraction of the polymer in the bulk is 0.01 and that of the particles in the bulk is 0.1. Reproduced with permission from [87]. Copyright (2007) American Institute of Physics

the ratio of the rod radius to the polymer Rg ; for the high grafting densities, this dependence has disappeared. The results were compared with experiments, and a good agreement was found.

2.3.3 Polymers and Nanoplatelets Finally, we consider the case of polymers and nanoplates. Balazs, Ginzburg, and co-workers developed a two-step approach in analyzing the structure and dispersion of such systems. First, polymer self-consistent field theory (SCFT) is used to compute the effective polymer-mediated interaction potential between the platelets

30

V. V. Ginzburg

Fig. 2.4 The DFT-calculated phase diagram for “hairy nanoparticles” with the particle/monomer volume ratio of 106. The Y-axis is the nanoparticle volume fraction, and the X-axis is the ratio of the polymer Rg to the particle radius a. Reproduced with permission from [90]. Copyright (2013) American Chemical Society

Fig. 2.5 Polymer-grafted nanorods in polymer melt. The cartoon on the left shows the schematics, with N being the length of the grafted ligands, and P being the length of the free chains. The phase diagrams on the right show the regions corresponding to rods being aggregated (red) or welldispersed (blue); triangles and squares are experimental data, and circles represent DFT calculations. a High grafting density; b Moderate grafting density. Reproduced with permission from [95]. Copyright (2013) American Chemical Society

[98, 99]. Then, DFT is constructed to model the anisotropic assemblies of oblate ellipsoids with long-range interactions due to the SCFT-calculated potentials [6, 7, 100– 103]. Trial single-particle densities are constructed to model various morphologies (Fig. 2.6). As shown in Fig. 2.7, for nanoplatelets with relatively low aspect ratio D/L = 30, the phase diagram is quite nontrivial and complex. In the example here, the platelets

2 Density Functional Theory-Based Modeling …

31

Fig. 2.6 The morphologies of oblate ellipsoid fluids: a Isotropic (I); b Nematic (N); c Smectic (Sm); d Columnar (Col); e Plastic Solid (“House of Cards”) (PS); f Crystal (Cr). Reproduced with permission from [103]. Copyright (2000) American Chemical Society

32

V. V. Ginzburg

Fig. 2.7 Phase diagrams of polymer–clay mixtures: a ρ gr = 0.04, N gr = 50, and b ρ gr = 0.02, N gr = 100. The platelet diameter D = 30 nm, thickness L = 1 nm. The free chain length P = 300. The Y-axis is the Flory–Huggins interaction parameter between the ligands and the free chains, the X-axis is the platelet volume fraction. Reproduced with permission from [103]. Copyright (2000) American Chemical Society

are modified by grafted ligands, similar to the nanorod example above. When the free chains are attracted to the ligands (χ < 0), the isotropic and plastic solid structures prevail at low filler loadings; eventually, the platelets and polymers arrange into a 3D crystal structure. When the free chains are repelled from the ligands (χ > 0), a wide isotropic-crystal coexistence is observed, indicating aggregation or poor dispersion. Note that in the calculations, we assume that the fillers interact via weak van der Waals attractive forces. As the platelet diameter is increased, the phase diagram becomes simpler. The isotropic, plastic solid, and columnar phases become squeezed to the limit of extremely low concentrations. It should become possible to consider a simpler model

2 Density Functional Theory-Based Modeling …

33

Fig. 2.8 The cartoon on the left shows the schematics, with N g being the length of the grafted ligands, and N f being the length of the free chains. The plot on the right shows the locus of the critical values of α = N f /N g at which the interaction force between the grafted monolayers becomes attractive for fixed bulk-free polymer density, ρ f σ f 3 = 0.6. The chain lengths of the grafted polymers are N g = 101 (squares) and N g = 151 (circles). σ g = σf = σ Reproduced with permission from [105]. Copyright (2009) American Institute of Physics

where the nanoplatelets are well-aligned and ask only whether the effective potential between them is attractive (causing aggregation) or repulsive (causing dispersion). This simplified problem was studied quite extensively (see, e.g., reviews [6, 7, 104]). In one example, Jain et al. [105] used DFT to estimate the interaction potential between two parallel plates in a polymer melt (Fig. 2.8). It was shown that the boundary between the aggregation and dispersion depends strongly on both the grafting density and the ratio of the ligand to free polymer chain lengths, as one indeed can expect. Overall, the use of DFT in predicting nanocomposite morphology has been quite extensive. However, as examples above show, most DFT applications in the nanocomposite field either utilize the “colloidal approximation” (integrating out the polymeric degrees of freedom) or are restricted to lower-dimensionality morphologies (usually 1D, sometimes 2D) and/or shorter polymers. This is because all polymeric DFTs are still computationally expensive. In the next section, we discuss a simplified approach that aims to reduce the computation time and enable the calculation of more complex morphologies.

2.4 The SCF-DFT Approach The hybrid Self-Consistent Field/Density Functional Theory (SCF-DFT) method was originally proposed by Thompson, Ginzburg, Matsen, and Balazs [106, 107] to

34

V. V. Ginzburg

describe the bulk morphologies of mixtures of nanospheres and diblock copolymers. It was subsequently used by many other investigators and applied to various problems, some of which are highlighted below. So far, the method is restricted to the case where the particles are nanospheres, though extensions to other shapes (e.g., oblate or prolate ellipsoids) should be reasonably straightforward. The starting point for the SCF-DFT approach is the SCFT of polymers (see books and reviews [108–111] for more details). Within SCFT, polymers are treated as Gaussian chains and the interaction between various monomers is local and captured by the Flory-Huggins lattice model [112–114]. The spherical nanofillers occupy multiple lattice sites; to describe their interactions, one needs to utilize a DFT description that captures long-ranged excluded volume effects. The SCF-DFT free energy for a mixture of a multicomponent polymer blend with a single nanosphere type is written as, ψj Q j F Nv =− ln kB T V αj ψjV j ⎡

1 1 + dr⎣ (χ N )αβ {ϕα (r) − φα } ϕβ (r) − φβ V 2 α,β −ξ (r) 1 − ϕα (r) 1 − V +

1 V

α

dr w P (r)ρ P (r) +

wα (r)ϕα (r)

α

dr ρ P (r) H S ϕ P (r)

(2.4)

Here, V is the total volume, T is temperature, N is the chain length of the first (reference) polymer chain, ψ j is the volume fraction of the j-th component, Qj is the partition function of the j-th component, and α j is the volume ratio of the j-th component and the first (reference) component. In addition, ϕ α (r) is the positiondependent volume fraction of the α-th chemical species, φ α is the overall volume fraction of the α-th chemical species, and wα (r) is the conjugate field. Finally, ξ (r) is the pressure-like field, and the matrix (χ N)αβ describes all the pairwise Flory– Huggins interactions. For the particles, one uses the DFT-like description based on the center probability distribution, ρ P (r), from which the position-dependent volume fraction is then computed via, ϕ P (r) =

1 Nv

dr ρ P r R P − r − r

(2.5)

2 Density Functional Theory-Based Modeling …

35

Here, is the standard Heaviside function. Also, consistent with DFT for hard spheres, one estimates the excess non-ideal free energy using a WeightedDensity Approximation (WDA) [27]. The Carnahan-Starling [115] excess term and a weighted density function are utilized, H S (x) = 1 ϕ P (r) = 3 2 Nv

4x − 3x 2 (1 − x)2

(2.6)

2 dr ρ P r + r w0 r + w1 r ρ P r + w2 r ρ P r (2.7)

For simplicity, in the expansion (2.7), w1 and w2 are both set to zero, and w0 (r) = (2R P − |r|). Lastly, the partition functions for the particles and the polymers are given by, QP =

dr exp[−w P (r)]

Q j= P =

drq r, α j

(2.8a) (2.8b)

In (2.8b), the propagator q is evaluated in a standard SCFT fashion [106–111]. The free energy (2.4) needs to be minimized with respect to densities, conjugate fields, and pressure; the resulting equations are solved iteratively. The solutions would then describe the morphologies of nanocomposites, including the distribution of nanoparticles within various polymer domains.

2.4.1 Nanoparticles in Block Copolymers—Bulk and Films Historically, the first example of SCF-DFT was the case where spherical nanoparticles were admixed with an AB-diblock copolymer; the nanoparticles were assumed to be strongly preferential to the A-block. Figure 2.9 shows the density profiles and particle center distributions for the lamellar morphology [106]. The model shows that the particles segregate into the A-lamellae; furthermore, larger particles prefer to be located at the center of the lamella (Fig. 2.9a, b), while the smaller ones tend to push closer to the edges (Fig. 2.9c). This result agrees qualitatively with experimental data of Bockstaller et al. [116] and other authors [117–120]. Similar particle segregation was calculated for other morphologies (cylindrical and spherical) [107]. Subsequent work by Balazs and co-workers discussed the influence of mixed spheres, as well as the behavior of the block copolymer/particle system in thin films [121–128]. It was shown, in particular, that under some conditions, the particles can segregate towards the surfaces and provide “self-healing” effect.

36

V. V. Ginzburg

Fig. 2.9 Concentration profiles of diblock-particle systems [ϕ A (x), density distribution of A blocks; ϕ P (x), and ρ P (x), distributions of particles and particle centers, respectively]. a Large particle (RP = 0.74Rg ), particle volume fraction φ P = 0.15. b Large particle (RP = 0.74Rg ), φ P = 0.03. c Small particle (RP = 0.5Rg ), φ P = 0.15. B blocks are not depicted. Three periods are shown to better illustrate the morphologies. Sketches showing the structure of each system accompany the profiles. Reproduced with permission from [106]. Copyright (2001) American Association for Advancement of Science

2.4.2 “Giant Surfactants”—Single-Ligand Nanoparticles The above theory was formulated assuming that the fillers were “hard spheres”. In reality, however, many nanoparticles have oligomeric ligands grafted to their surfaces (“giant surfactants” [19, 129–131], and the theory needs to take this effect into account. One of the first examples of the SCF-DFT extension to account for the effects of grafting was the study by Lee et al. [127], in which they calculated phases of the amphiphilic “tadpole” sphere-coil copolymers. It was shown that the spheres can organize into hexagonal closed-pack lattice, with polymers filling the spaces between them. This analysis was later refined and extended by other authors [132]. Similar arrangements were subsequently observed in Brownian Dynamics and other particle-based simulations [18, 20, 133]. Several recent studies utilized SCF-DFT to predict the morphology and phase behavior of single- or double-tethered nanoparticles with block-copolymer (rather than homopolymer) ligand [134–136]. In one example, Wang and co-workers investigated the phase behavior of ABP, APB, and PAB triblocks, where A and B are flexible chains, and P is a nanoparticle; the A-block is favorable to the particles. Figure 2.10 shows the calculated phase diagrams, based on 2D SCF-DFT simulations. The Y-axis is the strength of attraction between the A-block and the P-particle, and the X-axis is the A-block volume fraction. It can be seen that the morphology and the phase behavior are sensitive to the particle placement relative to the A-block.

2 Density Functional Theory-Based Modeling …

37

Fig. 2.10 a 2D ordered structures self-assembled by various giant surfactants: (Top) hexagonally packed cylinders formed by mixed A block and nanoparticles (NP) (C mix ); (Middle) parallel lamellae formed by mixed A block and NP and pure B block (LAM); (Bottom) hexagonally packed cylinders formed by pure B block (C B ). The orange color denotes the regions formed by mixed A block and NP, and the blue color denotes the regions formed by pure B block. b Phase diagrams for (Top) ABP, (Middle) APB, and (Bottom) BAP giant surfactants as a function of the chain length ratio of A block (f A ) and the interaction parameter between A block and NP (−χAP N). Reproduced with permission from [137]. Copyright (2019) American Chemical Society

38

V. V. Ginzburg

2.4.3 “Hairy Nanoparticles”—Single-Component Assemblies and Mixtures with Polymers The last example we consider is related to the application of SCF-DFT to polymergrafted or “hairy” nanoparticles (PGNP or HNP) [11, 17, 137]. This topic was briefly discussed in Sect. 3.1 when we described the use of DFT to estimate the liquid-tocrystal transition in bulk one-component HNP assemblies. We now highlight the use of SCF-DFT in understanding these systems. In 2009, Akcora and co-workers [138] experimentally investigated the dispersions of polystyrene (PS)-grafted silica-NP in PS matrix. As expected, they observed some cases where the particles were well-dispersed (long ligands) and some cases where the particles were aggregated (short ligands), in agreement with earlier theories [12, 21, 22, 139–141]. Surprisingly, under some conditions, the particles would form two-dimensional arrays (“sheets”) and one-dimensional chains (“strings”). Coarsegrained Monte Carlo simulations and analytical strong-segregation theory modeling [138, 142] successfully explained those morphologies for the case of nanocomposites with low NP loading; the combined modeling and experimental insights were summarized by Kumar and co-workers in their 2013 Macromolecules paper [17]. The reason for the anisotropic assembly was that the polymer shell (“canopy”) did not have to remain spherical; under some conditions, the HNPs could reduce their free energy by re-arranging the ligands and making their surfaces somewhat “patchy”; the particles would then be able to minimize the free energy further by “fusing” the “bald” patches together. In an SCF-DFT study, Ginzburg [143] investigated the formation of sheets, strings, and aggregates at different NP volume fractions and for different ligand lengths and grafting densities. In the HNP-homopolymer binary mixtures, the anisotropic assembly was caused by the interaction between the matrix and the ligands. Are the anisotropic morphologies going to be present if there is no matrix? The DFT analysis was discussed in Sect. 3.1 included only two phases—uniform liquid and face-centered cubic (FCC) crystal. However, Koerner et al. [144], Bockstaller et al. [145], and other authors demonstrated the formation of anisotropic structures in thin films of one-component HNPs under conditions of “moderate” and “sparse” grafting. To describe the phase behavior of these systems, Ginzburg [146] applied a slightly modified version of SCF-DFT; the results are shown in Figs. 2.11 and 2.12. The phase map in Fig. 2.11 shows the equilibrium morphologies for onecomponent nanocomposites having the core radius RP = 3.05 nm as the grafting density and the grafted chain length is varied. The structures predicted in simulations include FCC crystal and isotropic liquid, but also lamellar (sheets) and cylindrical (strings) morphologies. It was further hypothesized that the phase map can be replotted in scaled coordinates, RP /Rg and ϕ P (Fig. 2.12), and a reasonable agreement with experiments was obtained, although more studies are needed.

2 Density Functional Theory-Based Modeling …

39

Fig. 2.11 Phase map for the HNP melt. Here, N is ligand length and σ is grafting density. Symbols represent simulation results, with equilibrium (minimum free energy) morphologies shown as follows: yellow = lamellar, gray = sheets, orange = cylindrical, and blue = FCC spherical. Dashed lines are boundaries of the region studied in these simulations, while solid lines are approximate locations of transitions between various phases. Reproduced with permission from [147]. Copyright (2017) American Chemical Society

2.5 Summary and Outlook Density functional theory (DFT) is a powerful technique to study the phase behavior of complex fluids. Over the past four decades, DFT has been extensively parameterized for various systems, from hard spheres to Lennard–Jones spheres to hard ellipsoids and spherocylinders to flexible polymer chains. In particular, DFT is generally well-suited to model the behavior of a mixture comprised of hard spheres of different sizes; one can then combine one or more sphere types into polymer chains via the Wertheim perturbation procedure. At the same time, numerical solution of the DFT equations often remains challenging due to long-range nature of the non-ideal free energy terms in either WDA or FMT approximations; thus, most DFT examples for nanocomposites so far have been describing either 1D or 2D structures. Hybrid field-theory approaches, such as SCF-DFT, can often accelerate the calculations and allow for fast exploration of phase maps and various morphologies. The use of SCFT instead of DFT for polymer components neglects some intermolecular correlations but significantly increases the computation speed. Under some conditions, the use of compressible SCFT [104, 105, 148] can help improve the agreement with experiment and/or approximate the DFT results. The SCF-DFT approach, as originally formulated by Thompson et al. [106, 107], and subsequently refined and extended by other authors [127, 136, 146, 149], enables fast and straightforward

40

V. V. Ginzburg

Fig. 2.12 Phase map of the HNP one-component systems expressed in terms of ϕ P and RP /Rg . Symbols are labeled as in Fig. 2.11. Solid lines are guided to the eye depicting approximate phase boundaries. Stars with numbers represent the phase map locations of HNP systems from [144] and [147] (see text for more details). The dashed blue line is the predicted FCC melting transition. Reproduced with permission from [147]. Copyright (2017) American Chemical Society

calculation of the phase behavior for variety of nanocomposite systems (“bald” and “hairy” nanoparticles in homopolymers, homopolymer blends, and block copolymers; melts or solutions; bulk or thin films). It is feasible to suggest that in the future, SCF-DFT can be used for molecular design of nanocomposites in the same way as today, SCFT is used for molecular design of pure block copolymers [109, 150–154]. Acknowledgements I am thankful to Dow for supporting this work and gratefully acknowledge Drs. Jeffrey Weinhold and Jian Yang for helpful discussions.

References 1. 2. 3. 4. 5.

Q. Zeng, A. Yu, G. Lu, Prog. Polym. Sci. 33, 191 (2008) L.-T. Yan, X.-M. Xie, Prog. Polym. Sci. 38, 369 (2013) J. Yan, M. R. Bockstaller, K. Matyjaszewski, Progr. Polym. Sci., 101180 (2019) G. Allegra, G. Raos, M. Vacatello, Prog. Polym. Sci. 33, 683 (2008) V. V. Ginzburg, in Problems of Nonlinear Mechanics and Physics of Materials (Springer, 2019), p. 205. 6. A. C. Balazs, J. Bicerano, V. V. Ginzburg, in Polyolefin Composites (Wiley, 2007), p. 415. 7. A.C. Balazs, V.V. Ginzburg, Y. Lyatskaya, C. Singh, E. Zhulina, in Polymer-Clay Nanocomposites. ed. by T. Pinnavaia, G.W. Beall (Wiley, New York, 2000), p. 281 8. A. Karatrantos, N. Clarke, M. Kröger, Polym. Rev. 56, 385 (2016)

2 Density Functional Theory-Based Modeling … 9. 10. 11. 12. 13. 14. 15. 16. 17. 18. 19. 20. 21. 22. 23. 24. 25. 26. 27. 28. 29. 30. 31. 32. 33. 34. 35. 36. 37. 38. 39. 40. 41. 42. 43. 44. 45. 46. 47. 48. 49. 50. 51. 52. 53. 54. 55. 56. 57. 58. 59. 60.

41

J.J. de Pablo, Annu Rev Phys Chem 62, 555 (2011) J. Feng, H. Heinz, Adv. Polyolefin Nanocompos., 205 (2010) N.J. Fernandes, H. Koerner, E.P. Giannelis, R.A. Vaia, MRS Commun. 3, 13 (2013) V. Ganesan, A. Jayaraman, Soft Matter 10, 13 (2014) S.C. Glotzer, M.J. Solomon, Nat. Mater. 6, 557 (2007) H. Heinz, S.S. Patnaik, R.B. Pandey, B.L. Farmer, Modeli. Simul. Polym., 37 (2010). S.K. Kumar, B.C. Benicewicz, R.A. Vaia, K.I. Winey, Macromolecules 50, 714 (2017) S.K. Kumar, V. Ganesan, R.A. Riggleman, J. Chem. Phys. 147, 020901 (2017) S.K. Kumar, N. Jouault, B. Benicewicz, T. Neely, Macromolecules 46, 3199 (2013) R.L. Marson, T.D. Nguyen, S.C. Glotzer, MRS Commun. 5, 397 (2015) W.-B. Zhang et al., Macromolecules 47, 1221 (2014) Z.L. Zhang, M.A. Horsch, M.H. Lamm, S.C. Glotzer, Nano Lett 3, 1341 (2003) A. Jayaraman, in Theory and Modeling of Polymer Nanocomposites, ed. by V. Ginzburg, L. Hall (Springer, 2020) L.M. Hall, A. Jayaraman, K.S. Schweizer, Curr. Opin. Solid State Mater. Sci. 14, 38 (2010) P. Hohenberg, W. Kohn, Phys. Rev. 136, B864 (1964) W. Kohn, L.J. Sham, Phys. Rev. 140, A1133 (1965) W. Kohn, Rev. Mod. Phys. 71, 1253 (1999) T. Ramakrishnan, M. Yussouff, Phys. Rev. B 19, 2775 (1979) P. Tarazona, Phys. Rev. A 31, 2672 (1985) P. Tarazona, L. Vicente, Mol. Phys. 56, 557 (1985) W. Curtin, N. Ashcroft, Phys. Rev. A 32, 2909 (1985) A. Denton, N. Ashcroft, Phys. Rev. A 39, 4701 (1989) R. Leidl, H. Wagner, J. Chem. Phys. 98, 4142 (1993) J.F. Lutsko, M. Baus, Phys. Rev. A 41, 6647 (1990) J.F. Lutsko, M. Baus, Phys. Rev. Lett. 64, 761 (1990) Y. Rosenfeld, Phys. Rev. E 50, R3318 (1994) Y. Rosenfeld, J. Phys.: Condens. Matter 8, 9289 (1996) Y. Rosenfeld, M. Schmidt, H. Löwen, P. Tarazona, Phys. Rev. E 55, 4245 (1997) Y. Rosenfeld, P. Tarazona, Mol. Phys. 95, 141 (1998) Y. Rosenfeld, J. Phys.: Condens. Matter 14, 9141 (2002) P. Tarazona, Phys. A 306, 243 (2002) P. Tarazona, J.A. Cuesta, Y. Martínez-Ratón, in Theory and Simulation of Hard-Sphere Fluids and Related Systems (Springer, 2008), pp. 247. M. Baus, J.F. Lutsko, Phys. A 176, 28 (1991) A. Somoza, P. Tarazona, J. Chem. Phys. 91, 517 (1989) A. Somoza, P. Tarazona, Phys. Rev. A 41, 965 (1990) E. Velasco, A. Somoza, L. Mederos, J. Chem. Phys. 102, 8107 (1995) E. Velasco, L. Mederos, J. Chem. Phys. 109, 2361 (1998) E. Velasco, L. Mederos, D. Sullivan, Phys. Rev. E 62, 3708 (2000) E. Velasco, L. Mederos, D. Sullivan, Phys. Rev. E 66, 021708 (2002) G.J. Vroege, H.N. Lekkerkerker, Rep. Prog. Phys. 55, 1241 (1992) V.V. Ginzburg, M.A. Glaser, N.A. Clark, Liq. Cryst. 23, 227 (1997) H. Graf, H. Löwen, J. Phys.: Condens. Matter 11, 1435 (1999) A. Yethiraj, C.E. Woodward, J. Chem. Phys. 102, 5499 (1995) A. Yethiraj, J. Chem. Phys. 109, 3269 (1998) C.E. Woodward, J. Chem. Phys. 94, 3183 (1991) C.E. Woodward, A. Yethiraj, J. Chem. Phys. 100, 3181 (1994) D. Chandler, J.D. McCoy, S.J. Singer, J. Chem. Phys. 85, 5971 (1986) D. Chandler, J.D. McCoy, S.J. Singer, J. Chem. Phys. 85, 5977 (1986) E. Kierlik, M. Rosinberg, J. Chem. Phys. 97, 9222 (1992) E. Kierlik, M. Rosinberg, J. Chem. Phys. 99, 3950 (1993) S.K. Nath, P.F. Nealey, J.J. de Pablo, J. Chem. Phys. 110, 7483 (1999) J.B. Hooper, J.D. McCoy, J.G. Curro, J. Chem. Phys. 112, 3090 (2000)

42

V. V. Ginzburg

61. L. Frink, A. Salinger, M. Sears, J. Weinhold, A. Frischknecht, J. Phys.: Condens. Matter 14, 12167 (2002) 62. A.L. Frischknecht, J.D. Weinhold, A.G. Salinger, J.G. Curro, L.J. Douglas Frink, J.D. McCoy, J. Chem. Phys. 117, 10385 (2002). 63. J. Wu, AIChE J. 52, 1169 (2006) 64. C.P. Emborsky, Z. Feng, K.R. Cox, W.G. Chapman, Fluid Phase Equilib. 306, 15 (2011) 65. J.D. McCoy, K.G. Honnell, K.S. Schweizer, J.G. Curro, J. Chem. Phys. 95, 9348 (1991) 66. J.D. McCoy, K.G. Honnell, K.S. Schweizer, J.G. Curro, Chem. Phys. Lett. 179, 374 (1991) 67. N. Sushko, P. van der Schoot, M. Michels, J. Chem. Phys. 115, 7744 (2001) 68. T. Cherepanova, A. Stekolnikov, Chem. Phys. 154, 41 (1991) 69. J.B. Hooper, J.D. McCoy, J.G. Curro, F. van Swol, J. Chem. Phys. 113, 2021 (2000) 70. A. Yethiraj, Adv. Chem. Phys. 121, 89 (2002) 71. X. Xu, D. Cao, J. Wu, Soft Matter 6, 4631 (2010) 72. M. Wertheim, J. Stat. Phys. 35, 19 (1984) 73. M. Wertheim, J. Stat. Phys. 35, 35 (1984) 74. M. Schmidt, H. Löwen, J.M. Brader, R. Evans, Phys. Rev. Lett. 85, 1934 (2000) 75. J. Brader, R. Evans, M. Schmidt, H. Löwen, J. Phys.: Condens. Matter 14, L1 (2001) 76. R. Evans, J. Brader, R. Roth, M. Dijkstra, M. Schmidt, H. Löwen, Philos. Trans. R. Soc. Lond. Ser. A: Math. Phys. Eng. Sci. 359, 961 (2001) 77. J.M. Brader, R. Evans, M. Schmidt, Mol. Phys. 101, 3349 (2003) 78. S. Asakura, F. Oosawa, J. Chem. Phys. 22, 1255 (1954) 79. S. Asakura, F. Oosawa, J. Polym. Sci., A: Polym. Chem. 33, 183 (1958) 80. M. Rubinstein, R. H. Colby, Polymer Physics, vol. 23 (Oxford University Press, New York, 2003) 81. A. Gast, C. Hall, W. Russel, J. Colloid Interface Sci. 96, 251 (1983) 82. H.N. Lekkerkerker, W.-K. Poon, P.N. Pusey, A. Stroobants, P. Warren, EPL (Europhys. Lett.) 20, 559 (1992) 83. E. McGarrity, A. Frischknecht, M. Mackay, J. Chem. Phys. 128, 154904 (2008) 84. E. McGarrity, A. Frischknecht, L. Frink, M. Mackay, Phys. Rev. Lett. 99, 238302 (2007) 85. S. Tripathi, W.G. Chapman, J. Chem. Phys. 122, 094506 (2005) 86. S. Tripathi, W.G. Chapman, Phys. Rev. Lett. 94, 087801 (2005) 87. D. Cao, J. Wu, J. Chem. Phys. 126, 144912 (2007) 88. H.-Y. Yu, D.L. Koch, Langmuir 26, 16801 (2010) 89. A. Chremos, A.Z. Panagiotopoulos, H.-Y. Yu, D.L. Koch, J. Chem. Phys. 135, 114901 (2011) 90. H.-Y. Yu, D.L. Koch, Langmuir 29, 8197 (2013) 91. H.-Y. Yu, S. Srivastava, L.A. Archer, D.L. Koch, Soft Matter 10, 9120 (2014) 92. A.B. Bourlinos, R. Herrera, N. Chalkias, D.D. Jiang, Q. Zhang, L.A. Archer, E.P. Giannelis, Adv. Mater. 17, 234 (2005) 93. A.B. Bourlinos, S. Ray Chowdhury, R. Herrera, D.D. Jiang, Q. Zhang, L.A. Archer, E.P. Giannelis, Adv. Funct. Mater. 15, 1285 (2005). 94. S. Srivastava, P. Agarwal, L.A. Archer, Langmuir 28, 6276 (2012) 95. A.L. Frischknecht, M.J. Hore, J. Ford, R.J. Composto, Macromolecules 46, 2856 (2013) 96. A.L. Frischknecht, J. Chem. Phys. 128, 224902 (2008) 97. M.J.A. Hore, R.J. Composto, Macromolecules 47, 875 (2014) 98. A.C. Balazs, C. Singh, E. Zhulina, Macromolecules 31, 8370 (1998) 99. A.C. Balazs, C. Singh, E. Zhulina, Y. Lyatskaya, Accounts Chem. Res. 32, 651 (1999) 100. Y. Lyatskaya, A.C. Balazs, Macromolecules 31, 6676 (1998) 101. V.V. Ginzburg, A.C. Balazs, Macromolecules 32, 5681 (1999) 102. V. Ginzburg, A. Balazs, Adv. Mater. 12, 1805 (2000) 103. V.V. Ginzburg, C. Singh, A.C. Balazs, Macromolecules 33, 1089 (2000) 104. P.K. Jog, V.V. Ginzburg, R. Srivastava, J.D. Weinhold, S. Jain, W.G. Chapman, in Advances in Chemical Engineering (Elsevier, 2010), p. 131 105. S. Jain, V.V. Ginzburg, P. Jog, J. Weinhold, R. Srivastava, W.G. Chapman, J. Chem. Phys. 131, 044908 (2009)

2 Density Functional Theory-Based Modeling …

43

106. R.B. Thompson, V.V. Ginzburg, M.W. Matsen, A.C. Balazs, Science 292, 2469 (2001) 107. R.B. Thompson, V.V. Ginzburg, M.W. Matsen, A.C. Balazs, Macromolecules 35, 1060 (2002) 108. G. Fredrickson, The Equilibrium Theory of Inhomogeneous Polymers (Oxford University Press, 2006) 109. M.W. Matsen, F.S. Bates, Macromolecules 29, 1091 (1996) 110. A.C. Shi, in Developments in Block Copolymer Science and Technology, ed. by I.W. Hamley (Wiley-VCH, Weinheim, 2004) 111. F. Schmid, J Phys-Condens Mat 10, 8105 (1998) 112. S.F. Edwards, Proc. Phys. Soc. 85, 613 (1965) 113. P.J. Flory, J. Chem. Phys. 9, 660 (1941) 114. M.L. Huggins, J. Chem. Phys. 9, 440 (1941) 115. N.F. Carnahan, K.E. Starling, J. Chem. Phys. 51, 635 (1969) 116. M.R. Bockstaller, Y. Lapetnikov, S. Margel, E.L. Thomas, J. Am. Chem. Soc. 125, 5276 (2003) 117. B.J. Kim, J.J. Chiu, L. Bang, C.J. Hawker, D.J. Pine, E.J. Kramer, Abstr. Pap. Am. Chem. S. 230, U1066 (2005) 118. B.J. Kim, J.J. Chiu, G.R. Yi, D.J. Pine, E.J. Kramer, Adv. Mater. 17, 2618 (2005) 119. B.J. Kim, G.H. Fredrickson, C.J. Hawker, E.J. Kramer, Langmuir 23, 7804 (2007) 120. B.J. Kim, G.H. Fredrickson, E.J. Kramer, Macromolecules 41, 436 (2008) 121. J.Y. Lee, R.B. Thompson, D. Jasnow, A.C. Balazs, Macromolecules 35, 4855 (2002) 122. J.-Y. Lee, R.B. Thompson, D. Jasnow, A.C. Balazs, Phys. Rev. Lett. 89, 155503 (2002) 123. R.B. Thompson, J.Y. Lee, D. Jasnow, A.C. Balazs, Phys. Rev. E 66, 031801 (2002) 124. G.A. Buxton, J.Y. Lee, A.C. Balazs, Macromolecules 36, 9631 (2003) 125. J. Y. Lee, Z. Shou, and A. C. Balazs, Phys. Rev. Lett. 91 (2003) 126. J.Y. Lee, Z.Y. Shou, A.C. Balazs, Macromolecules 36, 7730 (2003) 127. J.Y. Lee, A.C. Balazs, R.B. Thompson, R.M. Hill, Macromolecules 37, 3536 (2004) 128. S. Tyagi, J.Y. Lee, G.A. Buxton, A.C. Balazs, Macromolecules 37, 9160 (2004) 129. X. Yu et al., Proc. Natl. Acad. Sci. 110, 10078 (2013) 130. B. Ni, X.-H. Dong, Z. Chen, Z. Lin, Y. Li, M. Huang, Q. Fu, S.Z. Cheng, W.-B. Zhang, Polym. Chem. 5, 3588 (2014) 131. W. Zhang, Y. Liu, J. Huang, T. Liu, W. Xu, S. Cheng, X. Dong, Soft Matter 15, 7108 (2019) 132. T. Zhang, C. Fu, Y. Yang, F. Qiu, J. Chem. Phys. 146, 054902 (2017) 133. S.C. Glotzer, M.A. Horsch, C.R. Iacovella, Z. Zhang, E.R. Chan, X. Zhang, Curr. Opin. Colloid in 10, 287 (2005) 134. B. Zhang, X. Ye, B.J. Edwards, J. Chem. Phys. 139, 244909 (2013) 135. T. Zhang, C. Fu, Y. Yang, F. Qiu, Macromolecules 51, 1654 (2018) 136. Y. Wang, J. Cui, Y. Han, W. Jiang, Langmuir 35, 468 (2019) 137. M.G. Moffitt, J. Phys. Chem. Lett. 4, 3654 (2013) 138. P. Akcora et al., Nat. Mater. 8, 354 (2009) 139. I. Borukhov, L. Leibler, Macromolecules 35, 5171 (2002) 140. A. Jayaraman, J. Polym. Sci. B: Polym. Phys. 51, 524 (2013) 141. V. Ganesan, C.J. Ellison, V. Pryamitsyn, Soft Matter 6, 4010 (2010) 142. V. Pryamtisyn, V. Ganesan, A.Z. Panagiotopoulos, H. Liu, S.K. Kumar, J. Chem. Phys. 131, 221102 (2009) 143. V.V. Ginzburg, Macromolecules 46, 9798 (2013) 144. H. Koerner, L. Drummy, B. Benicewicz, L. Yu, R. Vaia, Acs Macro Lett. 2, 670 (2013) 145. J. Lee, Z. Wang, J. Zhang, J. Yan, T. Deng, Y. Zhao, K. Matyjaszewski, M.R. Bockstaller, Macromolecules (2020) 146. V.V. Ginzburg, Macromolecules 50, 9445 (2017) 147. V. Goel, J. Pietrasik, H.C. Dong, J. Sharma, K. Matyjaszewski, R. Krishnamoorti, Macromolecules 44, 8129 (2011) 148. K. Hong, J. Noolandi, Macromolecules 14, 1229 (1981) 149. K. Chen, H.-S. Li, B.-K. Zhang, J. Li, W.-D. Tian, Sci. Rep.-Uk 6, 20355 (2016)

44

V. V. Ginzburg

150. G. Fredrickson, The Equilibrium Theory of Inhomogeneous Polymers, vol. 134 (Oxford University Press on Demand, 2006) 151. V. Ginzburg, J. Weinhold, P. Hustad, P. Trefonas, B. Kim, N. Laachi, and G. Fredrickson, in Directed Self-assembly of Block Co-polymers for Nano-manufacturing (Elsevier, 2015), p. 67 152. A. Arora, D.C. Morse, F.S. Bates, K.D. Dorfman, J. Chem. Phys. 146, 244902 (2017) 153. A. Arora, J. Qin, D.C. Morse, K.T. Delaney, G.H. Fredrickson, F.S. Bates, K.D. Dorfman, Macromolecules 49, 4675 (2016) 154. F.S. Bates, G.H. Fredrickson, Phys. Today 52, 32 (1999)

Chapter 3

Coarse-Grained Modeling of Polymer Nanocomposites: Field-Theoretic Simulations Jason P. Koski, Huikuan Chao, Christian Tabedzki, and Robert A. Riggleman

Abstract For several decades polymer field theory has been an important computational and theoretical tool for predicting and interpreting the phase behavior of polymers. Many emerging applications of polymer materials involve blending polymers with nanoparticles to improve performance; however, the thermodynamics of these systems remains relatively poorly understood. In this chapter, we summarize numerous recent advances in polymer field theory with a focus on our approach to extend polymer field theory to describe polymer nanocomposites. We discuss recent applications of the methods as well as the mutual advantages and disadvantages of various implementations and conclude with a discussion of the challenges and ongoing development of the methods.

3.1 Introduction One of the intrinsic challenges with modeling of polymer nanocomposites is the inherent multiple length scales involved with the materials, and phenomena on each length scale can affect the resulting properties [1–3]. On the most local level, one must consider the Coulombic, van der Waals, and in some cases Hydrogen-bonding interactions between all species; on the polymer segmental level, packing effects begin to come into play. On yet larger length scales, polymer conformations and J. P. Koski Sandia National Laboratories, P.O. Box 5800, Albuquerque, NM 87185, USA e-mail: [email protected] H. Chao Core Research and Development,The Dow Chemical Company, Midland, USA e-mail: [email protected] C. Tabedzki · R. A. Riggleman (B) Chemical and Biomolecular Engineering,University of Pennsylvania, Philadelphia, USA e-mail: [email protected] C. Tabedzki e-mail: [email protected] © Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1_3

45

46

J. P. Koski et al.

nanoparticle sizes and shapes exist, and finally on the largest scales one must account for the bulk structure of the composite, which could in general involve multiple phases coexisting. While there are established strategies for capturing the behavior on relatively small ( 20 nm) and continuum mechanics works well on the largest length scales, only a handful of approaches are able to predict the structure and phase behavior of composites on larger, mesoscale length scales. In addition to molecular simulations, two other statistical mechanical approaches are commonly used: polymer reference interaction site model (PRISM) theory and field-theoretic approaches, the latter of which is the primary subject of this chapter. As PRISM theory and background of this approach has been nicely reviewed recently by Martin et al. [4], the details of the theory will only be presented at a high level here in order to focus on the results generated for polymer nanocomposites. Briefly, a set of nonlinear matrix integral equations that are based on the microscopic interactions are employed to calculate the thermodynamic properties of the fluid of interest, and typically the focus is on the static structure factor between the various components, S(k). A challenge of standard PRISM theory is the apparent difficulty in incorporating densely grafted nanoparticles into the theory, although the hybrid MonteCarlo/PRISM theory approach of Jayaraman et al. provides an elegant solution to this issue [5, 6]. PRISM theory has played an instrumental role in developing theoretical phase diagrams for polymer nanocomposites [7, 8]. Separately, polymer field theory has a rich history that gives it some advantages over other approaches. From the early work of Edwards showing that one can estimate the statistics of Gaussian polymer chains with excluded volume interactions [9] to ubiquitous application to various block copolymer structures [10–15], field theory has a record of generally agreeing well with experiments. Experimental strategies for estimating the parameters of common versions of the theory are well-established and tabulated, and the theory lends itself to both analytic and numerical analysis, depending on the level of approximations employed [10]. Numerical implementations of field theory as either field-theoretic simulations (FTS) or as self-consistent field theory (SCFT) also allow the study of inhomogeneous (phase separated) states. Two primary strategies have emerged for the study of polymer nanocomposites using field-theoretic simulations. First among them was the seminal work by Thompson et al. [16] combining density functional theory with self-consistent field theory (SCFT/DFT) to predict the distribution of nanoparticles in block copolymer matrices. This method has been employed in a variety of applications with great success at capturing the behaviors observed in experiments [17, 18]. As this method is discussed at length in Chap. 2 of this text, we will not focus on an extended discussion of this approach. Rather, we focus on the hybrid particle/field theory, wherein explicit nanoparticles are retained in the partition function describing the system [19], and its subsequent generalization by many of us [20]. In this chapter, we present a detailed derivation and discussion of the extensions of polymer field theory that allow for the inclusion of excluded volume correlations (see Fig. 3.1) and the associated study of polymer nanocomposites using field-based simulations. To most clearly demonstrate the extensions of conventional methods, we first present a standard field theory derivation of a compressible diblock melt

3 Coarse-Grained Modeling of Polymer Nanocomposites …

47

Fig. 3.1 Segment density near a polymer wall for the standard field theory using delta function densities and for the theory using finite-sized segments. The latter gives rise to liquid-like layering near the wall

blended with a homopolymer. Here, we demonstrate the particle-to-field transformation and derive the corresponding density operators for the polymer chains. Second, we present the framework developed by Sides and coworkers [19] to include explicit particles and establish a hybrid particle-field theory (HPFT) technique used to study polymer nanocomposites. We then present extensions of these frameworks to include field-based nanoparticles that allow for rapid calculation of nanoparticle density distributions in bulk systems while also providing a method to trivially include field fluctuations through complex Langevin (CL) simulations. These extensions include field-based nanospheres, nanorods, simple grafted nanoparticles (homopolymer grafting), complex grafted nanoparticles (diblock, mixed, and Janus grafting), and the incorporation of advanced pair-potentials in a field-based formulation. Next, we provide a non-equilibrium dynamic mean-field theory that goes beyond the aforementioned equilibrium methods and allows the integration and study of dynamic processes. Finally, we present a short section on the numerical implementation of the various methods and highlight some recent results obtained using the methods presented herein before concluding by summarizing areas for future development and outstanding challenges.

3.2 Standard Field Theory—Compressible Diblock with Homopolymer We first present a standard field theory formalism of a compressible diblock copolymer melt with homopolymer. The polymers are modeled as discrete Gaussian chains with ND and NH segments for the diblock and homopolymer chains, respectively. Here, ND = NA + NB where NA and NB are the number of segments in the A and B block of the copolymer, respectively. The microscopic density of the diblock copolymer is given by

48

J. P. Koski et al.

ρˆK (r) =

nD NK i

δ(r − ri,j ),

(3.1)

j

where nD is the number of diblock chains and K denotes either the A or B block. The homopolymer microscopic density is given by ρˆH (r) =

nH NH i

δ(r − ri,j ),

(3.2)

j

where nH is the number of homopolymer chains. The polymer chains are connected via a Gaussian bonding potential nT N T −1 3|ri,j − ri,j+1 |2

βU0 =

i

2b2

j

,

(3.3)

where b is the statistical segment length of the polymer and T is either D or H to denote the type of polymer chain. Here, we assume that bA = bB = bH = b. A Helfand compressibility [21] potential is used to enforce an energetic penalty for deviations away from the total system density, ρ0 , given by κ βU1 = 2ρ0

d r [ρˆ+ (r) − ρ0 ]2 ,

(3.4)

where ρˆ+ = ρˆA + ρˆB + ρˆH is the spatially varying total microscopic density and κ controls the strength of the density fluctuations. Finally, a repulsive Flory-like potential is used to include enthalpic repulsions between dissimilar components βU2 =

χIJ I 15 vol%); at lower filler loadings, numerical predictions were substantially higher than the measured values. There can be a number of explanations for this discrepancy. For example, the model did not consider the role of interfacial resistance [26, 58, 59] (we will

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

247

Fig. 9.8 Composite thermal conductivity in HDPE/Al binary mixtures as function of Al filler volume fraction. Experimental data are compared with predictions using various micromechanical models, as well as FEA simulations. Reprinted with permission from [57]. Copyright (2003) Elsevier

address this topic in more detail below). Also, the digitization of the images could have led to incorrect assignment to some pixels in the regions crowded with filler particles. On the other hand, it was shown that constitutive models, such as Cheng and Vachon [45], predict thermal conductivity fairly well at filler loading of less than 10 vol%. This is consistent with the notion that the effective medium theories lose accuracy at higher filler volume fractions as the fillers tend to form large aggregates. Interestingly, though, the authors did not attempt to compare their results with the Bruggeman model which is expected to work better at high filler loadings. Annapragada et al. [60] studied thermal conductivity of particulate composites with polydisperse spherical fillers. They developed packing algorithms to generate representative volume elements (RVE), both in two and three dimensions. The predicted thermal conductivity was shown to be fairly close to the experimental

248

V. V. Ginzburg and J. Yang

Fig. 9.9 Comparison between experimental data (line) and FEA simulations (2D-filled squares; 3D-open circles) for the polypropylene/hollow glass particle composites. Reprinted with permission from [62]. Copyright (2007) Elsevier

value, and the approach certainly could be generalized to other composites with spherical fillers. Liang and Li [61, 62] studied thermal conductivity of polypropylene filled with hollow glass latex particles; in this case, thermal conductivity of the composite is lower than that of the pure matrix. As shown in Fig. 9.9, the predicted thermal conductivity agrees with the measured data reasonably well, both when two-dimensional and three-dimensional FEA models were used. Again, the role of thermal resistance at interface was not considered. Nayak et al. [63] investigated thermal conductivity of epoxy/pine wood dust (PWD) composites; again, the filler thermal conductivity (κ(PWD) = 0.068 W/m K) was less than that of the matrix (κ(epoxy) = 0.363 W/m K), so the overall thermal conductivity should decrease as the filler loading is increased. The authors used threedimensional (3D) sphere-in-cube lattice model, varying the effective sphere radius to change the volume fraction. The problem was solved using ANSYS software. Figure 9.10 shows the dependence of thermal conductivity on the PWD volume fraction; simulations and experiment are in a reasonable agreement, although the non-monotonic behavior of the simulated thermal conductivity is not fully explained and could be an artifact of the lattice model. The examples above considered composites with spherical fillers, monodisperse, or polydisperse. Anisotropic fillers provide further complexity since both positional and orientational distribution of fillers needs to be considered. In recent years, many studies have been devoted to polymer-carbon nanotube (CNT) composites [18, 64–67]. Indeed, with nominal thermal conductivity of CNTs being in excess of 1000 W/m K, one can expect to produce high-thermal conductivity composites with relatively small CNT volume fractions. It has been shown [11, 64, 68] that for polymer/CNT nanocomposites, their electrical conductivity, σ, increases dramatically (by 5–6 orders of magnitude) as the CNT volume fraction is changed from

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

249

Fig. 9.10 Thermal conductivity of epoxy/pine wood dust (PWD) composites as function of the filler volume fraction. Triangles are FEA simulation results, and squares are experimental data. Reprinted with permission from [63]. Copyright (2010) Elsevier

about 0.2 vol% to about 1 vol%. Indeed, according to percolation theory, highaspect ratio fillers such as CNT form continuous network at very low concentrations (for the dependence of percolation threshold on aspect ratio, see, for example, review by Bicerano et al. [69]). This percolated network accounts for most of the charge conduction, making polymer/CNT nanocomposites reasonably good conductors, even if not on the same scale as metals. However, thermal conductivity increases in polymer/CNT nanocomposites are not as significant as the electrical conductivity increases, despite the similarity between the two transport properties. Moniruzzaman and Winey [64] review a number of experimental studies on polymer-CNT thermal conductivity, concluding that in general, the composite TC can exhibit about twoto three-fold increase over the matrix TC; this is a substantial increase but nowhere near what is seen for electrical conductivity. Accordingly, several computational and theoretical studies have been performed to explain this discrepancy. For example, Shenogina et al. [35] simulated the heat flow between two nearby nanotubes in a polymer matrix using ABAQUS finite element software. They concluded that the rate of heat flow was fairly independent of the distance between the nanotubes, thus suggesting either absence or weakness of percolation effects. Singh et al. [59] used element-free Galerkin method to numerically compute effective thermal conductivity of polymer/CNT composite as function of CNT volume fraction and interfacial thermal resistance. The nanotubes were assumed to be perfectly aligned, and the calculated thermal conductivity was along the direction of their alignment. The overall TC thermal conductivity was shown to be a strong function of the CNT volume fraction and the interfacial thermal resistance. More recently, Li et al. [70] used 3D finite element modeling of polymer/singlewall-carbon nanotube (SWCNT) composite with disordered nanotubes, and compared results with experimental data on two model systems, epoxy/SWCNT and

250

V. V. Ginzburg and J. Yang

polyolefin/SWCNT (Fig. 9.11). The results demonstrated, once again, the importance of interfacial thermal resistance for proper understanding of heat transfer in these materials. Even so, the mechanism of heat transfer in the polymer/CNT composites is not yet fully understood, as more recent experimental studies [71, 72] indicated that the increase in heat conductivity as function of the CNT volume fraction could be indeed consistent with the nanotube percolation. Other recent applications of FEA modeling include those of polymer/platelet composites [73, 74] and those where mixed fillers are used [75]. One can expect that in the next several years, FEA simulations of composite properties, including thermal conductivity, will be dramatically expanded and will include formulations with multiple fillers, varying degree of anisotropy, and other complexities. Furthermore, as computers become faster, our ability to use simulations to screen formulations and design candidate systems will increase dramatically.

Fig. 9.11 a A finite element model of a randomly distributed SWCNT/polymer composite. The volume fraction of SWCNTs is 22%. b A temperature distribution of a steady-state thermal analysis of a randomly distributed SWCNT/polymer composite. The volume fraction of SWCNTs is 22%. c Calculated and experimental thermal conductivity (k c ) of SWCNT/epoxy composites as function of SWCNT volume fraction. d Same as (c) but for polyolefin/SWCNT composites. Here, Rksm is the interfacial thermal resistance between SWCNT and matrix. Reprinted with permission from [70]. Copyright (2012) Elsevier

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

251

As already mentioned, one critical challenge in ensuring the validity and accuracy of the continuum-level models (whether constitutive or FEA) is description of the heat transfer through interfaces. Below, we briefly review recent progress on this topic.

9.4.2 Interfacial Thermal Resistance Modeling Interfacial thermal resistance (often called Kapitza resistance following the pioneering work by Kapitza [25]) can be understood as follows. The matrix (such as polymer) and the filler (CNT or an inorganic particle) have different spectra of quantum states for the heat carriers (electrons, holes, and phonons). In most polymers, heat is carried only by phonons, and their density of states is substantially lower than in highly crystalline CNTs or inorganic fillers. As a result, many phonons are back-scattered at the interface between the matrix and the filler. The problem can be exacerbated if the interfacial coupling between the filler and the matrix is weak [76–78]. This results in a temperature discontinuity, T, at the interface; this discontinuity is proportional to the heat flux, J, J = ( T ).

(9.16)

The proportionality constant, , is the interfacial thermal conductivity and has units of W/(m2 K); the inverse of is the interfacial thermal resistance (usually labeled Rk ). It is often convenient to define interfacial thickness, h, as follows, h=

κ

(9.17)

where κ is the bulk thermal conductivity. Typical values of h are on the order of nanometers [26, 77]; thus, it is often reasonable to disregard the interfacial effects if the filler size is on the order of microns. In many FEA simulations of conventional polymer-inorganic composites discussed above, the assumption of “perfect” interface ( T = 0) was thus justified since the typical finite element size was much greater than h. However, if one tried to increase the composite thermal conductivity substantially higher, by increasing the filler loading and/or reducing the filler size, the interparticle distance Dint would eventually decrease to the point where it becomes comparable to h. Further increases in the filler volume fraction would then lead to no improvement in the overall TC. As Shenogin et al. [77] emphasize, in these nanocomposites, the fillers could be separated by 1 nm physically, yet from thermal standpoint, their separation could be as large as h ~ 10–20 nm. This insight helps us better understand the results from the FEA and micromechanical models in which the interfacial resistance was varied parametrically (Figs. 9.5 and 9.11)—once the filler volume fraction increased to the point where the interparticle distance becomes comparable to the thermal interfacial thickness, the overall thermal conductivity stops increasing.

252

V. V. Ginzburg and J. Yang

So far, we mainly discussed continuum approaches to thermal conductivity, where heat transfer through matrix, filler, and interface was described in a phenomenological manner. In order to predict the interfacial thermal resistance, one needs to turn to molecular models. We already mentioned the study by Shenogin et al. [77] who used Molecular Dynamics to study interfacial heat transport between a carbon nanotube and octane liquid. Alzina et al. [79] used multiscale modeling to study heat transfer in epoxy/glass composites at very low temperatures. They showed that theory and experiment agreed fairly well if one assumed the so-called diffuse mismatch model (DMM), in which all phonons were assumed to diffusely scatter at the interface. Roy et al. [80, 81] demonstrated using Molecular Dynamics the importance of coupling between the carbon nanotube and the polymer matrix. Shin et al. [82] developed a multiscale model combining nonequilibrium Molecular Dynamics and finite element analysis to compute thermal conductivity in SiC/epoxy composites. Similar approaches have been also applied to various other systems [78, 83–85]. One important conclusion from these and other studies was that the surface functionalization of the filler could be crucial to improving thermal conductivity of composites. Within both theories of interfacial resistance (acoustic mismatch model and diffuse mismatch model), the interfacial thermal conductivity is directly proportional to the overlap between vibrational density of states (VDOS) spectra of the matrix and the filler. Wang et al. [78] computed VDOS of pristine or organically modified graphene sheet and compared it with those of a model paraffin (Fig. 9.12). The calculation shows that accurately matching the VDOS of the filler and the matrix by using the right surface modifier is very important. Even though the overlap integral S increases substantially upon addition of virtually any organic modifier, butyl surfactant results in the highest S-value, leading to the most effective reduction in the interfacial resistance for a given surface coverage (Fig. 9.13). This analysis shows that even modest surface functionalization could lead to substantial improvement in the interfacial thermal transport. Recent experimental studies suggest that surface functionalization can indeed lead to some improvement in thermal conductivity in alumina/nylon-6 composites [86]. Prediction of interfacial thermal properties is still relatively new and rapidly developing field, and this short review does not attempt to be comprehensive. As computers become more powerful and atomistic force fields more accurate, we can expect to see more advances in predicting interfacial thermal resistance for more and more diverse filler/matrix pairs. Creating such a library will help in developing more accurate macroscopic FEA models and thus using modeling as part of new material design.

9.4.3 Multiscale Modeling As we discussed above, an accurate prediction of thermal conductivity in polymerinorganic nano- and micro-composites requires the knowledge of structure and dynamics on several length-scales, from atomistic (to determine the electron and phonon spectra and the density of states, both in the bulk and at interfaces) to

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

253

Fig. 9.12 Comparison of VDOS between paraffin (blue) and graphene with various surface functionalities (red). The captions (S = 0.006 etc.) describe the calculated VDOS overlap integrals. Reprinted with permission from [78]. Copyright (2015) American Chemical Society

254

V. V. Ginzburg and J. Yang

Fig. 9.13 Interfacial thermal resistance (relative to that of pristine graphene) as function of surfactant coverage for various functionalizations. Reprinted with permission from [78]. Copyright (2015) American Chemical Society

nanoscale (to determine the local interactions between the fillers and the structure of the polymer in their proximity) to microscale (to determine the filler dispersion and orientation) to macroscale (to understand the influence of processing conditions). Obviously, no single modeling approach can simulate all of these phenomena; to address them, we need to utilize multiscale modeling paradigm [87–93]. One successful example of such multiscale modeling is the recent work by Odegard et al. [93] in which thermal conductivity of graphene nanoplatelets in cycloaliphatic epoxy was studied by combined molecular dynamics (MD) and micromechanics (MM); MD simulations were used to predict the interfacial thermal resistance and MM simulations were then used to compute TC as function of the nanoplatelet dispersion, orientation, and loading. Overall, this is still a relatively new and rapidly growing field.

9.5 Summary and Outlook Thermally conductive materials are and will remain critically important for various industries, from electronics to energy to automotive. The use of nano- and microcomposite materials is often required to successfully navigate the balance of properties (thermal conductivity, electrical conductivity or lack thereof, mechanical

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

255

strength, thermal expansion, viscosity, etc.). The use of modeling is often required to reduce the number of potential experiments, develop new design criteria for the selection of matrix and filler materials, and/or understand the failure mechanisms for existing materials. Currently, most theoretical and computational research dealing with the prediction and description of thermal conductivity in composites is based on analytical or numerical micromechanical models. Most often, in these models, the composite morphology is simplified, and the fillers are assumed to be uniformly dispersed and— if non-spherical—oriented isotropically. While these approaches often are successful in describing experimental results in commercial composites, the success is typically accomplished by the introduction of fitting parameters (for example, interfacial or Kapitza resistance is often used as one). In our view, the main challenges for theoretical and computational prediction of thermal conductivity in composite materials are as follows. First, it is necessary to develop robust procedures (either EMA or FEA) to calculate thermal conductivities of composites with multiple fillers having different sizes and different shapes/aspect ratios. Second, it is necessary to understand the relationship between the processing conditions and the composite morphology (aggregation, orientation, and dispersion). Finally, it is necessary to understand the molecular details of heat transport on the nanoscale, both within the fillers and the matrix and through various interfaces. Addressing these challenges will likely take a long time and will require a significant modification of existing theoretical and computational tools. It is possible, even likely, that new tools (e.g., machine learning) will also be added to the mix. It is our hope that this review will help future researchers as they work on the new approaches to this old but fascinating problem. Acknowledgements We thank Dow for supporting this work. We are also grateful to Darren Hansen and Huikuan Chao for critical review of the manuscript and many helpful suggestions.

References 1. A.L. Moore, L. Shi, Mater. Today 17, 163 (2014) 2. X.C. Tong, Advanced Materials for Thermal Management of Electronic Packaging, vol. 30, 1st edn. (Springer, New York, 2011) 3. P.K. Schelling, L. Shi, K.E. Goodson, Mater. Today 8, 30 (2005) 4. F. Sarvar, D.C. Whalley, P.P. Conway, in 2006 1st Electronic Systemintegration Technology Conference (IEEE, 2006), p. 1292 5. H. Chen, V.V. Ginzburg, J. Yang, Y. Yang, W. Liu, Y. Huang, L. Du, B. Chen, Prog. Polym. Sci. 59, 41 (2016) 6. P. Keblinski, Modeling of Heat Transport in Polymers and Their Nanocomposites, In: Handbook of Materials Modeling: Applications: Current and Emerging Materials, 2-nd edn, editors: W. Andreoni, S. Yip, (Springer Nature, Cham, 2020), p. 975–997 https://doi.org/10.1007/978-3319-44680-6_31 7. A. Li, C. Zhang, Y.-F. Zhang, Polymers 9, 437 (2017)

256

V. V. Ginzburg and J. Yang

8. X. Yang, C. Liang, T. Ma, Y. Guo, J. Kong, J. Gu, M. Chen, J. Zhu, Adv. Compos. Hybrid Mater. 1, 207 (2018) 9. C. Huang, X. Qian, R. Yang, Mater. Sci. Eng. R Rep. 132, 1 (2018) 10. J. Ordonez-Miranda, R. Yang, J.J. Alvarado-Gil, Nanoscale Thermoelectrics (Springer, Berlin, 2014), p. 93 11. R. Haggenmueller, C. Guthy, J.R. Lukes, J.E. Fischer, K.I. Winey, Macromolecules 40, 2417 (2007) 12. I. Krupa, I. Novak, I. Chodak, Synth. Met. 145, 245 (2004) 13. A. Henry, G. Chen, Phys. Rev. Lett. 101, 235502/1 (2008) 14. T.F. Luo, K. Esfarjani, J. Shiomi, A. Henry, G. Chen, J. Appl. Phys. 109, 074321/1 (2011) 15. R.Y. Wang, R.A. Segalman, A. Majumdar, Appl. Phys. Lett. 89, 173113/1 (2006) 16. Z.H. Wang, J.A. Carter, A. Lagutchev, Y.K. Koh, N.H. Seong, D.G. Cahill, D.D. Dlott, Science 317, 787 (2007) 17. X.P. Huang, G.Q. Liu, X.W. Wang, Adv. Mater. 24, 1482 (2012) 18. Z.D. Han, A. Fina, Prog. Polym. Sci. 36, 914 (2011) 19. https://www.netzsch-thermal-analysis.com/uploads/tx_nxnetzschmedia/files/TPoP_web_ mit_Hervorhebung.pdf. Accessed on 19 Jan 2015 20. Y. Yang, in Physical Properties of Polymers Handbook, ed. by J.E. Mark (Springer Science & Business Media, New York, 2007), p. 156 21. A. Henry, G. Chen, Phys. Rev. Lett. 101 (2008) 22. Z. Lu, Y. Wang, X. Ruan, J. Appl. Phys. 123, 074302 (2018) 23. D. Bigg, Adv. Polym. Sci. 119, 1 (1995) 24. J.C.M. Garnett, Proc. Roy. Soc. Lond. Ser. A 73, 443 (1904) 25. P.L. Kapitza, J. Phys. 4, 181 (1941) 26. C.-W. Nan, R. Birringer, D.R. Clarke, H. Gleiter, J. Appl. Phys. 81, 6692 (1997) 27. J. Ordonez-Miranda, R. Yang, J.J. Alvarado-Gil, J. Appl. Phys. 114, 064306 (2013) 28. J. Ordonez-Miranda, R. Yang, J.J. Alvarado-Gil, J. Appl. Phys. 111, 044319 (2012) 29. J. Ordonez-Miranda, J.J. Alvarado-Gil, Compos. Sci. Technol. 72, 853 (2012) 30. M. Mooney, J. Colloid Sci. 6, 162 (1951) 31. H. Fricke, Phys. Rev. 24, 575 (1924) 32. I.H. Tavman, J. Appl. Polym. Sci. 62, 2161 (1996) 33. D.A.G. Bruggeman, Ann. Phys. Leipzig 24, 636 (1935) 34. D. Stroud, Superlattices Microstruct. 23, 567 (1998) 35. N. Shenogina, S. Shenogin, L. Xue, P. Keblinski, Appl. Phys. Lett. 87, 133106 (2005) 36. D.A. Brune, J. Bicerano, Polymer 43, 369 (2002) 37. P.E. Gharagozloo, K.E. Goodson, J. Appl. Phys. 108, 074309/1 (2010) 38. W. Lin, Modeling of thermal conductivity of polymer nanocomposites, in Modeling and Prediction of Polymer Nanocomposite Properties, ed. by V. Mittal (Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim, Germany, 2013) 39. Z. Hashin, S. Shtrikman, J. Appl. Phys. 33, 3125 (1962) 40. Z. Hashin, J. Compos. Mater. 2, 284 (1968) 41. R.L. Hamilton, O.K. Crosser, Ind. Eng. Chem. Fund. 1 (1962) 42. R. L. Hamilton, Thermal Conductivity of Heterogeneous Mixtures, Ph. D. Dissertation, University of Oklahoma (1960) 43. H. Hatta, M. Taya, J. Appl. Phys. 58, 2478 (1985) 44. Y. Agari, A. Ueda, S. Nagai, J. Appl. Polym. Sci. 49, 1625 (1993) 45. S. Cheng, R. Vachon, Int. J. Heat Mass Transf. 13, 537 (1970) 46. L. Nielsen, J. Appl. Phys. 41, 4626 (1970) 47. L. Nielsen, J. Appl. Polym. Sci. 17, 3819 (1973) 48. T. Lewis, L. Nielsen, J. Appl. Polym. Sci. 14, 1449 (1970) 49. A.D. Drozdov, J. deClaville Christiansen, Compos. Sci. Technol. 182, 107717 (2019) 50. K. Ramani, A. Vaidyanathan, J. Compos. Mater. 29, 1725 (1995) 51. R.W. Lewis, P. Nithiarasu, K. Seetharamu, Fundamentals of the Finite Element Method for Heat and Fluid Flow (Wiley, Hoboken, 2004)

9 Modeling the Thermal Conductivity of Polymer-Inorganic …

257

52. S.S. Rao, The Finite Element Method in Engineering (Butterworth-Heinemann, UK, 2005) 53. G. Dhatt, E. Lefrançois, G. Touzot, Finite Element Method (Wiley, Hoboken, 2012) 54. T.J. Hughes, The Finite Element Method: Linear Static and Dynamic Finite Element Analysis (Courier Dover Publications, USA, 2012) 55. L. Onsager, Phys. Rev. 37, 405 (1931) 56. L. Onsager, Phys. Rev. 38, 2265 (1931) 57. D. Kumlutas, I.H. Tavman, M.T. Coban, Compos. Sci. Technol. 63, 113 (2003) 58. R. Peterson, A. Anderson, J. Low Temp. Phys. 11, 639 (1973) 59. I.V. Singh, M. Tanaka, M. Endo, Int. J. Therm. Sci. 46, 842 (2007) 60. S.R. Annapragada, D. Sun, S.V. Garimella, Comp. Mater. Sci. 40, 255 (2007) 61. J.Z. Liang, F.H. Li, Polym. Test. 26, 1025 (2007) 62. J.Z. Liang, F.H. Li, Polym. Test. 26, 419 (2007) 63. R. Nayak, P.T. Dora, A. Satapathy, Comp. Mater. Sci. 48, 576 (2010) 64. M. Moniruzzaman, K.I. Winey, Macromolecules 39, 5194 (2006) 65. J.M. Wernik, S.A. Meguid, Appl. Mech. Rev. 63 (2010) 66. M. Rahmat, P. Hubert, Compos. Sci. Technol. 72, 72 (2011) 67. Z. Spitalsky, D. Tasis, K. Papagelis, C. Galiotis, Prog. Polym. Sci. 35, 357 (2010) 68. F. Du, R.C. Scogna, W. Zhou, S. Brand, J.E. Fischer, K.I. Winey, Macromolecules 37, 9048 (2004) 69. J. Bicerano, J.F. Douglas, D.A. Brune, J. Macromol. Sci. Rev. Macromol. Chem. Phys. C 39(4), 561–642 (1999) 70. X.T. Li, X.Y. Fan, Y.D. Zhu, J. Li, J.M. Adams, S. Shen, H.Z. Li, Comp. Mater. Sci. 63, 207 (2012) 71. B.-W. Kim, S.-H. Park, R. Kapadia, P. Bandaru, Appl. Phys. Lett. 102, 243105 (2013) 72. S.Y. Kwon, I.M. Kwon, Y.-G. Kim, S. Lee, Y.-S. Seo, Carbon 55, 285 (2013) 73. R.F. Hill, J.L. Strader, IEEE Trans. Compon. Packag. Technol. 30, 235 (2007) 74. B. Mortazavi, O. Benzerara, H. Meyer, J. Bardon, S. Ahzi, Carbon 60, 356 (2013) 75. K. Sanada, Y. Tada, Y. Shindo, Compos. Part A Appl. Sci. Manuf. 40, 724 (2009) 76. P. Keblinski, J.A. Eastman, D.G. Cahill, Mater. Today 8, 36 (2005) 77. S. Shenogin, L. Xue, R. Ozisik, P. Keblinski, D.G. Cahill, J. Appl. Phys. 95, 8136 (2004) 78. Y. Wang, H.F. Zhan, Y. Xiang, C. Yang, C.M. Wang, Y.Y. Zhang, J. Phys. Chem. C 119, 12731 (2015) 79. A. Alzina, E. Toussaint, A. Béakou, B. Skoczen, Compos. Struct. 74, 175 (2006) 80. A.K. Roy, B.L. Farmer, V. Varshney, S. Sihn, J. Lee, S. Ganguli, ACS Appl. Mater. Interfaces 4, 545 (2012) 81. V. Varshney, S.S. Patnaik, A.K. Roy, G. Froudakis, B.L. Farmer, ACS Nano 4, 1153 (2010) 82. H. Shin, S. Yang, S. Chang, S. Yu, M. Cho, Polymer 54, 1543 (2013) 83. M.R. Gharib-Zahedi, M. Tafazzoli, M.C. Böhm, M. Alaghemandi, Phys. Chem. Chem. Phys. 17, 14502 (2015) 84. K. Tanaka, S. Ogata, R. Kobayashi, T. Tamura, T. Kouno, Int. J. Heat Mass Transf. 89, 714 (2015) 85. D. Konatham, A. Striolo, Appl. Phys. Lett. 95, 163105 (2009) 86. K. Sato, A. Ijuin, Y. Hotta, Ceram. Int. (2015) 87. T. Gates, G. Odegard, S. Frankland, T. Clancy, Compos. Sci. Technol. 65, 2416 (2005) 88. T.C. Clancy, S.-J.V. Frankland, J.A. Hinkley, T.S. Gates, Int. J. Therm. Sci. 49, 1555 (2010) 89. S. Zhai, P. Zhang, Y. Xian, J. Zeng, B. Shi, Int. J. Heat Mass Transf. 117, 358 (2018) 90. A. Vahedi, M.H.S. Lahidjani, S. Shakhesi, Phys. B 550, 39 (2018) 91. A.G. Hoekstra, S. Portegies Zwart, P.V. Coveney, Multiscale modelling, simulation and computing: from the desktop to the exascale, Phil. Trans. R. Soc. A. 377, 20180355 (2019) 92. J.L. Suter, P.V. Coveney, ACS Omega 3, 6439 (2018) 93. S. Chinkanjanarot, J.M. Tomasi, J.A. King, G.M. Odegard, Carbon 140, 653 (2018)

Chapter 10

Predicting the Optical and Electrical Properties of Polymer Nanocomposites Michael J. A. Hore

Abstract Nanoparticles are frequently combined with polymers to create polymer nanocomposite materials with enhanced electrical, optical, or transport properties. In addition to the robust suite of theoretical techniques—including molecular dynamics, Monte Carlo simulations, and polymer field theory—that exists to predict structural information of such polymer nanocomposites, there is also a sizeable selection of techniques available to predict physical properties such as optical scattering/absorption and electrical/ionic conductivity of these materials. In many instances, techniques for predicting structural information may be coupled to those used to predict physical properties. This chapter presents a survey of common approaches to modeling both the optical and electrical properties of polymer nanocomposites, explaining the foundations of each technique, limitations, and highlighting select examples from the literature using each technique.

10.1 Introduction Polymer nanocomposites result from the combination of a polymer matrix with one or more nanoparticle components. The nanoparticles may be bare or polymer-grafted, and can have shapes ranging from isotropic spheres to complex geometries. A primary motivating factor in adding nanoparticles to polymer materials is to enhance the physical properties of the resulting polymer nanocomposite. These physical properties include the mechanical properties, optical properties, and electrical properties among others [1–3]. For example, carbon nanotubes may enhance the electrical conductivity and/or the mechanical properties of the nanocomposite, whereas noble metal nanoparticles can impart useful optical properties. Key to understanding the resulting physical properties of the nanocomposite is having a robust understanding of the nanoparticle distribution, orientation, or other morphological information. M. J. A. Hore (B) Department of Macromolecular Science and Engineering, Case Western Reserve University, Euclid Avenue, Cleveland, OH 10900, USA e-mail: [email protected] © Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1_10

259

260

M. J. A. Hore

As discussed elsewhere in this book, there are numerous computational approaches, including field theoretic calculations and particle-based simulations, to extract such information. The focus of this chapter is prediction of nanocomposite properties as a function of nanoparticle distribution, material morphology, and so on. The first section of this chapter contains an extensive discussion of calculating optical absorption and scattering by a polymer nanocomposite that contains metallic nanoparticles, such as Au nanospheres. Mie theory, the discrete dipole approximation (DDA), and finite-difference time-domain (FDTD) calculations can all be applied to the study of polymer nanocomposites. The second section of this chapter discusses determinating the electrical properties of a nanocomposite using resistor network models. Although not typically applied to polymer nanocomposite systems, this chapter closes with an introduction to the Poisson-Nernst-Planck formalism, which can be applied in the future to understand ion transport in polymer nanocomposites.

10.2 Calculation of Optical Properties Noble metal nanoparticles have attracted interest from the polymer nanocomposite community because of the manner in which they interact with light. Nanoparticles synthesized from elements such as Au or Ag interact with light to preferentially scatter or absorb certain wavelengths. The combination of scattering and absorption is referred to as extinction, and the ability to tune the wavelength where the majority of the extinction occurs is attractive for many applications. For nanoparticles composed of Au, Ag, and other noble metal nanoparticles, incident light creates collective oscillations of electrons along the surface of the nanoparticle (“surface plasmons”). This process is distinct from those that give rise to optical phenomena in quantum dot materials, such as CdSe. The result of the excitation of surface plasmons is one or more characteristic absorptions at wavelengths that depend on the nanoparticle size, shape, dispersion, and other factors. Photons with wavelengths equal to the surface plasmon resonance (SPR) wavelength experience strong absorption and scattering by the particles. When particles are present at high volume fractions (i.e., are close to one another spatially), the relative interparticle spacing affects the extinction of the nanocomposite. Generally, this “plasmonic coupling” results in a red-shifting of the SPR for spherical nanoparticles. For anisotropic nanoparticles, the polarization of the incident light, relative to the orientation of the nanoparticle, becomes an important determining factor, as does the spacing and relative orientation of the particles with respect to their neighbors. In all instances, the refractive indices of both the nanoparticle and surrounding matrix must be taken into account if an accurate prediction of the SPR wavelength is desired. The prediction of optical absorption or scattering by nanoparticles may be validated experimentally by UV-visible spectrophotometry (UV-vis), dark field optical microscopy, and Fourier-transform infrared spectroscopy to name a few. For the interested reader, Maier provides an extensive review of the fundamentals of plasmonics [4].

10 Predicting the Optical and Electrical Properties …

261

10.2.1 Mie Theory Applied to Polymer Nanocomposites Mie theory is the result of solving Maxwell’s equations analytically. In 1908, Gustav Mie published the result of solving Maxwell’s equation to describe the scattering of light by colloidal (spherical) metal particles, which provided a mechanism behind the colors of colloidal gold solutions. The extinction and scattering cross sections, Cext and Csca , respectively, are typically expressed in terms of their efficiencies. Mie theory gives the following expressions for the extinction and scattering efficiencies: Qext =

∞ Cext 2 = (2n + 1)Re(an + bn ) π r2 x2 n=0

(10.1)

Qsca =

∞ Csca 2 = (2n + 1)(|an | + |bn |) π r2 x2 n=0

(10.2)

where the scattering amplitudes an and bn are defined in terms of Riccati-Bessel functions. The mathematical expressions for these amplitudes are complicated, and the interested reader can find their expressions in the work of Bohren and Huffman [5]. In practice, for particles of size r, the summations in (10.1) and (10.2) can be truncated at a value nmax = x + 4x1/3 + 2, with x = kr = 2π r/λ. The absorption characteristics can be analyzed in terms of the absorption cross section Cabs = Cext − Csca . In addition, analysis with Mie theory can be extended to more complex particle architectures, such as spherical core-shell particles and others. However, analytical solutions for non-spherical shapes have proven elusive to date. Nevertheless, examples of approximate Mie-type theories for other geometries can be found in the literature [6, 7]. The application of Mie theory to predict the optical properties of nanocomposites is relatively straightforward, and consists primarily of calculating the extinction and scattering cross sections at wavelengths of interest. Fortunately, spherical nanoparticles are a common component of polymer nanocomposites, meaning that Mie theory is applicable to a number of nanocomposite systems [8, 9]. However, a limitation of this approach is that the calculations largely ignore the internal structure of the nanocomposite by assuming dispersed nanoparticles, and instead rely on characteristics of the components, such as the size of the nanoparticles and their refractive indices. In light of this, an important aspect of applying Mie theory is correctly representing the refractive indices of the material. As one example, this can be illustrated in recent work by Bockstaller et al. on dispersion of poly(styrene-r-acrylonitrile) (PSAN)-grafted SiO2 nanoparticles in a poly(methyl methacrylate) (PMMA) matrix [10]. At a wavelength of λ = 532 nm, the refractive indices of SiO2 , PSAN, and PMMA are 1.458, 1.573, and 1.489, respectively. Because of this, the authors were able to index match the PSAN-grafted SiO2 to the PMMA matrix—a condition that maximizes transmittance. The dielectric constant of the nanoparticles, which consist of a core and a shell, can be approximated using the Maxwell-Garnett effective

262

medium model [11]:

M. J. A. Hore

εeff = εshell 1 +

3fx (1 − fx)

(10.3)

where f is the volume fraction of the core (relative to the volume of the entire nanoparticle), and (εcore − εshell ) (10.4) x= (2εcore + εshell ) The dielectric constant (ε) is related to the refractive index (n) as ε = n2 . In practice, this approximation would be tabulated as a function of wavelength, and the extinction and scattering cross sections calculated. Using this approach, the authors found excellent quantitative agreement between Csca measured experimentally, and that calculated using Mie theory, as shown in Fig. 10.1. A similar approach was taken by Incel et al. in predicting the scattering and extinction of spherical CeO2 nanoparticles coated with SiO2 when incorporated into a polystyrene film [12]. The supporting information of [12] provides computer code demonstrating the calculation of extinction and scattering according to (10.1) and (10.2). Of the techniques discussed in this chapter for predicting the optical properties of nanocomposites, Mie theory is perhaps the most limiting in that it is restricted to spherically-symmetry scatterers, and cannot describe more complicated situations such as self-assembled structures, for example. In addition, while it has been shown to accurately describe the scattering and extinction cross sections, it is unable to produce detailed features such as the local electric field or the scattering cross section due to plasmonic coupling. To accurately tie the internal structure of a polymer nanocomposite to the resulting macroscopic optical behavior, more detailed approaches are needed.

Fig. 10.1 Scattering cross section Csca of polystyrene (PS)-grafted SiO2 nanoparticles in toluene as a function of the weight fraction of PS, φPS . Open points were calculated using Mie theory, and filled points are experimental measurements. Squares, circles, and triangles correspond to nanoparticles with diameters of 16, 120, and 500 nm, respectively. Reproduced with permission c from [8], Copyright 2014 American Chemical Society

10 Predicting the Optical and Electrical Properties …

263

10.2.2 The Discrete Dipole Approximation (DDA) While exact analytical solutions of Maxwell’s equations are only possible in certain limiting cases (e.g., spherical nanoparticles), certain approximations have been extremely successful in modeling a variety of systems. The Discrete Dipole Approximation (DDA) can be attributed to work produced by Purcell and Pennypacker in 1973 [13]. Originally developed to describe the scattering and absorption of light by interstellar dust, it models a continuous particle as a collection of discrete dipole particles. The electromagnetic response of the dipoles is calculated for an incident electromagnetic field Einc . Most often, software packages such as DDSCAT and ADDA are used to calculate the response. Recently, with the advent of general-purpose computing on graphical processing units (GPUs), codes have been developed that take advantage of the highly parallel nature of GPU architectures to increase the speed of DDA calculations. DDA-GPU is one such program, although other examples exist.

10.2.2.1

Theoretical Background

Traditionally, within DDA the nanoparticle (“target”) is composed of N dipoles arranged on a cubic lattice. In the original DDA formulation, the polarizibility of each dipole i was calculated from the Clausius-Mossotti relationship, 3d 3 αi = 4π

εi − 1 εi + 2

(10.5)

where εi is the dielectric function of dipole i, and d is the lattice constant of the cubic array. Draine and Flatau noted that this expression is only exact for kd = 0, where k = ω/c, with ω representing the angular frequency of the light and c the speed of light in a vacuum. If the wavelength of the light is much larger than the lattice constant of the dipoles, then the polarizibilty can be approximated as αiDG ≈

αi

1 + αi /d 3 (b1 + n2 b2 + n2 b3 S)(kd 2 ) − (2/3)ikd 3

(10.6)

√ In (10.6), i = −1, S is a real number that describes the polarization of the incident radiation, and n is the refractive index. The coefficients b1 = −1.891531, b2 = 0.1648469, and b3 = −1.7700004. Draine and Flatau note that this correction is most accurate for |n|kd < 1. For this reason, DDA calculations typically require a large number of dipoles to ensure that d is sufficiently small and the polarizibility is correctly determined. Because DDA can be used to define nanoparticles of arbitrary geometries, it is convenient to characterize a target by an effective radius aeff . In fact, some software packages such as DDSCAT require this value as a parameter to the calculation. The effective radius of a target is calculated by setting the actual volume of a target equal

264

M. J. A. Hore

to the volume of an equivalent sphere, resulting in an expression aeff =

3V 4π

13

=

3N 4π

13 d

(10.7)

where N is the number of dipoles that the target contains, V is the physical volume of the target, and d is the spacing of the dipoles. For a spherical nanoparticle with radius rs , this expression simplifies greatly, and the effective radius can be written, aeff = rs = d

3N 4π

13 (10.8)

While it is not surprising that the effective radius of a sphere would be equal to its physical radius, (10.8) is useful as it provides guidance regarding the number of dipoles (N ) that are necessary to accurately model the extinction from that particle. Similarly, for the special case of a nanorod, this expression reduces to aeff =

13 3 (rr2 L) 4

(10.9)

Show in Fig. 10.2a is a nanorod target with a physical diameter 15 nm and length 40 nm, and which contains 6152 discrete dipoles. From (10.7)–(10.9), the lattice spacing of the target can be calculated as d = 1.05 nm. For targets composed of Au, this lattice spacing implies |n|kd ≈ 0.02 – 0.04, which is well below the condition required by Draine and Flatau. To mimic structures that may occur within a

Fig. 10.2 DDA target structures. a A DDA target consisting of a single nanorod with N = 6157 dipoles (shown as spheres) representing a particle with a physical size of 15 × 40 nm. For this target, aeff = 25.6 nm (10.7). b Two side-by-side oriented nanorods separated by a distance h, constructed from the target in (a). c Two end-to-end oriented nanorods, separated by a distance h

10 Predicting the Optical and Electrical Properties …

265

nanocomposite, such as aggregated or oriented nanoparticles, targets can be created using the nanorod target as a template, as demonstrated in Fig. 10.2b, c. To calculate the scattering and absorption cross sections, the incident electric field at each lattice point and the polarization of each discrete dipole must be determined. Each dipole experiences an electric field Einc = E0 exp ik · rj − iωt

(10.10)

which represents the incoming, external electromagnetic radiation with frequency ω. Each discrete dipole interacts with this incoming electromagnetic field, and in turn, with all dipoles contained within the target. Therefore, the net electric field for dipole j is the difference of the two contributions, i.e., Ej = Einc −

Ajk Pk

(10.11)

k=j

where Pk = αk Ek is the polarization of dipole k, and exp(ikrjk ) ikrjk − 1 2 Ajk = × k (ˆrjk rˆjk − I3 ) + (3ˆrjk rˆjk − I3 ) rjk rjk2

(10.12)

In (10.12), I3 is the 3 × 3 identity matrix, rjk = |rj − rk |, and rˆjk = (rj − rk )/rjk . The diagonal terms Ajj = αj−1 , reducing (10.11) to

Ajk Pk = Einc

(10.13)

k

This linear system is then solved using standard linear algebra methods to obtain the polarization for each dipole j, i.e., Pj . The absorption and scattering cross sections, Cabs and Csca , respectively, are obtained from the incident electromagnetic field and the individual dipole polarizations. The extinction cross section is the sum of the scattering and absorption terms, Cext = Csca + Cabs . For a target composed of NDDA dipoles, the absorption and scattering cross sections read: Cabs

NDDA ∗ 2 4π k −1 ∗ 3 2 Im Pj · αj = Pj − k |Pj | |E0 |2 j=1 3 Csca =

NDDA 4π k Im Ej∗ · Pj − Cabs 2 |E0 | j=1

(10.14)

(10.15)

266

M. J. A. Hore

where Ej∗ , Pj∗ , and αj∗ denote the complex conjugates of those quantities. The scattering and absorption efficiencies, Qsca and Qabs , are obtained by normalizing the 2 . respective cross sections by π aeff Because it captures the effects of both scattering and absorption, Qext = Qsca + Qabs is a convenient quantity to calculate to characterize the optical response of nanocomposites that contain nanoparticles with a plasmonic response. However, for anisotropic nanoparticles, such as gold nanorods, the extinction coefficient is polarization dependent. In particular, surface plasmons are excited only by p-polarized light (i.e., the electric field is parallel to the plane of incidence). For this reason, to correctly model the optical response of a rod-like object, Qext needs only to be calculated for two orientations of the rods: parallel and perpendicular with respect to the polarization of the incident light. For more anisotropic objects, a larger number of orientations of the object will need to be considered, while for a sphere, only one orientation is necessary to correctly model the optical response. Surface plasmon resonances (SPRs) are indicated by large enhancements in the scattering/absorption cross sections at particular wavelengths. The behavior of the extinction cross section with respect to wavelength is primarily dependent on the incident electromagnetic field, the interactions between individual dipoles, and the relative refractive indices of the particles and matrix material. For this reason, DDA is an effective method not only for calculating the optical response of isolated nanoparticles within a polymer matrix, but also the optical response of self-assembled nanoparticles within nanocomposites. For instance, nanoparticles in close proximity to one another will exhibit surface plasmon coupling, which may result in a red or blueshift of the position of the surface plasmon resonance relative to the position in isolated particles. However, because the total number of dipoles scales with the number of nanoparticles in the DDA target, assemblies consisting of large numbers of nanoparticles are computationally expensive and in many instances, computationally intractable. In these cases, other techniques such as FDTD, described later in this chapter, may be more applicable.

10.2.2.2

Correction of the Dielectric Function

The previous discussion of the theoretical background of DDA did not explicitly consider the effect of material type on the extinction characteristics of nanoparticles. The effect of material type (e.g., gold or silver) on the optical properties determined by a DDA calculation can be seen in (10.5) and (10.6). The values of the material dielectric function directly modify the polarizibilities of the discrete dipoles. From the free electron model, the dielectric function of a material can be expressed as: ε(ω) = 1 −

ωp2 ω2

(10.16)

where ωp is the plasma frequency of the material. This expression neglects several important contributions. First, it does not consider the effect of collisions of the

10 Predicting the Optical and Electrical Properties …

267

electrons with the positively charged, stationary atomic cores. To include this effect, a relaxation time τ for the free electron gas is introduced into the model, leading to a corrected dielectric function: εb (ω) = 1 −

ωp2 ω(ω + i/τ )

(10.17)

where the subscript b designates that this is the dielectric function of the bulk material. However, in the case that DDA is used to calculate the optical properties of polymer nanocomposites, it may be necessary to correct for the presence of the nanoparticle surface, from which electrons may collide. The result of such corrections is an additional surface relaxation term τa ≈ aeff /vF , where vF is the Fermi velocity. Physically, τa represents the timescale of collisions of electrons with the nanoparticle surface. The resulting dielectric function is εs (ω) = 1 −

ωp2 ω(ω + i/τ + i/τa )

(10.18)

where the subscript s designates that the dielectric function was corrected for surface damping. Typically, only bulk dielectric data is available in the scientific literature. Hence, to obtain a dielectric function suitable for calculating the extinction spectra of nanoparticles, the bulk dielectric data must be corrected as: ωp2 ωp2 εs (ω) = εb (ω) + − (10.19) ω(ω + i/τ ) ω(ω + i/τ + i/τa ) In practice, the dielectric function must be corrected each time the value of aeff changes for a given DDA system. For gold nanoparticles, ωp = 8.55 eV, /τ = 0.108 eV, and vF = 1.41 × 106 m/s.

10.2.2.3

Examples from the Literature

DDA has been used in several studies aiming to predict and interpret the optical response of polymer nanocomposites and similar materials. It is particularly useful in that targets can be constructed from the outputs of other modeling techniques, such as Monte Carlo or molecular dynamics simulations, and then examined with an appropriate DDA code. In addition, DDA has been applied to numerous experimental studies by constructing targets that are based on electron micrographs, for example. Here, we highlight a few such studies to illustrate the application of DDA to predict the optical properties of polymer nanocomposites. DDA has seen a lot of applications in the characterization of surface plasmons in Au nanoparticles. Work from El-Sayed and coworkers demonstrated a “plas-

268

M. J. A. Hore

mon ruler” effect in which the wavelength of the surface plasmon shifted exponentially with the distance between pairs Au nanodiscs [14]. The relative shift scaled as λ/λ0 ∼ exp(−x/Dτ ), where D is the nanodisc diameter, x is their separation distance, and τ is a unitless decay constant. Experiments found the decay constant τ = 0.18 ± 0.02 whereas DDA found τ = 0.23 ± 0.03, implying that plasmon coupling took place within distances equal to about 20% of the nanodisc size. For anisotropic nanoparticles, such as gold nanorods, the details of plasmonic coupling depend on both the separation of the nanorods as well as their relative orientations [15]. While the studies highlighted above considered nanoparticles in a vacuum or deposited on a surface in air, it is trivial to extend the application of DDA to polymer nanocomposites by taking into account the refractive index of the nanocomposite. Autophobic dewetting is a well-known phenomenon that can result in the aggregation of polymer-grafted nanoparticles within a chemically-identical polymer matrix [16, 17]. As a general guideline, nanospheres have been observed to aggregate when the degree of polymerization of the brush N is around three times smaller than that of the matrix P, i.e., P > 3N . For nanorods, it has been observed that aggregation occurs for P > 2N . A significant number of computational studies have found more detailed expressions for these transitions that depend on grafting density and other factors [1, 18]. A result of aggregation due to autophobic dewetting is that nanoparticles which exhibit surface plasmon resonances come into close contact with one another, and the surface plasmons in each nanoparticle begin to couple to those in others. Monte Carlo has been used to predict the equilibrium structures that appear due to this process. For instance, in the case of spherical nanoparticles, Monte Carlo has predicted that sheets, clusters, and other assemblies of nanoparticles are predominant, depending on various factors. For the case of nanorods, the particles generally form side-by-side aligned structures upon aggregation in polymer thin films, with an interparticle separation that can be modulated by varying the molecular weight of the grafted polymers. DDA is useful in these instances since the absorption and scattering of light can be calculated for representative structures that are either observed experimentally, or predicted from Monte Carlo simulations, for example. Hore et al. used a combination of Monte Carlo simulations, DDA calculations, and experiments to investigate the coupling between autophobic dewetting and the optical properties of polystyrene (PS)-functionalized Au nanorods within PS thin films. As seen in the optical spectra in Fig. 10.3, the theoretical results quantitatively capture many aspects of the experimental measurements, showing an increasing blue shift in absorption as nanorods become increasingly aggregated. However, because of the simplicity of the DDA calculations, the effects of polydispersity in the sample—both in terms of nanoparticle size and aggregate structure—are not effectively captured.

10 Predicting the Optical and Electrical Properties …

269

Fig. 10.3 (Left) UV-Vis absorption data for Au nanorod/polystyrene nanocomposites as a function of matrix degree of polymerization (P). As P increases, nanorods increasingly aggregate, leading to a blueshift in the absorption wavelength due to plasmonic coupling between nanoparticles. (Right) DDA calculations of the extinction efficiency of isolated rods, pairs of rods, and tetramers of rods to mimic increasing aggregation with molecular weight. The trends are in reasonable quantitative c agreement with experiments. Reproduced with permission from [17], Copyright 2014 American Chemical Society

10.2.3 Finite-Difference Time-Domain (FDTD) Method The finite-difference time-domain method was introduced in the mid-1960s by Yee [19] FDTD can be applied to obtain time-dependent solutions of the electric and magnetic fields for arbitrary systems. A major characteristic of FDTD is that the fields are staggered spatially and temporally. FDTD is best suited to modeling systems that do not exhibit strong resonances—a situation that would require a large number of iterations to fully describe the evolution of the fields. To illustrate the fundamentals of the FDTD approach, we briefly review it here, but for a full description, the interested reader should consult more complete texts, such as those by Sullivan, Schneider, and others [20, 21]. In addition, several commercial and open source software packages exist that implement FDTD, including Lumerical, Angora, MEEP, and many others. 10.2.3.1

Theoretical Background

As its name suggests, FDTD is a finite difference technique that is solved numerically on a grid. Because of this, it is can be trivially parallelized for multi-core CPUs and GPUs using MPI/OpenMP, or CUDA/OpenCL, respectively. Implementation of FDTD requires the use of a Yee cell, which represents the manner in which the electric (E) and magnetic fields (B) are related to one another spatially. In the case of polymer nanocomposites, FDTD may be used to calculate the local electric and magnetic fields for analyzing materials for surface-enhanced Raman spectroscopy (SERS) applications, the reflectance/transmittance of a nanocomposite, or features relating to plasmonics such as the extinction cross section. The Yee cell describes a particular manner in which to co-locate the E and B fields onto a cubic lattice. For each cubic cell, which is labeled by three indices lmn,

270

M. J. A. Hore

(l+1,m+1,n)

(l,m+1,n)

(l,m,n)

y

(l+1,m,n)

x

z

Fig. 10.4 Schematic of the Yee cell describing the positions of the electric and magnetic fields in an FDTD calculation. The electric and magnetic fields are staggered in space

the components of E are placed at the midpoint of each edge of the cube, while the components of B are placed in the centers of each face of the cube. This is shown schematically in Fig. 10.4. The Yee cell staggers E and B in space, and guarantees that each point of E is surrounded by components of B, and vice versa. The Yee cell satisfies the two divergence conditions in the macroscopic definition of Maxwell’s equations: ∇ ·H=0 (10.20) ∇ ·E=

ρ ε0

(10.21)

To completely describe the system of interest, knowledge of the conductivities and dielectric responses of each of the material components is necessary. The remaining Maxwell equations (i.e., the “curl equations”) yield the time evolution of the E and H fields: 1 ∂E = ∇ ×H (10.22) ∂t ε0 1 ∂H =− ∇ ×E ∂t μ0

(10.23)

Note that (10.22) neglects the presence of any current density J that may appear in the system, and that μ0 H = B. μ0 is the vacuum permeability. In addition, to perform

10 Predicting the Optical and Electrical Properties …

271

the calculation for a real material, the dielectric constants ε of the material must also be accounted for in (10.22). As a brief example of the implementation of FDTD using the concept of a Yee cell, consider applying FDTD in one dimension, for simplicity. In one dimension, (10.22) and (10.23) reduce to: 1 ∂Hy ∂Ex =− ∂t ε0 ∂z

(10.24)

∂Hy 1 ∂Ex =− ∂t μ0 ∂z

(10.25)

To solve (10.24) and (10.25) numerically, both the spatial and temporal derivatives are replaced by finite differences, resulting in: τ +1/2

Ex

τ −1/2

(n) − Ex t

(n)

1 1 1 Hyτ n + 2 − Hyτ n − 2 =− ε0 x

Hyτ +1 n + 21 − Hyτ n + 21 t

τ +1/2

=−

1 Ex μ0

τ +1/2

(n + 1) − Ex x

(10.26) (n)

(10.27)

where n is an index on the Yee cell in the z-direction (cf., Fig. 10.4), τ is the current time step, t is the size of a time step, and x is the lattice spacing. These equations can be cast in another form which provides update equations for the E and H fields: Exτ +1/2 (n) = Exτ −1/2 (n) − Hyτ +1

1 1 t Hyτ n + − Hyτ n − ε0 x 2 2

1 1 t τ +1/2 τ n+ = Hy n + − E (n + 1) − Exτ +1/2 (n) 2 2 μ0 x x

(10.28)

(10.29)

To perform the FDTD calculation, (10.28) and (10.29) are iterated in time τ for each lattice site n to trace the evolution of the fields within the system. Note that the staggered configuration of the Yee cell results in a staggering of the solutions in both time in space. For instance, the electric field E at site n is determined at time (τ + 1/2) using the previous value of E at (τ − 1/2) along with the magnetic field H at staggered lattice sites (n + 1/2) and (n − 1/2). The new value of H at time (τ + 1) is then determined from its value at time τ and the values of the electric field at time (τ + 1/2). The calculation proceeds in this staggered fashion until the desired temporal evolution of the fields is captured in the calculation. For this reason, strongly resonating systems will typically require a large number of iterations of (10.28) and (10.29) to fully capture the temporal evolution of the system, which may be prohibitively expensive from a computational standpoint. The extension from one dimension to three dimensions follows a similar procedure as shown above.

272

M. J. A. Hore

Although the process outlined above is relatively straightforward, in practice there are several additional considerations that must be taken into account to accurately model a polymer nanocomposite. First, the choices of x and t must be chosen to ensure that the calculation is stable and accurate captures the propagation of any electromagnetic waves. In √ particular, to account for the finite speed of light, t is chosen to be t = x/ nc, where c is the speed of light in a vacuum and n is the dimensionality of the system. In addition to these values, the boundaries of the calculation must be treated to, for example, absorb outgoing radiation. A commonly used boundary is the perfectly matched layer (PML), which absorbs radiation at the boundary to prevent unphysical reflections back into the system of interest. To analyze scattering of incident radiation by objects, it is common to use the total field/scattered field (TF/SF) source to separate outgoing electromagnetic radiation from an incoming plane wave. The scattering and absorption cross sections are calculated from the absorbed power (Pabs ) of the total field and the power of the scattered field (Psca ) as Csca =

Psca P0

(10.30)

Cabs =

Pabs P0

(10.31)

where P0 is the power of the incident plane wave [22]. The total extinction cross section is the sum of the two contributions, Cext = Csca + Cabs . In practice, to analyze the scattering of electromagnetic radiation by a polymer nanocomposite, one would interrogate the material by subjecting it to pulses of different wavelengths and polarizations, and recording the average scattering and absorption at each wavelength.

10.2.3.2

Examples from the Literature

As with DDA, FDTD calculations have been used throughout the scientific literature to predict the optical properties of polymer nanocomposites. As one example that combines multiple theoretical techniques to understand a polymer nanocomposite, Wang et al. used FDTD to predict the plasmonic properties of Au nanorod/polystyrene composites as a function of nanorod separation and nanorod size [23]. The authors of this work combined experiments with self-consistent field theory (SCFT) calculations to demonstrate that the particles were more likely to aggregate as the polymer matrix molecular weight increased and/or the nanorod length increased. By analyzing the interparticle spacing from scanning electron microscopy (SEM) images, the authors found that nanoparticles exhibited a very uniform spacing of ca. 35 nm upon aggregation. Using this value for the interparticle separation, FDTD calculations were able to quantitatively reproduce the extinction characteristics of the nanocomposites by considering the scattering and absorption of incident radiation by a pair of Au nanorods. In this case, though, FDTD did not provide any particular advan-

10 Predicting the Optical and Electrical Properties …

273

tage over DDA calculations, and the results of the two techniques were quite similar [17, 23]. In more complex situations, FDTD provides significant advantages over DDA in that it can accurately reproduce many aspects of the electromagnetic field. In a related example, Glor et al. used a combination of ellipsometry and FDTD calculations to probe the out-of-plane alignment and reorientation dynamics of Au nanorods that were embedded in a PMMA thin film [24]. FDTD calculations allowed the authors to determine the polarizability of a Au nanorod from the electric near-field distribution, and compare to ellipsometry measurements to determine the average angle between the nanorod orientation and that of the film/substrate. Another study by Wu et al. investigated the optical properties of cylinder-forming polystyrene-b-poly(4-vinyl pyridine) (PS-b-P4VP) films with Au or Ag nanoparticles within the cylindrical P4VP phase, with the objective of using the material as a meta-lens [25]. The distribution of nanoparticles within the cylindrical phases caused negative refraction of incident light, and FDTD calculations demonstrated the material could focus the light and split the beam.

10.3 Calculation of Electrical Properties Beyond predicting the interaction of a nanocomposite with light, predicting the electrical properties, such as conductivity/resistance, of a polymer nanocomposite has garnered considerable attention. The desire to mass produce flexible electronics, for instance, has motivated the design and development of transparent conductor technologies. Calculation of electrical conductivity in polymer nanocomposites is many times related to the concept of percolation of nanoparticles throughout a material. In the case of anisotropic nanoparticles such as carbon nanotubes, nanowires, or nanorods the percolation threshold may be low—especially as the aspect ratio ν = L/D increases. At and after percolation, conductive nanoparticles form one or more continuous, conductive paths through the material—leading to enhanced electrical conductivity.

10.3.1 Resistor Network Models 10.3.1.1

Theoretical Background

A common approach to modeling the electrical conductivity of a polymer nanocomposite is to co-locate structural information onto a simple cubic (3D) or square (2D) mesh of spacing r, and apply finite-difference techniques to determine the current through the material [26]. This “resistor network model” approach assumes that at each grid point r within the system, the material is either conducting or nonconducting, and described by a conductivity σ (r) at each point. In this case, structural

274

M. J. A. Hore

Fig. 10.5 Example of a 2D mesh, with mesh size r, containing a percolating network of nanowires of length L = 3 r in 2D (shown in black). The regions of the mesh containing nanowires have electrical conductivities σNP , while the surrounding polymer matrix (white regions) have conductivities σP . A potential difference of V0 is applied across the material

information used to construct the arrangement of σ (r) may come from Monte Carlo, coarse-grained particle dynamics models, or other techniques. This representation is illustrated in Fig. 10.5. Given the spatial distribution of σ , the current J(r) can be calculated at each point through the system according to J(r) = σ (r)∇V (r)

(10.32)

subject to the condition that at each point ∇ · J(r) = 0. This condition is equivalent to Kirchhoff’s Law, stating that at each grid point i surrounded by points j,

G ij (Vi − Vj ) = 0

(10.33)

r σ (ri ) + σ (rj ) 2

(10.34)

j

where the conductance G ij =

The resulting physical system, and its interpretation in terms of a resistor network, can be seen in Fig. 10.6. Once the spatial dependence of σ (r) is known, the current is calculated by applying the appropriate boundary conditions. A common approach is to set the voltage at a constant value of V = V0 on one end of the system and V = 0 on the opposite end. After application of the boundary conditions, (10.34) can be evaluated at each grid

10 Predicting the Optical and Electrical Properties …

275

Fig. 10.6 Illustration of the translation of a carbon nanotube nanocomposite into a resistor network. c Reproduced with permission from [27], Copyright 2008 Elsevier

point to produce the conductance throughout the system, followed by the evaluation of (10.33) to obtain the voltage Vi at each point. A convenient, equivalent form of (10.33) is given by j G ij Vj (10.35) Vi = j G ij which implies a system of linear equations that can be solved with standard linear algebra techniques and software libraries. Finally, the current through the material can be calculated by evaluating I=

G ij (Vi − Vj )

(10.36)

j

for all points i at the boundary of the system [28].

10.3.1.2

Examples from the Literature

Resistor network models have been successful in describing the electrical behavior of several classes of polymer nanocomposites, including Ag nanowire nanocomposites, carbon nanotube (CNT) nanocomposites, graphene nanocomposites, and others. Hu et al. used a resistor network to model piezoresistance in CNT/epoxy nanocomposites, demonstrating that near the percolation threshold, CNT nanocomposites were more sensitive than more traditional strain gauges [27]. Dalmas et al. showed that this approach is also valid for curved, conductive fibrous networks, while others have shown its applicability to understand the effects of shear flow on electrical conductivity [29, 30]. Work from Winey et al. has used this model to quantify the conductivity of Ag nanowire composites, connecting both simulations and experimental measurements [31–33]. In a study by White et al., nanowire morphologies were generated randomly, and the conductivity through the nanocomposite was evaluated using a resistor net-

276

M. J. A. Hore

Fig. 10.7 (Left) Simulated morphologies of nanowires within a polymer nanocomposite as a function of their orientational order parameter S. (Right) Simulated nanocomposite conductivities from a resistor network model for nanowires as a function of S. The numbers to the right of each curve indicate the volume fraction of nanowires in each system. Reproduced with permission from [31], c Copyright 2009 American Physical Society

work model. As shown in Fig. 10.7, as the volume fraction of nanowires increased, their orientational order S increased, resulting in an increase in electrical conductivity. Amjadi and coworkers also employed a resistor network model to predict the performance of Ag nanowire/elastomer composites when used as strain sensors [34]. More recent work from Kwon et al. combined coarse-grained molecular dynamics simulations with a resistor network model to investigate the effect of nanoparticle shape and flexibility on the conductivity of polymer nanocomposites [35].

10.3.2 The Poisson-Nernst-Planck (PNP) Formalism Although its use in the polymer nanocomposite field is not as widespread as in others, the Poisson-Nernst-Planck (PNP) formalism has shown promise as a reliable method to model ionic transport phenomena in a number of systems, such as with polymer membranes or solid-state nanochannels. In addition, it has been widely employed to interpret experimental investigations of polymer translocation. Looking to the future, this technique may be a viable approach for predicting and understanding macroscopic ionic currents from structural simulations of ionomer melts, for example. In taking such an approach, it is key to assume that the timescales of ionic motions are much faster than those of the surrounding polymers and nanoparticles. In other words, one must assume the polymers and nanoparticles are essentially stationary. In the solution state, as is the case when modeling polymer translocation, this assumption is typically true. However, in the melt state, this assumption may or may not apply, and so future researchers must take this into account.

10 Predicting the Optical and Electrical Properties …

10.3.2.1

277

Theoretical Background

At its core, PNP is a mean-field theory that couples the Poisson equation for the spatial distribution of electrostatic potential (φ) to the Nernst-Planck equation for predicting ion transport in response to that potential. Characteristic to the PNP approach is selfconsistently solving the Poisson and Nernst-Planck equations on a grid until the desired level of error is achieved. In a typical implementation, the electrostatic potential is first determined by solving the Poisson or linearized Poisson-Boltzman equation subject to the system’s boundary conditions. For the case using the Poisson equation as an initial guess, ∇ · ε(r)∇φ = −

ρ ε0

(10.37)

where ε(r) captures the spatial dependence of the dielectric constant throughout the system, and ρ is the charge density in the system. Note that ρ may contain both mobile charge density due to ions in the system, and fixed charges due to charged interfaces, etc. In aqueous systems, a commonly made approximation is that ε(r) = 80 for regions containing solvent, and ε(r) = 2 for insulating regions such as those composed of silicon nitrides, polymers, proteins, and the like. Lenart and coworkers recently used PNP theory to model ion transport through dendritic nanoparticles, and characterized the permeability of the nanoparticles by a hardness parameter hNP . Under this approximation, the dielectric constant of regions containing the nanoparticles was calculated as ε(r) = hNP × 2 + (1 − hNP ) × 80, where the hardness parameter 0 ≤ hNP ≤ 1 [36]. At the boundaries of the system, a typical strategy is to apply a combination of periodic and/or Dirichlet boundary conditions to fix the value of the electrostatic potential φ. Starting from a uniform value of φ = 0, the Poisson equation can be solved to arbitrary precision through a successive over-relaxation (SOR) algorithm, where each new iteration of the potential at grid point i, φin+1 , can be expressed in terms of the current value of the potential φin as: φin+1 = φ˜i + (1 − λ)φin where the value

⎛ φ˜i = ⎝

j

⎞ ⎛ ⎞ 2ε ε 2ε ε i j i j ⎠ ⎝ ⎠ φjn εi + εj ε + εj i j

(10.38)

(10.39)

with elements j being all adjacent points in the mesh [37]. Typically this process is iterated until the relative difference between φ n+1 and φ n is less than 10−8 . The initial value of the electrostatic potential is then used to solve the NernstPlanck equation, Di Zi ci (r)∇φ(r) = 0 (10.40) ∇ · Di ∇ci (r) + kB T

278

M. J. A. Hore

where Di and ci are the diffusion coefficients and concentrations, respectively, of ion type i, and Zi is the charge carried by that ion. To more easily solve the Nernst-Planck equation, it can be converted into a form that resembles a Laplace-like equation through a Slotboom transformation: [38] Zi φ(r) ψi (r) = Ci exp − kB T

(10.41)

∇ · εeff ,i ∇ψi (r) = 0

(10.42)

leading to the equation The new dielectric-like function εeff ,i contains the diffusion coefficients Zi φ(r) εeff ,i (r) = Di exp − kB T

(10.43)

The Nernst-Planck equation is solved to desired accuracy using the same approach outlined above for the Poisson equation. Typically, it is solved iteratively using an SOR approach until the error is on the order of 10−7 , after which the Poisson equation is solved using the newly determined concentration profiles. This self-consistent solution is repeated until the error in both equations is satisfactory. After obtaining a solution for φ(r) and ci (r), the ionic currents and ion fluxes can be calculated from the Nernst-Planck solution, i.e., ci (r)Zi ∇φ(r) (10.44) ji (r) = −Di ∇ci (r) + kB T 10.3.2.2

Examples from the Literature

Examples applying the PNP formalism to understand polymer nanocomposites are rare in the literature—if they exist at all. However, several relevant studies do exist showing the applicability of this technique to understanding such materials. Meng et al. used PNP calculations to predict Li+ conductivity in confined environments, such as in thin films of solid electrolyte [39]. Chan and coworkers also used PNP calculations to investigate the formation of ionic layers between graphene sheets, with the goal of understanding the flow of Li ions in the system [40].

10.4 Summary and Outlook Looking to the future, polymer nanocomposites are likely to continue to enable new technologies and materials due to a large palette of particle types/functionalities, polymer materials, and self-assembly strategies. At this juncture, a mature suite

10 Predicting the Optical and Electrical Properties …

279

of computational tools exists for predicting structural information in polymer nanocomposites—including molecular dynamics (MD), Monte Carlo (MC), dissipative particle dynamics (DPD), polymer field theory, and many others—that have been experimentally-validated under a number of conditions. In many instances, these techniques are suitable for coupling to others, like those described in this chapter, for calculating optical, electrical, and ionic transport characteristics in polymer nanocomposites. In fact, several examples exist in the literature that do exactly this, and it is likely that this approach will continue to be successful going forward. In addition, the advancement of computer hardware, most notably the graphical processing unit (GPU), has significantly increased the speed with which these calculations can be performed. Many of the techniques discussed in this chapter are, at their core, finite-element techniques that can be trivially parallelized on GPU hardware. This in itself may enable more efficient computing of both nanocomposite structure and optical/electrical properties when those techniques are coupled to one another, and is sure to significantly advance our understanding of polymer nanocomposites and their physical properties. Acknowledgements This work was supported in part by a National Science Foundation CAREER Award (DMR-1651002). The identification of software packages does not imply endorsement, nor that these are necessarily the best for a given purpose.

References 1. 2. 3. 4. 5. 6. 7. 8. 9. 10. 11. 12. 13. 14. 15. 16.

17. 18. 19.

S.K. Kumar, N. Jouault, B. Benicewicz, T. Neely, Macromolecules 46, 3199–3124 (2013) M. Moniruzzaman, K.I. Winey, Macromolecules 39, 5194–5205 (2006) M.J.A. Hore, R.J. Composto, Macromolecules 47, 875 (2013) S.A. Maier, Plasmonics: Fundamentals and Applications, 1st edn. (Springer, New York, 2007), pp. 65–87 C.F. Bohren, D.R. Huffman, Absorption and Scattering of Light by Small Particles, 1st end (John Wiley & Sons, New York, 1998) R.J. Martin, J. Modern Optics 40, 2467 (1993) B. Hourahine, K. Holms, F. Papoff, J. Phys.: Conf. Ser. 367, 012010 (2012) A. Dang, S. Ojha, C.M. Hui, C. Mahoney, K. Matyjaszewski, M.R. Bockstaller, Langmuir 30, 14434 (2014) A. Incel, T. Güner, O. Parlak, M.M. Demir, A.C.S. Appl, Mater. Interf. 7, 27539–27546 (2015) V.A. Markel, J. Optical Soc. Am. A 33, 1244 (2016) D.B. Stojanovi´c, L. Brajovi´c, D. Dramli´c, V. Radmilovi´c, P. Uskovo´c, R. Aleksi´c, Prog. Org. Coatings 76, 626 (2013) W.R. Lenart, M.J.A. Hore, Nano-Structures & Nano-Objects 16, 428 (2018) E.M. Purcell, C.R. Pennypacker, Astrophys. J. 186, 705 (1973) P.K. Jain, W. Huang, M.A. El-Sayed, Nano Lett. 7, 2080 (2007) A.M. Funston, C. Novo, T.J. Davis, P. Mulvaney, Nano Lett. 9, 1651 (2009) P. Akcora, H. Liu, S.K. Kumar, J. Moll, Y. Li, B.C. Benicewicz, L.S. Shadler, D. Acehan, A.Z. Panagiotopoulos, V.A. Pryamitsyn, V. Ganesan, J. Ilavsky, P. Thiyagarajan, R.H. Colby, J.F. Douglas, Nature Mater. 8, 354 (2009) M.J.A. Hore, A.L. Frischknecht, R.J. Composto, ACS Macro Lett. 1, 115 (2012) A.L. Frischknecht, M.J.A. Hore, J. Ford, R.J. Composto, Macromolecules 46, 2856 (2013) K. Yee, IEEE Trans. Antennas Propag. 14, 302 (1966)

280

M. J. A. Hore

20. D.M. Sullivan, Electromagnetic Simulation using the FDTD Method, 2nd edn. (Wiley, New Jersey, 2013) 21. J. B. Schneider, Understanding the Finite-Difference Time-Domain Method. 2017. http://www. eecs.wsu.edu/~schneidj/ufdtd. Date Accessed: Jan 2020 22. C. Tira, D. Tira, T. Simon, S. Astilean, J. Mol. Struc. 1072, 137–143 (2014) 23. D. Wang, M.J.A. Hore, X. Ye, C. Zheng, C.B. Murray, R.J. Composto, Soft Matter 10, 3404– 3413 (2014) 24. E.C. Glor, R.C. Ferrier, C. Li, R.J. Composto, Z. Fakhraai, Soft Matter 13, 2207 (2017) 25. L.Y.L. Wu, B. Leng, W. He, A. Bisht, C.C. Wong, 2013 IEEE 5th International Nanoelectronics Conference (INEC) (Singapore, 2013), pp. 393–396 26. S. Kirkpatrick, Rev. Mod. Phys. 45, 574 (1973) 27. N. Hu, Y. Karube, C. Yan, Z. Masuda, H. Fukunaga, Acta Mater. 56, 2929–2936 (2008) 28. N. Hu, Z. Masuda, C. Yan, G. Yamamoto, H. Fukunaga, T. Hasida, Nanotechnology 19, 215701 (2008) 29. F. Dalmas, R. Dendievel, L. Chazeau, J.-Y. Cavaillé, C. Gauthier, Acta Mater. 54, 2923–2931 (2006) 30. A.E. Eken, E.J. Tozzi, D.J. Klingenberg, W. Bauhofer, J. Appl. Phys. 109, 084342 (2011) 31. S.I. White, B.A. DiDonna, M. Mu, T.C. Lubensky, K.I. Winey, Phys. Rev. B 79, 024301 (2009) 32. S.I. White, R.M. Mutiso, P.M. Vora, D. Jahnke, S. Hsu, J.M. Kikkawa, J.E. Fischer, K.I. Winey, Adv. Func. Mater. 20, 2709–2716 (2010) 33. R.M. Mutiso, M.C. Sherrott, K.I. Winey, Phys. Rev. B 86, 214306 (2012) 34. M. Amjadi, A. Pichitpajongkit, S. Lee, S. Ryu, I. Park, ACS Nano 8, 5154–5163 (2014) 35. S. Kwon, H.W. Cho, G. Gwon, K. Kim, B.J. Sung, Phys. Rev. E 93, 032501 (2016) 36. W.R. Lenart, W. Kong, W.C. Oltjen, M.J.A. Hore, J. Mater. Chem. B 7, 6428–6437 37. D.S. Bolintineanu, A. Sayyed-Ahmad, H.T. Davis, Y.N. Kaznessis, PLoS Comput. Biol. 5, e100027 (2009) 38. J.W. Slotboom, Electron Lett. 5, 677–678 (1969) 39. D. Meng, B. Zheng, G. Lin, M.L. Sushko, Commun. Comput. Phys. 16, 1298–1322 (2014) 40. Y. Chan, M. Saeed, S.-L. Lee, J.J. Wylie, Sci. Rep. 9, 11712 (2019)

Chapter 11

Data-Driven Multiscale Science for Tire Compounding: Methods and Future Directions Hongyi Xu , Richard J. Sheridan , L. Catherine Brinson , Wei Chen , Bing Jiang, George Papakonstantopoulos, Patrycja Polinska , and Craig Burkhart Abstract Modern tire compound design is confronted with the simultaneous optimization of multiple performance properties, most of which have tradeoffs between the properties. In order to uncover new design principles to overcome these historical tradeoffs, multiscale compound experiment, physics, and simulation are being developed and integrated into next-generation design platforms across the tire industry. This chapter describes the efforts in our laboratories to quantify compound structures and properties at multiple scales—from nanometers to microns—and their application in compound simulations. This integration of experiment and simulation has been H. Xu Department of Mechanical Engineering, The University of Connecticut, Storrs, CT 06269, USA e-mail: [email protected] R. J. Sheridan · L. Catherine Brinson Department of Materials Science and Engineering, Duke University, Durham, NC 27708, USA e-mail: [email protected] L. Catherine Brinson e-mail: [email protected] W. Chen Department of Mechanical Engineering, Northwestern University, Evanston, IL 60208, USA e-mail: [email protected] B. Jiang · G. Papakonstantopoulos · C. Burkhart (B) Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, Akron, OH 44306, USA e-mail: [email protected] B. Jiang e-mail: [email protected] G. Papakonstantopoulos e-mail: [email protected] P. Polinska Global Materials Science, and Tire and Performance Science Divisions, The Goodyear Tire and Rubber Company, 7750 Colmar-Berg, Luxembourg e-mail: [email protected] © Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1_11

281

282

H. Xu et al.

found to be critical to highlighting the levers in data-driven multiscale compound design. We also provide a glimpse into the next set of capabilities, particularly from data science, which will impact future compound design.

11.1 Introduction In the face of global climate change, governments, research institutes and the automobile industry are pursuing strategies to reduce CO2 emissions from passenger and light-commercial vehicles. This effort requires complementary measures for car components which have a high impact on fuel consumption. Tires, which are the only vehicle component in direct contact with the ground, are responsible for 5–10% of the fuel consumption of a vehicle, mainly due to rolling resistance. The European Commission (EC) plans to reduce the total vehicle energy consumption by 30% by 2030 [1] compared to 2021 by targeting several actions, including tire labeling. The tire labeling regulation, shown in Fig. 11.1, comprises three performance areas: fuel efficiency, wet grip, and noise. Lowering a tire’s rolling resistance index will reduce fuel consumption, but on the other hand may have a negative influence on wet grip or other performance measures such as noise emissions. Optimizing these three areas simultaneously will require breaking through current tradeoffs into new material design frontiers.

Fig. 11.1 Tire labeling showing specifications for fuel efficiency, wet grip and noise. Reproduced from [1]

11 Data-Driven Multiscale Science for Tire Compounding …

283

While tire performance requires a complex interplay of design, compound science and manufacturing capability, the focus of this Chapter resides in compound science. From a materials standpoint, rubber compounds are complex materials, with chemical and structural features operating on multiple time and size scales. Compared to other materials-based industries, one of the differentiating aspects of tire technology is the time-tested sulfur vulcanization process which occurs during the manufacturing phase. This chemical process transforms the material properties from a flowing rubber formulation into a three-dimensional viscoelastic solid. In this step various additives (e.g., sulfur and accelerators) are dry-mixed and heated to affect crosslinking into an elastomeric network. The filler component achieves a reinforcement effect due to both physical interactions and additional chemical links with the elastomeric network [2–5], providing a large degree of strengthening of the rubber compound. Carbon blacks and amorphous silicas are the most widely used reinforcing nanofillers in the rubber industry. Without reinforcing fillers, tires would need to be replaced considerably more often, resulting in an increased burden on end-of-life-tire management, an increase in tire manufacturing energy requirements, as well as an increase in greenhouse gas emissions per vehicle unit-distance driven [6]. The mechanical properties of rubber compounds are dominated by a complex combination of multiscale chemistry and structure. The main structural entities include the vulcanized elastomer network (on the order of nanometers per crosslink), the filler-filler network (tens to hundreds of nanometers) and the filler-rubber interphase (tens of nanometers). The combination of the latter two structures creates the mechanical percolation network in a rubber compound. The most difficult structure to quantify is the filler-rubber interphase, which is formed by the mutual influences of the filler and rubber chemistries. This region of rubber surrounds the filler particles and has a mechanical response which may be strongly altered by its physical and/or chemical proximity to the filler surface. This structure has been investigated for over 50 years, sometimes being described in the compounding literature as “occluded rubber” [7]. Despite decades of indirect evidence and speculation, there exists limited direct mechanical evidence or visualization of such interphase properties. Experimental studies have recently indicated this interphase can extend from a few nanometers (nm) to over 50 nm [8, 9]. Understanding how these structures and scales interact with one another is critical to expanding current compound design frontiers.

11.1.1 Early Laboratory Compound Design Concepts The historical practice of compounding was, and still is, a somewhat empirical occupation. Nevertheless, this empirical grounding led to realizing the connection between laboratory dynamic mechanical properties and performance. In one of the seminal tread compounding design papers of the mid-1980s, Nordsiek [10], promoted the concept of viscoelastic properties as critical to tread (and tire) performance. Figure 11.2 demonstrates the design principles: a viscoelastic spectrum, in this case the normalized energy loss, tan δ, is swept as a function of temperature. The

284

H. Xu et al.

Fig. 11.2 Integral rubber concept. Tread performance is determined by temperature/frequency windows in tan δ spectra. Reproduced with permission from [10]. Copyright (1985) Huthig GmbH

breakthrough concept involved the realization of different temperature windows could be mapped onto various tread performance properties. In principle, one could tune each performance behavior—rolling resistance, wet traction, cold weather traction, by optimizing the tan δ spectrum in each window. Variants of this design principle are still used today. Despite the obvious utility of this design idea, two major problems require resolution: (1) Next-neighbor performance regions, such as rolling resistance and wet traction, are difficult to decouple without chemical and structural intuition; (2) Given the very large recipe design space, it is not clear how compound recipe ingredients have to be selected and formulated to optimize each property. These problems have been traditionally solved by expert compounders, who by their experience and training map formulations onto properties. In reality, reducing this design knowledge to a quantitative physicochemical basis requires many domain knowledge sets: rubber chemistry and structure; filler chemistry, its structure and surface area; coupling agent chemistries for fillers with functional surfaces; the resultant filler-rubber interactions; sulfur vulcanization chemistry and its crosslinking networks; and finally, a computational platform which integrates such chemical and physical structures and properties into predictions. These domains must be mustered into a cohesive knowledge ecosystem in order to reveal deeper compound design principles. A promising direction for merging these design needs is offered by the development of multiscale science, which incorporates high fidelity experiment, modeling and simulation as core knowledge resources in a data science framework. This field

11 Data-Driven Multiscale Science for Tire Compounding …

285

has emerged as one of the focal research areas in tire technology. Multiscale methods integrate, guide and optimize internal structure, and therefore provide design levers to understand and control material performance at multiple scales. Such qualities make this design approach highly attractive for next-generation rubber compounds. Driven by some of the advances outlined in this Chapter, recent developments of nanoscale experimental characterization methods as well as computational infrastructure are opening the way for the detailed elucidation of the fundamental compound structures and properties responsible for primary tire performance.

11.1.2 Chapter Scope In Sect. 11.2, we present an overview of the data-driven experimental, mathematical, and computational tools which have been developed in our laboratories to understand nanoparticle-filled rubber composites. The linear viscoelastic properties of carbon-black-filled styrene-butadiene rubber composites are measured using dynamic mechanical analyses, and the resulting viscoelastic spectra are compared to simple models which ignore nanoscale structure such as particle distribution and interphase. Techniques to reconstruct compound filler microstructure are described, based on N-point correlation functions and particle descriptors. A computational analysis of the generation of representative volume elements (RVE) is presented, and an optimal statistical reconstruction is demonstrated. The interphase structure is then inferred based on the reconstruction of the viscoelastic measurement by optimization. Finally, in Sect. 11.3, we give a glimpse into near-term future directions. Going forward, the integration of experimental, physics-based simulation and machine learning design methods are seen as critical for future compound design practices. Data science is central in the integration of multidisciplinary tire compounding environment. We see the development of these capabilities as critical to modern adaptive design approaches.

11.2 Methods Framework We present a framework for the computational design of viscoelastic nanoparticle composites in order to achieve optimal material properties which cannot readily be found by traditional trial-and-error approaches. This framework integrates knowledge from experimental tests into well-defined numerical microstructure models to predict the properties of the nanocomposite. Specifically, a microstructure model is established to capture the complex microstructure characteristics of the composites, the properties of each phase in the microstructure is obtained from experimental tests, and simulations for overall response prediction demonstrate agreement with validation tests.

286

H. Xu et al.

Dynamic mechanical analysis (DMA) is an established macro-scale technique to interrogate the linear viscoelastic response of materials through a gentle application of oscillatory strain while monitoring the force transmitted through a specimen in real time [11]. Using the principle of time–temperature superposition (TTS), the smalldeformation mechanical response in terms of the complex modulus E* or the loss tangent tan δ can be evaluated over many decades of frequency. Here, we use the tan δ peak as a characteristic marker of the glass transition, whether in the temperature or frequency domain. This provides a geometry- and material-agnostic point in the viscoelastic spectrum that can be tracked with high precision and accuracy. Here we focus on a carbon-black-filled styrene-butadiene rubber (CB-SBR) composite [8]. Experimental DMA data from this system at various composite loadings is displayed in Fig. 11.3a, b, plotted in the temperature domain and frequency domain, respectively. The viscoelastic spectrum is a strong function of particle loading, and the tan δ peak is a particularly sensitive measure of changes in viscoelastic behavior. Note that a shift of the tan δ in temperature space moves opposite to the corresponding shift of tan δ in the frequency space. The change of tan δ with filler has been observed in a variety of systems by many independent groups—some of that change is due to the inherent elasticity of the filler itself, but the complete response is more complex [12–21]. Interactions between the nanofillers and

Fig. 11.3 Dynamic mechanical analysis (DMA) is a common experimental technique for determining viscoelastic properties of polymer-based materials. Experimental set-up (a). The tan δ spectra represented in the temperature (b) and frequency domains (c); each curve represents one sample and is not averaged. Corresponding glass transition temperature (T g ) shifts are plotted to show a shift towards higher temperatures at ∼9 vol% followed by a shift towards lower temperatures (d) [8]. Adapted with permission from [8, 23]. Copyright (2012, 2016) Elsevier BV

11 Data-Driven Multiscale Science for Tire Compounding …

287

the surrounding polymer chains alter the mobility of these polymer chains, resulting in a regime of “interphase” polymer, in which the material properties differ from the bulk matrix. Due to the high surface-to-volume ratio of nanofillers, the effects of this special region play an important role in the overall properties of nanocomposites, especially viscoelastic responses. Experimental observations have shown that the storage/loss modulus curve may be broadened or shifted in the time/temperature domain [22]. Since the properties of fillers are not time dependent, much of the improvement in the composite properties is ascribed to the interphase region. We will follow the study of Wood et al. [23] as an example and demonstration of the method to model tan δ shifts as a mechanical phenomenon due to the presence of filler and interphase.

11.2.1 Simple Representations of Filled Soft Composites 11.2.1.1

1D Scalar Models

The extent to which this CB-SBR compound can be modeled with very simple approaches should first be established. Wood [23] showed that a one-dimensional model of the system comprised of a perfectly elastic material (representing the carbon filler) in series with a Prony series material (representing the polymer matrix) is sufficient to recapitulate a tan δ shift to lower temperatures at high volume fractions (consistent with the shift to higher frequencies illustrated in Fig. 11.4). This shift in the tan δ peak occurs in the model when the particle modulus is substantially higher than the matrix modulus and represents the natural influence of the elastic particle on the relaxation behavior of the composite compared to the neat polymer.

Fig. 11.4 A one-dimensional model is constructed that models an elastomeric composite with increasing volume fraction using an elastic spring in series with a 27 unit Prony series (a). When the particles are introduced (>0 vol%), the tan δ peaks shifts immediately to higher frequencies and reduces in magnitude. The magnitude of this shift and the drop in the maximum of tan δ is tied to the stiffness of the particle phase, 5 GPa (b) and 50 GPa (c). The shifting with increasing particle volume fraction is consistently towards increasing ‘relaxation frequency’ and thus decreasing relaxation time. Adapted with permission from [23]. Copyright (2016) Elsevier BV

288

H. Xu et al.

No interphase is considered or necessary to obtain this shift in relaxation spectra toward shorter relaxation times. See Fig. 11.4.

11.2.1.2

3D Uniform Models

Although a one-dimensional model recovers important aspects of the experimental data and illustrates the essential effect of the elastic filler alone, several aspects must still be modeled, including the sensitivity of the tan δ peak position to volume fraction, microstructure and the behavior of the overall viscoelastic spectrum beyond the peak position. To increase the realism of the system, Wood created a threedimensional finite element (FE) model that was otherwise comparable to the 1D model. A representative volume element (RVE) was generated by dispersing particle elements in a cube of matrix elements in a uniform, random spatial distribution. For several RVEs constructed this way with varying filler fractions, the viscoelastic spectrum was calculated. The location of the tan δ peak in temperature space for these models also decreases, but with a less strong dependence on filler volume fraction than the one-dimensional models, and more in-line with the experimental result. See Fig. 11.5. In these models of elastic filler in a viscoelastic matrix, the temperature dependence of the tan δ peak monotonically decreased with increasing filler content, which fails to recover the initial increase at lower filler levels illustrated in Fig. 11.3 and other experimental data. In order to bridge this gap, additional realism was injected into the models by using a representative, reconstructed microstructure to account for particle distribution, following Deng et al. [8], and adding contributions from interphase [24, 25] polymer in the vicinity of the filler particles with altered relaxation times.

Fig. 11.5 A three-dimensional finite element model was constructed to represent a realistic tan δ behavior as particles concentration increases. The results—storage/loss modulus in (a) and tan δ in (b)—show a progressive shifting mechanism that both reduces tan δ magnitude and shifts the peak to higher frequencies (c). The tan δ shift to higher frequencies corresponds to a shift to lower temperatures (d, e). Adapted with permission from [23]. Copyright (2016) Elsevier BV

11 Data-Driven Multiscale Science for Tire Compounding …

289

11.2.2 Filler Microstructure Statistical Characterization and Stochastic Reconstruction The information of microstructure obtained in experimental observation is usually in the form of 2D image that cannot be used directly in material analysis and design due to the necessity of using 3D digital microstructure in material property analysis in order to obtain high accuracy in simulation results. The techniques of microstructure characterization are able to abstract quantitative descriptors from the image. Such descriptors are considered as the potential design variables due to their capability of capturing the key statistical features of the microstructure. Taken the prespecified descriptors as inputs, the reconstruction techniques generate multiple statistically equivalent random microstructure samples, which are passed into the material property analysis to obtain the microstructure-property relation. There have been many other modeling frameworks for nanocomposites, operating at various length scales and with various assumptions [26–37]. However, none of these attempts to model the spatial distribution of particles, have shown a strong effect on the final properties of a composite [22, 38–40]. The understanding of these microstructure-property relationships appears to be necessary for composite material design. To create an accurate representation of microstructure, a method is needed to generate FE geometries from experimental data taken from the samples of interest. Among nanoscale imaging techniques that provide sufficient spatial resolution, scanning and transmission electron microscopy (SEM and TEM, respectively) also have contrast in the CB-SBR system suitable for classifying pixels as either filler or matrix using simple binarization algorithms. It is possible to create FE geometries the directly from the binarized sample images, however a more rigorous and robust strategy is to “learn” the underlying particle distribution properties and generate new statistically representative samples for simulation, rather than testing a large number of specimens directly to gather statistics. Finally, with the geometry generated, it is possible to fit an interphase (size, shape, properties) to match DMA results from real composites. There are several published works using this strategy [41, 42] but we will follow Deng et al. [8] as an example here to introduce the framework, outlined in Fig. 11.6.

11.2.2.1

Microstructure Characterization and Reconstruction Based on Correlation Functions

The most widely used microstructure reconstruction techniques rely on the 2-point correlation function, which is defined as (in a two-phase random media): S2i (x1 , x2 ) ≡ I (i) (x1 )I (i) (x2 )

(11.1)

290

H. Xu et al.

Fig. 11.6 The basic framework of data-driven modeling methods (“target” refers to the correlations of the digitized medium, “actual” are the correlations of reconstructed material). Adapted with permission from [8]. Copyright (2012) Elsevier BV

where I is an indicator function: (i)

I (x) =

1, x ∈ phase 1 0, x ∈ phase 0

(11.2)

The physical meaning of the two-point correlation function is the probability of finding two points with a given distance r in the same phase of the random media. Therefore, two-point correlation is a function of distance r, and it can be denoted as S2i (r ). r can be any value from 0 to infinity, so the 2-point correlation function is usually truncated to a finite length by the microstructure image window size. Based upon the definition, a two-point correlation function should follow several boundary conditions [43]: • If r = 0, S2i (r ) equals to the volume fraction of composite; • If r → ∞, S2i (r ) approaches to the square of volume fraction; • The derivative of S2i (r ) at r = 0 is equal to the surface area per unit volume. Even though high accuracy can be obtained using 2-point correlation functions in microstructure characterization and reconstruction, the following challenges need further research efforts:

11 Data-Driven Multiscale Science for Tire Compounding …

291

• The computational cost of microstructure reconstruction using 2-point correlation function is usually very high due to the large number of optimization iterations which adjust the image pixel by pixel in order to match the target 2-point correlation function. The high cost makes it impractical to apply this method on high-resolution image with a large window size, or reconstruction in dimension spaces higher than 2D. • The vague physical meaning of the 2-point correlation function makes it hard to be used as design variables for microstructure. It is also difficult to relate the 2-point correlation function to the physics-based processing-microstructure model, the output of which is usually in the form of microstructure descriptors such as volume fraction, cluster number, radius, etc. Besides, a large amount of material analysis/design works have been done based on 2-point correlation function [43–45] or microstructure descriptors [46, 47]. A unified microstructure characterization and reconstruction technique is needed to relate these works with each other such that researchers can utilize existing data more efficiently. Similarly, we can define other types of correlation functions (Fig. 11.7) [48– 50]. The cluster correlation C2i is defined as the probability that finding two points with a distance r within one cluster of the filler phase. The surface correlation is defined as the probability that finding two points with a distance r located on the boundary of the filler phase. Surface correlations capture the morphology of interphase. The lineal path correlation is the probability that an entire line of length r lies in the filler phase. Different correlation function emphasizes on different aspects of microstructure features. In this work, the digital microstructure image is represented by a 0–1 binary matrix. “1” represents filler, and “0” represents matrix. The purpose of characterization is to quantify the distribution status of “1” pixels in the space. There are two methods of evaluating correlation functions:

Fig. 11.7 Definition of different types of correlation functions

292

H. Xu et al.

(1) The method using pixel-pixel distance histogram. This method follows the definition that 2-point correlation function is the normalized probability of finding two “1” pixels of distance r. Firstly, we calculate the distances between any two “1” pixels in the image. Based on the “1” pixel-pixel distance list, we obtain a frequency vector (histogram) of the pixel-pixel distance counts (how many pixel-pixel distances of 1, 2, 3 … are observed from phase “1” in the image), which is noted as: H r = n|I (i) (x) = 1, I ( j) (x) = 1 , i, j = 1, 2, 3, . . . , n = 0, 1, 2, . . . (11.3) where n is the distance between two pixels. The non-integer √ distances (e.g., the distance between two pixels on the diagonal direction is 2n) are rounded into the closest integer. i, j represents different “1” pixels. (2) We calculate the distances between any two pixels in the image (no matter “1” and “0”). Based on the pixel-pixel distance list, we obtain a frequency vector (histogram) of the pixel-pixel distance counts (how many pixel-pixel distances of 1, 2, 3 are observed from the entire image), which is noted as: H r = n|I (i) (x) = 1 or 0, I ( j) (x) = 1 or 0 , i, j = 1, 2, 3, . . . , n = 0, 1, 2, . . . (11.4) where n is the distance between two pixels. The non-integer √ distances (e.g., the distance between two pixels on the diagonal direction is 2n) are rounded into different pixels (regardless of its value). the closest integer. i, j represents the number of pixel-pixel distance H r = n|I (i) (x) = 1, I ( j) (x) = 1 represents r = n we can observe in “1” phase; H r = n|I (i) (x) = 1 or 0, I ( j) (x) = 1 or 0 represents the highest possible number of pixel-pixel distance r = n we can observe in the entire image regardless of the value of pixels. Therefore, we can calculate the 2-point correlation function as: S2i (r

= n) =

H r = n|I (i) (x) = 1, I ( j) (x) = 1

, H r = n|I (i) (x) = 1 or 0, I ( j) (x) = 1 or 0

i, j = 1, 2, 3, . . . , n = 0, 1, 2, . . .

(11.5)

Microstructure reconstruction is an inverse problem. It can be naturally formulated as an optimization problem as shown in (11.6), where the discrepancies between the target statistical descriptors and that of a reconstructed image are minimized. For example, if the two-point correlation and two-point cluster correlation are used, the resulting optimization formulation can be written as: E=

r

S2i (r )

−

2 i S 2 (r )

2

i i + C2 (r ) − C 2 (r )

(11.6)

11 Data-Driven Multiscale Science for Tire Compounding … i

293

i

where S 2 and C 2 are the resultant correlations of the reconstructed digitized medium at each of the discrete distance values r used in computationally determining the correlation functions. S2i and C2i are thus the target correlations to be realized. E is a fictitious “energy”, in this case a multicomponent cost function, and is defined as a sum of squared differences between target correlations and those calculated from a generated microstructure. Therefore, the smaller the fictitious energy E, the closer the reconstructed microstructure is to the target. An illustrative example of the general microstructure reconstruction process is shown in Fig. 11.8. Traditional gradient-based optimization algorithms are unable to seek the global optimal solution due to the high nonlinearity and complexity of the resulting problem. Stochastic optimization methods such as simulated annealing [48, 50] and genetic algorithms [51] have been introduced to solve the resulting optimization problem. Here the simulated annealing algorithm is employed to reconstruct the microstructure of the two-phase material. The general formulation is reviewed as follows: (1) Generating an initial binary microstructure. Based on the correlation functions, an initial microstructure with a given volume fraction of black pixels (secondary phase) can be randomly generated with uniform distribution. The black pixels will be randomly scattered within the image matrix while preserving the given volume fraction. (2) Generating new binary microstructures. A sequence of trial realizations of microstructures is generated by randomly moving the black pixels within the image matrix.

Fig. 11.8 Demonstration of the microstructure reconstruction process. Adapted with permission from [52]. Copyright (2013) Elsevier BV

294

H. Xu et al.

(3) Accepting or rejecting the new generated microstructures. A realization of microstructure will be accepted with the probability: p(E) =

1, E ≤ 0 E exp − kT , E > 0

(11.7)

where E = E − E is the energy difference between the new and old realizations of microstructure, and T is a fictitious temperature in simulated annealing algorithm known as the cooling schedule. (4) Iterative process termination. The iterative optimization process terminates once the temperature T is equal to zero or the energy E is lower than a predetermined value, say 1 × 10−5 . Otherwise, go to Step 2. The optimizationbased stochastic reconstruction process is computationally expensive when it is applied to reconstruct high-resolution 3D microstructures. When other efficient MCR approaches (e.g., physical descriptor-based approach, random field-based approach, machine learning-based approach, etc. [53]) is employed, characterization of the reconstructed microstructures using multiple correlation functions is often needed for the purpose of validation. 11.2.2.2

2D Viscoelastic Reconstruction

In our realization of a data-driven framework (Fig. 11.8) [8], the reconstruction is based on correlation functions, specifically two-point radial correlation and twopoint cluster radial correlation in two dimensions. After binarizing an image of the microstructure, the result is used to generate the correlation functions. These functions then served as a target for an optimization problem, where an image was sought that produced correlation functions that were the most similar to the target. Local optima were found by generating uniformly random binary images and subjecting them to a simulated annealing algorithm [52]. The annealed reconstructions were then used as inputs to an FE simulation. To simulate composite response, the binary images are directly translated into a two-dimensional plane-strain simulation and examples of the reconstructed microstructures for the chosen system are shown in Fig. 11.10c, where the particles are the black pixels. Note that subsequent work [41] has extended this approach to three-dimensional models. In order to include the effect of an interphase of altered properties, based on the strong interaction between carbon black and the rubber matrix, it was assumed that the local interphase properties around each particle could be represented by a simple, constant shift in relaxation time (see Fig. 11.9). This simple assumption can account for the reduced mobility of the polymer in the vicinity of the particles but at the same time reduces the number of parameters needed to optimize against the real composite viscoelastic spectrum to two: the width of the interphase domain and magnitude of the shift factor. Figure 11.10 shows the result of the composite predictions as the simulated interphase thickness was varied while the viscoelastic shift was maintained at one decade

11 Data-Driven Multiscale Science for Tire Compounding …

295

Fig. 11.9 Relation of material properties between interphase and bulk matrix by a simple shift in frequency/time space representing increase of relaxation times in the interphase domain relative to the matrix polymer. Adapted with permission from [8]. Copyright (2012) Elsevier BV

and filler fraction was held at 20%. The filled rubber literature reports a range of estimates for the interphase length, from 2 to 30 nm [2, 9, 54]. The tan δ shift at larger thicknesses (representing 50 and 75 nm interphase) is quite extreme compared to the experimental data, indicating that a single-layer (25 nm) thickness of interphase is the most appropriate. The role of the assumed shift factor for the interphase properties relative to the matrix (Ds) was also examined, as is illustrated in Fig. 11.11. Here, relaxation shifts from 0.5 to 2.0 decades are shown with the thickness held at one layer (25 nm). These shifts are in the range of possibility established experimentally for thermoplastics [55–57] and rubbers [58]. Based on these simulations, interphase polymer with a shift of 1.5 decades slower than that of the matrix material is the most appropriate to fit the experimental data. Overall, these results are reasonable, and similar results are also obtained with different approaches, such as the inverse modeling method [59].

11.2.2.3

Microstructure Characterization and Reconstruction Based on Physical Descriptors

A physical descriptor-based characterization and reconstruction approach [41, 60] is also proposed to enable statistical mapping of processing parameters to the physically meaningful statistical microstructure descriptors. Particle fillers of the nanocomposites are described using three categories of microstructure features: composition, dispersion and geometry. These three categories provide a complete representation of the microstructure.

296

H. Xu et al.

Fig. 11.10 a, b Comparison of predicted tan δ curves with experimental data: here the interphase properties are fixed while the interphase thickness is varied. c Visualization of the definition and effect of thickness for this simulation. Thickness t is in units of geometry mesh pixels, one pixel corresponds to approximately 25 nm. Adapted with permission from [8]. Copyright (2012) Elsevier BV

At the lowest fidelity level, composition indicates the percentage of each material constituent (e.g., volume fraction of nanoparticles). Composition is the lowest order of microstructure information as it only captures the homogenized response of an entire material system. One level down, dispersion represents the spatial distribution patterns of each phase. Local feature-induced material properties are reflected by the dispersion status of different phases in the material. For example, the nearest distance between carbon nanoparticles in polymer composites determines both the damping property and electrical conductivity. At the lowest level, geometry provides a more detailed description of the shape information of each phase (e.g., fillers in polymer composites). Geometry descriptors also have a strong impact on certain

11 Data-Driven Multiscale Science for Tire Compounding …

297

Fig. 11.11 Comparison of predicted tan δ curves against experimental data: here the interphase thickness is fixed while the interphase properties, decades of shift (Ds), varied. Increasing Ds indicates increasingly longer relaxation times for the interphase. Reproduced with permission from [8]. Copyright (2012) Elsevier BV

material properties [61]. For example, the pore size of porous material determines the yield point and critical load in microbuckling. It should be noted that due to the heterogeneity, descriptors used at each level are statistical, including mean and higher order moments such as variance, skewness etc. The microstructure characterization process is illustrated by the flowchart in Fig. 11.12. The following information are obtained from image processing for characterization: (1) A binary image that identifies different phases (black-polymer matrix, whitefillers);

Fig. 11.12 2D microstructure characterization flowchart. Adapted with permission from [60]. Copyright (2014), Elsevier BV

298

H. Xu et al.

(2) A matrix-shielded image that retains the grayscale information of the filler phase. The matrix phase is marked by “0”. This image is used to identify the coordinates of the particle centers; (3) An isolated particle image that only highlights the filler particles isolated from the particle clusters. This image is used for characterizing particle sizes and geometries. The composition descriptor, VF of the nanoparticle filler, is known beforehand from the material processing information. Dispersion descriptors such as neighbor distances or Morisita’s index [62] can be evaluated from the coordinate list of filler’ centers. Here we choose the cumulative distribution function (CDF) of the nearest distance (nd ) among filler’ centers. Based on the binary image and the isolated particle image, two geometry descriptors are evaluated: each particle’s area Ae and the aspect ratio ρ. The geometry of filler is approximated with ellipse of major radius R and minor radius r. Aspect ratio ρ is defined as: ρ=

R2D r

(11.8)

Particle area Ae (mean Ae ) can be related to the equivalent radius of the particle rc , and the total number of particles N : rc_2D =

R2D × r =

Ae =

L 2 × VF N2D

Ae π

(11.9)

(11.10)

where L is the side length of the microstructure image. Symbols with a bar overhead are deterministic variables; symbols without an overhead bar are random variables, which are described by distribution functions instead of a single value. Orientation (θx , θ y , θz ) of the filler is assumed to be uniformly distributed with respect to the 3D Cartesian coordinate system. Statistics of all the geometry descriptors are represented by their probability distribution functions (PDF). Figure 11.13 shows the process of 3D descriptor-based multi-phase microstructure reconstruction to match the pre-specified descriptors. There are four major steps: (1) Pre-specification of target composition, dispersion, and geometry descriptors; (2) Dispersion reconstruction: the location of each particle’s center is determined by matching dispersion descriptors using the Simulated Annealing (SA) algorithm. This strategy is similar to the pixel-moving optimization approach that is used in the correlation function-based reconstruction. Starting from a set of randomly dispersed particle centers, the algorithm moves particle centers’ locations randomly. After each random move, the dispersion descriptors (CDF of nd ) is re-evaluated and compared with the target values. Both the “good” moves that lead to a better matching in target dispersion descriptors, and the

11 Data-Driven Multiscale Science for Tire Compounding …

299

Fig. 11.13 Flowchart of multi-phase descriptor-based reconstruction. Adapted with permission from [60]. Copyright (2014) Elsevier BV

“bad” moves that lead to a worse matching, could be accepted, with probabilities determined by the Simulated Annealing (SA) schedule. This step generates an image where only the locations of filler’ centers are indicated, referred to as “center distribution map”. (3) Geometry reconstruction: at the locations of particle centers, the algorithm reconstructs each particle based on the geometry descriptors. Values of each particle’s geometrical descriptors are generated by sampling the statistical distribution functions obtained in characterization. The reconstructed geometry is placed onto a randomly selected particle center in the center distribution map. (4) Composition adjustment: this is the final step of reconstruction when the digital image is fine tuned to match the composition descriptors (volume fraction of the filler phase). The volume fraction of the reconstructed image is adjusted by adding/subtracting pixels on phase boundaries. The quality of the 3D reconstruction (Fig. 11.14) is assessed quantitatively by comparing the correlation functions of the 2D cross-sections from the 3D reconstruction with the original 2D image. The target 2D image and several 2D cut samples from the 3D reconstruction are shown in Fig. 11.7b. Figure 11.7a also compares the mean 2-point correlation functions of the 2D cut samples with the 2-point correlation function of 2D target image. Figure 11.7b compares the surface correlation functions.

300

H. Xu et al.

Fig. 11.14 Comparison of the correlation function of the target 2D microstructure and the mean correlation function of the 2D cuts from 3D reconstruction. a Comparison of 2-point correlation functions; b Comparison of surface correlation functions. Adapted with permission from [60]. Copyright (2014), Elsevier BV

11.2.3 Nanocomposite Properties and Statistical Study of the Representative Volume Element In real applications, it is often computationally expensive to use a single, strictly qualified RVE size with high precision. Especially when dealing with three-dimensional FE simulations, the number of elements as well as the computation time increases cubically as the length of a side increases [58]. Statistical methods such as taking the average properties of multiple realizations make it possible to achieve higher precision at a smaller RVE size [these RVEs are sometimes referred to as statistical volume elements (SVEs)] [63–65]. Therefore, it is especially appealing to find optimal conditions avoiding one large RVE and instead using a smaller RVE with multiple realizations that reduces the computational cost but still satisfies the desired precision. Here we introduce a microstructure-based modeling framework [8] for viscoelastic polymer nanocomposites applied to 3D microstructures characterized and reconstructed by a descriptor-based method. The determination of the smallest RVE size and the minimum number of realizations for a given volume size is demonstrated on a three-phase RVE containing 10% particles by volume. The influences of volume fraction (VF), composition (interphase layer) and dispersion of the particles on the RVE study results are also discussed in this section.

11.2.3.1

Comparison of Two Mesh Strategies: Voxel Mesh Versus Conformal Mesh

The selection of meshing strategy has a strong impact on material property predictions. In simulating composites, a trade-off often must be made between ease of creation of the mesh, accuracy of the structural representation, and computational

11 Data-Driven Multiscale Science for Tire Compounding …

301

efficiency of the models. Here we consider two mesh strategies, voxel mesh and conformal mesh, to understand their impacts on the prediction of material properties. The advantages of a voxelated mesh is that it is very easy to generate and apply to microstructures, while the drawback is that to obtain a good quality representation of a complex microstructure, very small voxels may be required which can result in large computational cost. The potential advantages of a conformal mesh is the ability to track complex microstructures more closely with the cost of more difficult meshing strategies and complications of appropriate mesh gradients which again may lead to larger computational costs. To explore these two options, a very simple model structure is established as a comparative study with only two cubic inclusions, surrounded by interphase and matrix material. For the voxel mesh, the simulated properties using different mesh sizes are compared in Fig. 11.15. It is found that the impact of mesh size on the simulation result is negligible, so we can use coarser mesh to reduce the computational costs without reducing the prediction accuracy. On the other hand, a large discrepancy can be observed in the low frequency domain when the conformal mesh is used in simulations (Fig. 11.16). We also observe many distorted elements in the conformal mesh

Fig. 11.15 Voxel mesh: simulation results using voxel meshes of different mesh sizes but the same VF. Adapted with permission from [58]. Copyright (2018) Elsevier BV

Fig. 11.16 Conformal mesh: simulation results with different mesh sizes but the same VF. Adapted with permission from [58]. Copyright (2018) Elsevier BV

302

H. Xu et al.

or even mesh errors when applying the conformal mesh on more complex structures (results not shown here). Therefore, voxelated mesh is recommended in this study.

11.2.3.2

Relationship Between RVE Volume Size and the Variations in Simulated Material Properties

If unlimited computational resources were available, we can simply predict material properties with a large RVE model of a high resolution. However, in realistic cases, this strategy of unlimited computational resources and time is rarely the best solution. In order to achieve a balance between prediction accuracy and computational efficiency, microstructure models of different sizes are tested to understand the influence of RVE/SVE volume size on the predicted material properties [58]. At the outset, a sufficiently large microstructure RVE model is established to provide a reference property and computational cost. For each smaller volume size cut from this large benchmark model, a convergence study is conducted to guarantee a sufficient number of samples at that size. A trade-off between a single very large RVE and multiple smaller representative SVEs will be achieved with respect to computational cost and simulation accuracy. In order to quantitatively measure the mean and variance from the simulations, we selected the frequency point where tan δ reaches its peak and compared the mean and standard deviation of the peak value for each of the volume sizes in Fig. 11.17. The standard deviation between the simulations decreases as the RVE volume increases. However, even though we pre-selected a seemly large number of realizations in the FE simulations, the effective tan δ peak still shows a bias in the mean for very small volumes. This bias becomes negligible after the volume size reaches 103 voxels. Also considering the computational costs presented in Fig. 11.17, we suggest 103 voxels as the optimal RVE size as a balance of computation time and the processing time corresponding to the number of realizations. One simulation with a volume of 603 voxels costs 2680 min, while 76 simulations with a volume of 103 voxels only

Fig. 11.17 Statistical study of the relation between RVE volume size and the predicted properties. Adapted with permission from [58]. Copyright (2018), Elsevier BV

11 Data-Driven Multiscale Science for Tire Compounding …

303

cost 56 min while introducing less than 2% error. The use of sufficient realizations of V = 103 voxels instead of the full RVE represents a reduction in computational time of two orders of magnitude while still achieving the desired precision [58]. The ability to reduce computation time by several orders of magnitude will allow us to rapidly fill design of experiments (DOEs) for data mining and to consider more complex microstructures where large RVEs would be prohibitive in future studies.

11.2.3.3

Computational Analysis of Nanocomposites with FE Modeling

Finally, we establish realistic FE models based on the stochastically reconstructed 3D digital microstructures. Influences on the filled elastomers’ properties mainly come from three aspects: the filler, the polymer matrix, and the interphase. The fillers are considered as elastic with Young’s modulus of 73 (GPa), Poisson’s ratio 0.19, and density 2.2 g/cm3 . The matrix is assigned linear viscoelastic material properties whose frequency response is given by the property curves in Fig. 11.8 obtained from physical experiments. Here, as earlier (Fig. 11.9), the property of the interphase is assumed to be related to the property of the matrix by shifting and broadening in the frequency domain [11, 66]. The assumption for the shifting and broadening behaviors are based on our observation of the comparison between the master curves of the filled and unfilled systems in experiments [8]. In Fig. 11.18, the storage and loss modulus of the matrix (solid curves) are obtained from experiments and the interphase modulus (dashed curves) are then obtained by shifting those of the matrix to a lower frequency and applying a broadening factor. We use ABAQUS to solve the RVEs given the material properties for each phase stated above. The dynamic moduli are calculated in the frequency-domain

Fig. 11.18 Three-phase FE model and master curves including (left) storage modulus, (right) loss modulus. In these plots, the experimental data of the real matrix material is labeled “Matrix” and the “Interphase” curve is generated by artificially shifting the matrix curve to lower frequency and applying a broadening factor. Reproduced with permission from [58]. Copyright (2018) Elsevier BV

304

H. Xu et al.

Fig. 11.19 Finite element models (60 × 60 × 60) with representative microstructures and interphase gradients match experimental results at high filler concentrations, even when tan δ appears to shift to higher frequencies, or lower temperatures [8]. We observe that the peak position, at this high filler loading, is nearly the same with or without interphase, therefore controlled by the presence of the stiff phase. Adapted with permission from [23]. Copyright (2016) Elsevier BV

viscoelastic module for small strain oscillations. In Fig. 11.19, we demonstrate the necessity of considering the interphase. Two RVE models, one with interphase (interphase VF = 49.6%) and one without interphase, are established for nanocomposites with a filler VF of 28.5%. The predicted material properties are validated with the experimental test results by DMA. Significant prediction error in the low frequency domain is observed in the model without interphase, while the model with interphase successfully captures the tan δ values in the full frequency domain. Wood [23] used a two-layer strategy to generate the interphase gradient required to observe positive tan δ peak temperature shift [56]. Following the reconstruction strategy of Deng et al. and Xu et al. [8, 67], a reconstruction using SEM images of a CB-SBR was produced and transformed into a three-dimensional FE mesh. In Fig. 11.19, the effect of the optimal interphase gradient is contrasted with the same mesh without any interphase effect. The interphase mainly increases the loss of the material at lower frequencies, while the tan δ peak position and magnitude are dominated by the pure particle effect.

11.2.4 Summary We have presented and demonstrated a framework of capabilities for the computational assessment of viscoelastic nanoparticle composites. We have done so to establish the important structural features needed to both replicate and extend our understanding of complex rubber compounds. From the use of dynamic mechanical analyses (DMA) and scanning electron microscopy (SEM), we provide structure– property relationships down to the nanometer scale. This combination of macro-scale

11 Data-Driven Multiscale Science for Tire Compounding …

305

experimentation, and nanoscale characterization, is necessary to link mesoscale-level structure to observed viscoelastic behavior. This endeavor has also shown the importance of three structural entities to compound viscoelastic behavior: filler morphology, the far-field rubber matrix, and the filler-rubber interphase. Although it is considered a purely elastic material, and mechanically the simplest, the filler morphology itself is one of the most complex features of a rubber compound. Standard dry-mixing of a compound formulation are known widely to affect the overall filler morphology [68] and the subsequent mechanical properties. We have delineated a number of micrograph image analysis and reconstruction methods for filler morphology which are useful in the building of realistic compound models. The second structural entity which is relevant for this style of mesoscale modeling and simulation is the far-field rubber matrix. It is perhaps the simplest morphological entity at the mesoscale, compared to the filler and interphase morphologies. In this light, unfilled rubber samples are constructed and analyzed solely by DMA methods. The construction of master curves, via generalized Maxwell models (i.e., Prony series constructions) are the main item contributed to the overall mesoscale continuum models. Of the structural elements, the filler-rubber interphase, is the most difficult to ascertain. Its viscoelastic properties and geometrical extent in this work are determined by a set of methods of increasing complexity. The simplest methods allow for a shifting of the far-field rubber master curves to account for the general fillerrubber interaction effects, as well as an iterative estimation of the interphase size. This mechanical model has been demonstrated in the literature [56, 69–71] as a gradient in glass transition temperature, T g , as a function of distance from the filler surface. This simplest interphase model, that of a single mechanical behavior, can only estimate the effective viscoelastic and geometric behavior. More complex interphase models, in which these mechanical gradients are captured by incorporating both master curve shifting and spectral broadening, have been shown to be quantitative. From a design perspective, the utilization of shifting and spectral broadening bring into play the ability to perform ‘what-if’ scenarios on this elusive structural element. The ability to perform these ‘what-if’ scenarios with good accuracy is also dependent upon the size extent of the mesoscale models in play. The size scale, also known as the representative volume element (RVE) size, is somewhat dependent on the correlation lengths of the underlying filler morphologies. The number of finite-elements in the continuum model also define the accuracy of the simulation. There exists a tradeoff between number of elements and computational convergence. We have also shown the requirements for obtaining very good accuracy from the number of elements perspective, using sub-sized cells which we call statistical volume elements (SVEs). The reader may find the use of SVEs to be an attractive computational alternative to full-size, high-resolution RVEs. Combining filler morphological reconstruction with interphase analysis and cell size allows a more complete design tool set for unraveling the impact of design intricacies of rubber compounds. This process allows one to vary the design scenario at hand. One can use these capabilities to obtain quantitative correspondence with

306

H. Xu et al.

known compound viscoelastic behavior. However, one can also use the same analyses in a discovery context, by varying the developed design space in such a way which allows a more extensive evaluation compared to experiment. Finally, there also exists the ability to examine features which are outside the realm of current experimental facility, which enable one to potentially search for limiting viscoelastic behaviors and/or demonstrating the value of a previously unconsidered design space.

11.3 Future Directions In this final section, we illustrate the trends which are escalating in data-driven multiscale sciences, especially as they concern tire compounding. So far, we have emphasized mesoscale-level models which are physics-based. We see two additional major trends in compound design: (1) the increasing research into material and cheminformatics [72]; and, hand-in-hand (2) the explosion in the use of machine learning tools for chemical and material problems. These areas are complementary to the more traditional physics-based tools, and are part of an overall adaptive materials design ecosystem [73] for compounding.

11.3.1 Material Informatics and Cheminformatics Data-centric informatics, which we consider to be a form of feature engineering, is being leveraged in compound materials science by the advent or accumulation of large-scale databases from external [74] and internal R&D sources, respectively. There are many elements which can be considered for this style of data environment, shown in Fig. 11.20. The underlying principle of these environments is the centrality of design, leveraging the knowledge sets from physics-based simulations, data science, material characterization and chemistry, and theory. These wide-ranging environments require a level of data integration which historically has not been a priority. The implementation of ‘data lakes’ will be a key unifying element of such systems. On another front, we also see the use of chemically relevant feature engineering, also known as cheminformatics, being leveraged for data-centric compound design solutions [74]. In Fig. 11.21, the incorporation of rubber structure and other structural elements are used in compound design. One of the major reasons for defining chemical features is the ability to enable large-scale data compression from typical corporate formulation databases. In machine learning applications without such feature engineering, it is not unusual to have input vectors in the many hundreds to describe compound formulations. Most industrially relevant compounds are comprised of

11 Data-Driven Multiscale Science for Tire Compounding …

307

Fig. 11.20 Elements of a materials informatics environment for compound design. Such environments merge knowledge from many technical disciplines, tying the elements into a design framework at the core

Fig. 11.21 General schemes for standard laboratory-based compound design versus cheminformatics enabled design. Note that the relevant chemical features (cheminformatics) are described and input into the machine learning process. This process requires existing data and is complementary to standard practices. Adapted from [72]. Copyright (2019) The Tire Society

308

H. Xu et al.

approximately 10–15 ingredients, which means these input vectors, for each formulation, are very sparse. The resultant cheminformatics machine learning models also have the advantage of being potentially more generalizable than the sparse, large-scale formulation vector approach.

11.3.2 Machine Learning Image classification and reconstruction are a major application of convolutional deep learning networks. One of the many adaptations possible is the use of transfer learning for compound morphological reconstruction. In Fig. 11.22, the workflow for this approach is shown. The main advantage of the transfer learning approach is that of data economy. In typical trainings of convolutional neural networks, millions of images are needed. Most industrial concerns, including tire manufacturers, do not have millions of images in internal image databases. The knowledge accumulated in the deep learning network model is leveraged by training the network with new compound morphological structures from much smaller image databases. These models can then be used

Fig. 11.22 Rubber compound microstructural reconstruction workflow. This method utilizes large image databases for the original VGG-19 deep learning networks. This large-scale deep learning network was transferred to the new application, in this case, rubber compound reconstruction. Reproduced with permission from [75]. Copyright (2018) Springer Nature Ltd

11 Data-Driven Multiscale Science for Tire Compounding …

309

for image reconstruction and model building for simulations or for other machine learning-based structure–property relationships [75].

11.3.3 Summary Moving outside of the strictly physics-based approach of this chapter, we have illustrated emerging trends in tire compound design which are complementary to our data-driven multiscale approach. Many materials design areas, outside of tire compounding, have leveraged extensive external and internal corporate databases, computational materials science at many levels, analytical characterization techniques and machine learning methodologies. We view these methods and data sources as complementary and of significant utility in general tire compound design. The next 5–10 years should see the further integration of these environments into mainstream tire compound design, with each company utilizing these resources depending on their cultures and resources. The combination and integration into a cohesive compound design environment will greatly accelerate the development of new, optimal and robust compounds for tire technology. We look forward to seeing the materials and tire design worlds seamlessly integrated into fully functional virtual design ecosystems.

References 1. European Commission, Proposal on the labelling of tyres with respect to fuel efficiency and other essential parameters, Document 52018PC0296, 17 May 2018. https://eur-lex.europa.eu/ legal-content/EN/TXT/?uri=CELEX:52018PC0296. Accessed on 12/09/2019; Commission takes action to reinforce EU’s global leadership in clean vehicles, Press Release, 8 Nov 2017. https://europa.eu/rapid/press-release_IP-17-4242_en.htm. Accessed on 12/09/2019 2. L. Leblanc, Rubber–filler interactions and rheological properties in filled compounds. Prog. Polym. Sci. 27, 627–687 (2002) 3. J. Fröhlich, W. Niedermeier, H.D. Luginsland, Compos. Part A Appl. Sci. Manuf. 36, 449–460 (2005) 4. I. Morozov, B. Lauke, G. Heinrich, Comput. Mater. Sci. 47, 817–825 (2010) 5. A. Mostafa, A. Abouel-Kasem, M.R. Bayoumi, M.G. El-Sebaie, J. Test. Eval. 38, 347–359 (2010) 6. Reinforcing Fillers in the Rubber Industry, Fact Sheet 2012. European Tyre and Rubber Manufacturers’ Association 7. A. Medalia, Effective degree of immobilization or rubber occluded within carbon black aggregates. Rubber Chem. Technol. 45, 1171–1194 (1972) 8. H. Deng et al., Utilizing real and statistically reconstructed microstructures for the viscoelastic modeling of polymer nanocomposites. Compos. Sci. Technol. 72, 1725–1732 (2012) 9. M. Qu et al., Nanoscale visualization and multiscale mechanical implications of bound rubber interphases in rubber-carbon black nanocomposites. Soft Matter 7, 1066–1077 (2011) 10. K.H. Nordsiek, The “integral rubber” concept: an approach to an ideal tire tread rubber. Kautschuk Gummi Kunstoffe 38, 178–185 (1985)

310

H. Xu et al.

11. H.F. Brinson, L.C. Brinson, Polymer Engineering Science and Viscoelasticity (Springer, Berlin, 2008). https://doi.org/10.1007/978-0-387-73861-1 12. V. Arrighi, I.J. McEwen, H. Qian, M.B. Serrano Prieto, The glass transition and interfacial layer in styrene-butadiene rubber containing silica nanofiller. Polymer (Guildf) 44, 6259–6266 (2003) 13. E. Donth et al., Fine structure of the main transition in amorphous polymers: entanglement spacing and characteristic length of the glass transition. Discussion of examples. Macromolecules 29, 6589–6600 (1996) 14. J. Fröhlich, R. Thomann, R. Mülhaupt, Toughened epoxy hybrid nanocomposites containing both an organophilic layered silicate filler and a compatibilized liquid rubber. Macromolecules 36, 7205–7211 (2003) 15. M. Jacob, B. Francis, S. Thomas, K.T. Varughese, Dynamical mechanical analysis of sisal/oil palm hybrid fiber-reinforced natural rubber composites. Polym. Compos. 27, 671–680 (2006) 16. M.A. López-Manchado, J. Biagiotti, L. Valentini, J.M. Kenny, Dynamic mechanical and Raman spectroscopy studies on interaction between single-walled carbon nanotubes and natural rubber. J. Appl. Polym. Sci. 92, 3394–3400 (2004) 17. M.A.L. Manchado, L. Valentini, J. Biagiotti, J.M. Kenny, Thermal and mechanical properties of single-walled carbon nanotubes–polypropylene composites prepared by melt processing. Carbon 43, 1499–1505 (2005) 18. J.K. Mishra, I. Kim, C.-S. Ha, New millable polyurethane/organoclay nanocomposite: preparation, characterization and properties. Macromol. Rapid Commun. 24, 671–675 (2003) 19. P. Pötschke, M. Abdel-Goad, I. Alig, S. Dudkin, D. Lellinger, Rheological and dielectrical characterization of melt mixed polycarbonate-multiwalled carbon nanotube composites. Polymer (Guildf) 45, 8863–8870 (2004) 20. G. Tsagaropoulos, A. Eisenburg, Direct observation of two glass transitions in silica-filled polymers. Implications to the morphology of random ionomers. Macromolecules 28, 396–398 (1995) 21. Y. Sun, Z. Zhang, K.-S. Moon, C.P. Wong, Glass transition and relaxation behavior of epoxy nanocomposites. J. Polym. Sci. Part B Polym. Phys. 42, 3849–3858 (2004) 22. T. Ramanathan et al., Functionalized graphene sheets for polymer nanocomposites. Nat. Nanotechnol. 3, 327 (2008) 23. C.D. Wood, A. Ajdari, C.W. Burkhart, K.W. Putz, L.C. Brinson, Understanding competing mechanisms for glass transition changes in filled elastomers. Compos. Sci. Technol. 127, 88–94 (2016) 24. C.P. Tsui, C.Y. Tang, T.C. Lee, Finite element analysis of polymer composites filled by interphase coated particles. J. Mater. Process. Technol. 117, 105–110 (2001) 25. F.T. Fisher, L.C. Brinson, Viscoelastic interphases in polymer–matrix composites: theoretical models and finite-element analysis. Compos. Sci. Technol. 61, 731–748 (2001) 26. G.M. Odegard, T.S. Gates, K.E. Wise, C. Park, E.J. Siochi, Constitutive modeling of nanotube– reinforced polymer composites. Compos. Sci. Technol. 63, 1671–1687 (2003) 27. G.D. Smith, D. Bedrov, L. Li, O. Byutner, A molecular dynamics simulation study of the viscoelastic properties of polymer nanocomposites. J. Chem. Phys. 117, 9478–9489 (2002) 28. J.S. Smith, D. Bedrov, G.D. Smith, A molecular dynamics simulation study of nanoparticle interactions in a model polymer-nanoparticle composite. Compos. Sci. Technol. 63, 1599–1605 (2003) 29. F.W. Starr, T.B. Schrøder, S.C. Glotzer, Molecular dynamics simulation of a polymer melt with a nanoscopic particle. Macromolecules 35, 4481–4492 (2002) 30. D. Brown, V. Marcadon, P. Mélé, N.D. Albérola, Effect of filler particle size on the properties of model nanocomposites. Macromolecules 41, 1499–1511 (2008) 31. N. Sheng et al., Multiscale micromechanical modeling of polymer/clay nanocomposites and the effective clay particle. Polymer (Guildf) 45, 487–506 (2004) 32. G.D. Seidel, D.C. Lagoudas, Micromechanical analysis of the effective elastic properties of carbon nanotube reinforced composites. Mech. Mater. 38, 884–907 (2006)

11 Data-Driven Multiscale Science for Tire Compounding …

311

33. X.-L. Gao, K. Li, A shear-lag model for carbon nanotube-reinforced polymer composites. Int. J. Solids Struct. 42, 1649–1667 (2005) 34. N.D. Alberola, P. Mele, Interface and mechanical coupling effects in model particulate composites. Polym. Eng. Sci. 37, 1712–1721 (1997) 35. Z. Hashin, P.J.M. Monteiro, An inverse method to determine the elastic properties of the interphase between the aggregate and the cement paste. Cem. Concr. Res. 32, 1291–1300 (2002) 36. R.A. Dickie, Heterogeneous polymer–polymer composites. I. Theory of viscoelastic properties and equivalent mechanical models. J. Appl. Polym. Sci. 17, 45–63 (1973) 37. T. Mori, K. Tanaka, Average stress in matrix and average elastic energy of materials with misfitting inclusions. Acta Metall. 21, 571–574 (1973) 38. R. Qiao, H. Deng, K.W. Putz, L.C. Brinson, Effect of particle agglomeration and interphase on the glass transition temperature of polymer nanocomposites. J. Polym. Sci. Part B Polym. Phys. 49, 740–748 (2011) 39. J. Cho, I.M. Daniel, Reinforcement of carbon/epoxy composites with multi-wall carbon nanotubes and dispersion enhancing block copolymers. Scr. Mater. 58, 533–536 (2008) 40. R.K. Duncan et al., Viscoelastic behavior of nanotube-filled polycarbonate: effect of aspect ratio and interface chemistry. Int. J. Smart Nano Mater. 1, 53–68 (2010) 41. H. Xu, Y. Li, C. Brinson, W. Chen, A descriptor-based design methodology for developing heterogeneous microstructural materials system. J. Mech. Des. 136, 051007 (2014) 42. Y. Wang et al., Identifying interphase properties in polymer nanocomposites using adaptive optimization. Compos. Sci. Technol. 162, 146–155 (2018) 43. Y. Jiao, F.H. Stillinger, S. Torquato, Modeling heterogeneous materials via two-point correlation functions: basic principles. Phys. Rev. E 76, 31110 (2007) 44. S. Torquato, Random Heterogeneous Materials: Microstructure and Macroscopic Properties (Springer, New York, 2013) 45. C.L.Y. Yeong, S. Torquato, Reconstructing random media. II. Three-dimensional media from two-dimensional cuts. Phys. Rev. E 58, 224–233 (1998) 46. I.A. Morozov, B. Lauke, G. Heinrich, A novel method of quantitative characterization of filled rubber structures by AFM. KGK Kaut. Gummi Kunstst. 64, 24–27 (2011) 47. L. Karásek, M. Sumita, Characterization of dispersion state of filler and polymer-filler interactions in rubber-carbon black composites. J. Mater. Sci. 31, 281–289 (1996) 48. C.L.Y. Yeong, S. Torquato, Reconstructing random media. Phys. Rev. E 57, 495–506 (1998) 49. S. Torquato, Optimal design of heterogeneous materials. Annu. Rev. Mater. Res. 40, 101–129 (2010) 50. H. Xu, R. Liu, A. Choudhary, W. Chen, A machine learning-based design representation method for designing heterogeneous microstructures. J. Mech. Des. 137 (2015) 51. B.C. Collins, K. Matous, D. Rypl, Three-dimensional reconstruction of statistically optimal unit cells of multimodal particulate composites. Int. J. Multiscale Comput. Eng. 8, 489–507 (2010) 52. Y. Liu, M.S. Greene, W. Chen, D.A. Dikin, W.K. Liu, Microstructure reconstruction for stochastic multiscale material design, in Proceedings of the ASME 2011 International Design Engineering Technical Conferences and Computers and Information in Engineering Conference, vol. 5. 37th Design Automation Conference, Parts A and B (ASME, 2011), pp. 497–507. https://doi.org/10.1115/DETC2011-48323 53. R. Bostanabad et al., Computational microstructure characterization and reconstruction: review of the state-of-the-art techniques. Prog. Mater. Sci. 95, 1–41 (2018) 54. P.F. Brune et al., Direct measurement of rubber interphase stiffness. Macromolecules 49, 4909– 4922 (2016) 55. J.A. Forrest, K. Dalnoki-Veress, The glass transition in thin polymer films. Adv. Colloid Interface Sci. 94, 167–195 (2001) 56. C.J. Ellison, J.M. Torkelson, The distribution of glass-transition temperatures in nanoscopically confined glass formers. Nat. Mater. 2, 695–700 (2003)

312

H. Xu et al.

57. Y. Li, M. Kröger, W.K. Liu, Nanoparticle effect on the dynamics of polymer chains and their entanglement network. Phys. Rev. Lett. 109, 118001 (2012) 58. A. Hu et al., Computational analysis of particle reinforced viscoelastic polymer nanocomposites—statistical study of representative volume element. J. Mech. Phys. Solids 114, 55–74 (2018) 59. J. Gao et al., An inverse modeling approach for predicting filled rubber performance. Comput. Methods Appl. Mech. Eng. 357, 112567 (2019) 60. H. Xu, D.A. Dikin, C. Burkhart, W. Chen, Descriptor-based methodology for statistical characterization and 3D reconstruction of microstructural materials. Comput. Mater. Sci. 85, 206–216 (2014) 61. R. Tian et al., A multiresolution continuum simulation of the ductile fracture process. J. Mech. Phys. Solids 58, 1681–1700 (2010) 62. M. Morisita, Iσ-index, a measure of dispersion of individuals. Res. Popul. Ecol. (Kyoto) 4, 1–7 (1962) 63. A.S. Dalaq, D.W. Abueidda, R.K. Abu Al-Rub, I.M. Jasiuk, Finite element prediction of effective elastic properties of interpenetrating phase composites with architectured 3D sheet reinforcements. Int. J. Solids Struct. 83, 169–182 (2016) 64. X. Yin, W. Chen, A. To, C. McVeigh, W.K. Liu, Statistical volume element method for predicting microstructure–constitutive property relations. Comput. Methods Appl. Mech. Eng. 197, 3516–3529 (2008) 65. J. Zhao, O.Y. Kontsevoi, W. Xiong, J. Smith, Simulation-aided constitutive law development— assessment of low triaxiality void nucleation models via extended finite element method. J. Mech. Phys. Solids 102, 30–45 (2017) 66. K.W. Putz, C.A. Mitchell, R. Krishnamoorti, P.F. Green, Elastic modulus of single-walled carbon nanotube/poly(methyl methacrylate) nanocomposites. J. Polym. Sci. Part B Polym. Phys. 42, 2286–2293 (2004) 67. H. Xu et al., Stochastic reassembly strategy for managing information complexity in heterogeneous materials analysis and design. J. Mech. Des. 135 (2013) 68. A. Jean, D. Jeulin, S. Forest, S. Cantournet, F. N’Guyen, A multiscale microstructural model of carbon black distribution in rubber. J. Microscopy 241, 243–260 (2011) 69. P. Rittigstein, R.D. Priestley, L.J. Broadbelt, J.M. Torkelson, Model polymer nanocomposites provide an understanding of confinement effects in real nanocomposites. Nat. Mater. 6, 278–282 (2007) 70. M. Zhang, S. Askar, J.M. Torkelson, L.C. Brinson, Stiffness gradients in glassy polymer model composites: comparisons of quantitative characterization by fluorescence spectroscopy and atomic force microscopy. Macromolecules 50, 5447–5458 (2017) 71. M. Tauban, J.-V. Delannoy, P. Sotta, D.R. Long, Effect of filler morphology and distribution state on the linear and nonlinear mechanical behavior of nanofilled elastomers. Macromolecules 50, 6369–6384 (2017) 72. B. Kelly, B. Crookston, N. Isitman, C. Burkhart, Machine Learning Guided Discovery of New Compounds, Paper 6.2 (Tire Society Conference, Akron, OH, 2019) 73. D. Xue, P.V. Balachandran, J. Hogden, J. Theiler, D. Xue, T. Lookman, Accelerated search form materials with targeted properties by adaptive design. Nat. Commun. 7, 11241 (2016) 74. Materials Genome Initiative, Center for Hierarchical Materials Design (CHiMaD). https://chi mad.northwestern.edu/. Accessed on 12/9/2019 75. X. Li, Y. Zhang, H. Zhao, C. Burkhart, L.C. Brinson, W. Chen, A transfer learning approach for microstructure reconstruction and structure-property predictions. Sci. Rep. 8, 13461 (2018)

Index

A Absorption, 265 Adam and Gibbs theory, 127 Ag nanowire, 275 α relaxation, 85, 86, 89, 92 Anisotropic assembly, 38 Aspect ratio, 298 Associating polymer, 16 Atomic closures, 17

B Bare nanoparticles, 103 Boron nitride, 244 Boundary curvature, 103 Bound layer, 83, 84, 92, 119 Bound polymer, 86–88, 94 Bound polymer layer, 81, 85, 91, 94 Bound rubber layer, 82 Broadband Dielectric Spectroscopy (BDS), 85, 90 Bruggeman model, 244, 245, 247

C Carbon nanotube, 236, 240, 248, 249, 252, 275 Cellulose Nanocrystal (CNC), 185–187, 192, 197 Chain conformation, 3 Cheminformatics, 306 Clausius-Mossotti relationship, 263 “Cloaking” effect, 126 Cluster correlation, 291 CNC-PMMA, 187 Coarse-grained, 180, 181, 197

Coarse-grained polymer, 104 Coarse-graining, 181 Colloidal limit, 24, 27 Columnar, 32 Complex grafted nanoparticles, 61 Composition, 296 Concentrated Polymer Brush (CPB), 191, 192 Concentration tensor, 208–210 Conductance, 274 Conformal mesh, 300 Correction of the dielectric function, 266 Critical chain length, 189, 192

D Data lakes, 306 Dead layer, 90, 94 Debye Waller Factor, 182 Density Functional Theory (DFT), 23, 25– 28, 30, 33–35, 38, 39, 138, 156, 157 Density gradient, 114 Depletion attraction, 27 Descriptors, 289 Diblock copolymers, 34 Differential Scanning Calorimetry (DSC), 90 Diffusion coefficient, 87, 92, 93 Discrete Dipole Approximation (DDA), 260 Dispersed/aggregated, 3 Dispersion, 296 Dissipative Particle Dynamics (DPD), 141, 161, 163, 167 1D scalar models, 287 3D uniform models, 288

© Springer Nature Switzerland AG 2021 V. V. Ginzburg and L. M. Hall (eds.), Theory and Modeling of Polymer Nanocomposites, Springer Series in Materials Science 310, https://doi.org/10.1007/978-3-030-60443-1

313

314 Dynamic mechanical analyses, 286, 304 Dynamic Tg , 123 E Effective Medium Approximation (EMA), 236, 241, 245, 255 Electrical properties, 259, 273 Energy renormalization, 181–185, 197 Entropy-enthalpy compensation effect, 182 Equivalent continuum, 220, 224, 225–227 Eshelby, 206–208, 210, 227 Extinction, 261 Extinction cross section, 265

F Failure, 214, 215, 228 Feature engineering, 306 Field-theoretic simulations, 46 Field theory, 47 Finite-Difference Time-Domain (FDTD), 260, 269 Finite Element Analysis (FEA), 215–219, 228–230, 246, 248–252, 255 Flory-Huggins lattice model, 34 Flory-Huggins χ parameter, 3 Flow battery, 133–135, 141, 168 Free interface, 106 Fuel cell, 133, 134, 139–141, 149, 157, 158, 167, 168 Fundamental Measure Theory (FMT), 25, 27, 39

G Geometry, 296 Glass transition temperature, 118 Glassy, 90 “Glassy” (immobilized) layer, 83 Glassy layer, 83–85, 90, 94 Grafted nanoparticles, 58 Grafting density, 4

H Hairy Nanoparticle (HNP), 27, 38 Homogenization, 208, 210–212, 226, 228 Hybrid particle-field theory, 47, 51

I Ideal dispersion, 103 Imidazole, 140, 158, 159

Index Implementation of FDTD, 271 Interfacial density gradient scale, 125 Interfacial density scale, 109 Interfacial density variance scale, 116 Interfacial dynamics, 82, 86 Interfacial interaction strength, 103 Interfacial layers, 81, 85, 86, 91, 102 Interfacial mobility scale, 106 Interfacial thermal resistance, 251, 252, 254 Interphase, 226, 227, 283, 288 Interphase gradient, 304 Intra-molecular pair correlation function, 9 Inverse Boltzmann method, 181, 183–185 Ionic liquid, 134, 140, 157, 159 Ionic transport, 276 Ion transport, 260 Isotropic, 32

K Kapitza radius, 242 Kapitza resistance, 242, 251, 255 Kirchhoff’s Law, 274

L Laminate, 212–214 Large-scale Atomic/Molecular Massively Parallel Simulator (LAMMPS), 187 Lineal path correlation, 291 Local Density Approximation (LDA), 25 Local interphase properties, 294 Local packing frustration, 115

M Machine learning, 308 Material informatics, 306 Matrix relaxation time, 121 Maxwell-Garnett effective medium model, 262 Maxwell-Garnett (MG) model, 241 Maxwell’s equations, 270 Mean square displacement, 183, 184, 188 Mesoscale DDFT (MDDFT), 161, 163, 169 Mesoscale model, 193, 197 Mesoscopic simulation, 134, 160, 161 Metamodel, 179, 188 MG model, 241, 243, 245 Micromechanical model, 240, 245, 251, 255 Micro-mechanics, 206, 226, 227 Microstructure characterization, 289 Mie theory, 260 Mobile layer, 94

Index Mobility, 84 Mobility gradient, 106 Molecular closures, 17 Molecular dynamics, 134, 138, 142, 150, 168, 181, 186, 188, 197 Monte Carlo field-theoretic simulations, 74 Monte Carlo simulations, 38 Mori-Tanaka, 209, 211, 226, 228

N Nafion, 133, 136–157, 162, 165, 168, 169 Nanoparticle limit, 24 Nanoparticle-Organic Hybrid Materials (NOHM), 27 Nanoplatelets, 24 Nanoplates, 29 Nanorods, 24, 28 Nanospheres, 24, 34 Nearest distance, 298 Nernst-Planck equation, 277 Nuclear Magnetic Resonance (NMR), 82– 84, 83, 90

O Occluded rubber, 283 Optical absorption, 260 Optical properties, 259

P Particle’s area, 298 Percolation, 136, 139, 164–166, 244, 249, 250, 273 Perfectly Matched Layer (PML), 272 Physical descriptor-based characterization and reconstruction, 295 Plasmonic coupling, 260 Plastic solid, 32 2-point correlation function, 289 Poisson and Nernst-Planck equations, 277 Poisson-Boltzman equation, 277 Poisson-Nernst-Planck formalism, 260 Polarization, 266 Polybutadiene (PB), 186, 192, 194, 195 Polycarbonate (PC), 183, 184, 186, 192, 194, 195 Polyelectrolyte Membrane (PEM), 133– 135, 137–141, 147, 161, 167–169 Polymer field theory, 46 Polymer-Grafted Nanoparticle (PGNP), 38 Polymer mobility, 82, 85, 86, 94

315 Polymer-nanoparticle interaction strength, 104 Polymer Reference Interaction Site Model (PRISM) theory, 1 Poly(methyl methacrylate) (PMMA), 186, 192, 194–196 Polystyrene (PS), 185, 186, 192, 194 Potential of Mean Force (PMF), 24, 194–197 Proton transport, 133, 135–137, 141, 143, 145, 149, 157–159, 168 pyPRISM, 1 R Reconstructed microstructure, 288 Reconstruction, 289 Relaxation, 85 Relaxation profile, 113 Relaxation time, 84, 86, 87, 89, 91–93, 106 Representative Volume Element (RVE), 217, 220–225, 285, 305 Resistor network models, 260, 273 Resonance Enhanced Dynamic Light Scattering (REDLS), 89 RVE volume size, 302 S Scanning Electron Microscopy (SEM), 289, 304 Scattering, 260 Scattering and absorption efficiencies, 266 Scattering cross sections, 261, 265 Second order Legandre parameter, 184 Segmental dynamics, 81, 83, 87, 90, 91, 94 Segmental mobility, 90 Segmental relaxation time, 106 Self-Consistent Field/Density Functional Theory (SCF-DFT), 23, 27, 33, 36, 38, 39 Self-Consistent Field Theory (SCFT), 25, 30 Self-consistent PRISM theory—molecular simulation, 11 Self-intermediate scattering function, 108 Semi-Dilute Polymer Brush (SDPB), 191, 192 Sheets, 38 Simulated annealing, 293, 298 Single-particle density, 25 Slotboom transformation, 278 Small Angle Neutron Scattering (SANS), 83, 94 Small Angle X-Ray Scattering (SAXS), 90 SPDB, 192

316 Stochastic optimization methods, 293 Storage and loss modulus, 303 Strings, 38 Strong-segregation theory, 38 Structure-property, 203, 230 Styrene-butadiene rubber, 286 Successive Over-Relaxation (SOR) algorithm, 277 Sulfonated poly(ether-ether ketone) (SPEEK), 137, 147, 160–167, 169 Surface correlation, 291 Surface plasmon resonance, 260 Surface plasmons, 260 T Tan δ, 283 Temperature dependence, 288 Tg , 85, 87, 88, 91, 94 Theoretically-informed Langevin dynamics, 69 Thermal conductivity, 235, 236–252, 254, 255 Thermal Interface Materials (TIM), 236 Thermodynamic Tg , 123 Thin polymer film, 103 Three-dimensional Finite Element (FE) model, 288

Index Time of Flight (TOF), 84 Total Field/Scattered Field (TF/SF) source, 272 Transfer learning, 308 Transmission Electron Microscopy (TEM), 289 Two-dimensional plane-strain simulation, 294 Two-layer strategy, 304 Two-point correlation, 290

V Viscoelastic spectrum, 288 Volume fraction, 296 Voxel mesh, 300

W Weighted Density Approximation (WDA), 25, 35, 39 Wertheim perturbation scheme, 26 Wetting, 3

Y Yee cell, 269